Based on an established course and covering the fundamentals, central areas and contemporary topics of this diverse fiel

*879*
*153*
*20MB*

*English*
*Pages 460
[461]*
*Year 2016*

- Author / Uploaded
- Marvin L. Cohen
- Steven G. Louie

*Table of contents : ContentsPrefacePart I Basic concepts: electrons and phonons 1 Concept of a solid: qualitative introduction and overview 1.1 Classification of solids 1.2 A first model of a solid: interacting atoms 1.3 A second model: elementary excitations 1.4 Elementary excitations associated with solids and liquids 1.5 External probes 1.6 Dispersion curves 1.7 Graphical representation of elementary excitations and probe particles 1.8 Interactions among particles 2 Electrons in crystals 2.1 General Hamiltonian 2.2 The Born–Oppenheimer adiabatic approximation 2.3 The mean-field approximation 2.4 The periodic potential approximation 2.5 Translational symmetry, periodicity, and lattices 3 Electronic energy bands 3.1 Free electron model 3.2 Symmetries and energy bands 3.3 Nearly-free electron model 3.4 Tight-binding model 3.5 Electron (or hole) velocity in a band and the f-sum rule 3.6 Periodic boundary conditions and summing over band states 3.7 Energy bands for materials 4 Lattice vibrations and phonons 4.1 Lattice vibrations 4.2 Second quantization and phonons 4.3 Response functions: heat capacity 4.4 Density of states 4.5 Critical points and van Hove singularities Part I ProblemsPart II Electron interactions, dynamics, and responses 5 Electron dynamics in crystals 5.1 Effective Hamiltonian and Wannier functions 5.2 Electron dynamics in the effective Hamiltonian approach 5.3 Shallow impurity states in semiconductors 5.4 Motion in external fields 5.5 Effective mass tensor 5.6 Equations of motion, Berry phase, and Berry curvature 6 Many-electron interactions: the homogeneous interacting electron gas and beyond 6.1 The homogeneous interacting electron gas or jellium model 6.2 Hartree–Fock treatment of the interacting electron gas 6.3 Ground-state energy: Hartree–Fock and beyond 6.4 Electron density and pair-correlation functions 6.5 g(r, r′) of the interacting electron gas 6.6 The exchange-correlation hole 6.7 The exchange-correlation energy 7 Density functional theory (DFT) 7.1 The ground state and density functional formalism 7.2 The Kohn–Sham equations 7.3 Ab initio pseudopotentials and density functional theory 7.4 Some applications of DFT to electronic, structural, vibrational, and related ground-state properties 8 The dielectric function for solids 8.1 Linear response theory 8.2 Self-consistent field framework 8.3 The RPA dielectric function within DFT 8.4 The homogeneous electron gas 8.5 Some simple applications 8.6 Some other properties of the dielectric function Part II ProblemsPart III Optical and transport phenomena 9 Electronic transitions and optical properties of solids 9.1 Response functions 9.2 The Drude model for metals 9.3 The transverse dielectric function 9.4 Interband optical transitions in semiconductors and insulators 9.5 Electron–hole interaction and exciton effects 10 Electron–phonon interactions 10.1 The rigid-ion model 10.2 Electron–phonon matrix elements for metals, insulators, and semiconductors 10.3 Polarons 11 Dynamics of crystal electrons in a magnetic field 11.1 Free electrons in a uniform magnetic field and Landau levels 11.2 Crystal electrons in a static B-field 11.3 Effective mass and real-space orbits 11.4 Quantum oscillations: periodicity in 1/Band the de Haas–van Alphen effect in metals 12 Fundamentals of transport phenomena in solids 12.1 Elementary treatment of magnetoresistance and the Hall effect 12.2 The integer quantum Hall effect 12.3 The Boltzmann equation formalism and transport in real materials 12.4 Electrical and thermal transport with the linearized Boltzmann equation Part III ProblemsPart IV Many-body eﬀects, superconductivity, magnetism, and lower-dimensional systems 13 Using many-body techniques 13.1 General formalism 13.2 Interacting Green’s functions 13.3 Feynman diagrams and many-body perturbation theory techniques 14 Superconductivity 14.1 Brief discussion of the experimental background 14.2 Theories of superconductivity 14.3 Superconducting quasiparticle tunneling 14.4 Spectroscopies of superconductors 14.5 More general solutions of the BCS gap equation 14.6 Field theoretical methods and BCS theory 15 Magnetism 15.1 Background 15.2 Diamagnetism 15.3 Paramagnetism 15.4 Ferromagnetism and antiferromagnetism 15.5 Magnetism in metals 15.6 Magnetic impurities and local correlation effects 16 Reduced-dimensional systems and nanostructures 16.1 Density of states and optical properties 16.2 Ballistic transport and quantization of conductance 16.3 The Landauer formula 16.4 Weak coupling and the Coulomb blockade 16.5 Graphene, carbon nanotubes, and graphene nanostructures 16.6 Other quasi-2D materials Part IV ProblemsReferencesIndex*

Fundamentals of Condensed Matter Physics

Based on an established course and covering the fundamentals, central areas, and contemporary topics of this diverse field, Fundamentals of Condensed Matter Physics is a much-needed textbook for graduate students. The book begins with an introduction to the modern conceptual models of a solid from the points of view of interacting atoms and elementary excitations. It then provides students with a thorough grounding in electronic structure and many-body interactions as a starting point to understanding many properties of condensed matter systems – electronic, structural, vibrational, thermal, optical, transport, magnetic, and superconducting – and the methods used to calculate them. Taking readers through the concepts and techniques, the text gives both theoretically and experimentally inclined students the knowledge needed for research and teaching careers in this field. It features over 246 illustrations, 9 tables and 100 homework problems, as well as numerous worked examples, for students to test their understanding. Marvin L. Cohen is University Professor of Physics at the University of California at Berkeley and Senior Faculty Scientist at the Lawrence Berkeley National Laboratory. His research covers a broad spectrum of subjects in theoretical condensed matter physics. He is an elected member of the National Academy of Sciences, the American Academy of Arts & Sciences, and the American Philosophical Society. He has received numerous awards, including the US National Medal of Science, the Buckley Prize and the Lilienfeld Prize of the American Physical Society, the von Hippel Award of the Materials Research Society, and the Dickson Prize in Science. He has received honorary degrees from the University of Montreal, the Hong Kong University of Science & Technology, and the Weizmann Institute of Science. He is a former President of the American Physical Society. Steven G. Louie is Professor of Physics at the University of California at Berkeley and Senior Faculty Scientist at the Lawrence Berkeley National Laboratory. His research spans a broad spectrum of topics in theoretical condensed matter physics and nanoscience. He is an elected member of the National Academy of Sciences, the American Academy of Arts & Sciences, and an academician of the Academia Sinica of the Republic of China (Taiwan). He has won numerous awards and prizes for his work, including the Rahman Prize and the Davisson–Germer Prize of the American Physical Society, the Materials Theory Award of the Materials Research Society, and the Sustained Outstanding Research in Solid State Physics Award of the US Department of Energy. He and Cohen shared the Foresight Institute Richard P. Feynman Prize in Nanotechnology (Theory).

Fundamentals of Condensed Matter Physics MARVIN L. COHEN University of California, Berkeley

STEVEN G. LOUIE University of California, Berkeley

University Printing House, Cambridge CB2 8BS, United Kingdom Cambridge University Press is part of the University of Cambridge. It furthers the University’s mission by disseminating knowledge in the pursuit of education, learning and research at the highest international levels of excellence. www.cambridge.org Information on this title: www.cambridge.org/9780521513319 c Cambridge University Press 2016 This publication is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published 2016 Printed in the United Kingdom by TJ International Ltd. Padstow Cornwall A catalogue record for this publication is available from the British Library Library of Congress Cataloguing in Publication data Names: Cohen, Marvin L., author. | Louie, Steven G., 1949– author. Title: Fundamentals of condensed matter physics / Marvin L. Cohen and Steven G. Louie, Department of Physics, University of California at Berkeley, Materials Sciences Division, Lawrence Berkeley National Laboratory. Description: Cambridge, United Kingdom : Cambridge University Press, 2016. | 2016 | Includes bibliographical references and index. Identifiers: LCCN 2016003013| ISBN 9780521513319 (hardback) | ISBN 0521513316 (hardback) Subjects: LCSH: Condensed matter. Classification: LCC QC173.454.C64 2016 | DDC 530.4/1–dc23 LC record available at http://lccn.loc.gov/2016003013 ISBN 978-0-521-51331-9 Hardback Additional resources for this publication at www.cambridge.org/cohenlouie Cambridge University Press has no responsibility for the persistence or accuracy of URLs for external or third-party internet websites referred to in this publication, and does not guarantee that any content on such websites is, or will remain, accurate or appropriate.

To Suzy and Jane

Contents

Preface

page xi

Part I

Basic concepts: electrons and phonons

1 Concept of a solid: qualitative introduction and overview 1.1 1.2 1.3 1.4 1.5 1.6 1.7

Classification of solids A first model of a solid: interacting atoms A second model: elementary excitations Elementary excitations associated with solids and liquids External probes Dispersion curves Graphical representation of elementary excitations and probe particles 1.8 Interactions among particles

2 Electrons in crystals 2.1 2.2 2.3 2.4 2.5

General Hamiltonian The Born–Oppenheimer adiabatic approximation The mean-field approximation The periodic potential approximation Translational symmetry, periodicity, and lattices

3 Electronic energy bands 3.1 3.2 3.3 3.4 3.5 3.6

Free electron model Symmetries and energy bands Nearly-free electron model Tight-binding model Electron (or hole) velocity in a band and the f-sum rule Periodic boundary conditions and summing over band states 3.7 Energy bands for materials

4 Lattice vibrations and phonons 4.1 Lattice vibrations 4.2 Second quantization and phonons vii

3 3 4 6 7 8 9 13 13

20 20 21 22 22 23

31 31 33 39 43 48 52 55

63 63 71

Contents

viii

4.3 Response functions: heat capacity 4.4 Density of states 4.5 Critical points and van Hove singularities

91

Part I Problems

Part II

Electron interactions, dynamics, and responses

5 Electron dynamics in crystals 5.1 5.2 5.3 5.4 5.5 5.6

77 79 84

Effective Hamiltonian and Wannier functions Electron dynamics in the effective Hamiltonian approach Shallow impurity states in semiconductors Motion in external fields Effective mass tensor Equations of motion, Berry phase, and Berry curvature

101 101 103 107 108 113 114

6 Many-electron interactions: the homogeneous interacting electron gas and beyond

119

6.1 The homogeneous interacting electron gas or jellium model 6.2 Hartree–Fock treatment of the interacting electron gas 6.3 Ground-state energy: Hartree–Fock and beyond 6.4 Electron density and pair-correlation functions 6.5 g(r, r ) of the interacting electron gas 6.6 The exchange-correlation hole 6.7 The exchange-correlation energy

121 123 126 130 132 135 136

7 Density functional theory (DFT) 7.1 7.2 7.3 7.4

The ground state and density functional formalism The Kohn–Sham equations Ab initio pseudopotentials and density functional theory Some applications of DFT to electronic, structural, vibrational, and related ground-state properties

8 The dielectric function for solids 8.1 8.2 8.3 8.4 8.5 8.6

Linear response theory Self-consistent field framework The RPA dielectric function within DFT The homogeneous electron gas Some simple applications Some other properties of the dielectric function

Part II Problems

141 142 144 150 152

159 159 163 164 166 169 173

178

Contents

ix

Part III Optical and transport phenomena 9 Electronic transitions and optical properties of solids 9.1 9.2 9.3 9.4 9.5

Response functions The Drude model for metals The transverse dielectric function Interband optical transitions in semiconductors and insulators Electron–hole interaction and exciton effects

10 Electron–phonon interactions 10.1 The rigid-ion model 10.2 Electron–phonon matrix elements for metals, insulators, and semiconductors 10.3 Polarons

11 Dynamics of crystal electrons in a magnetic field 11.1 11.2 11.3 11.4

Free electrons in a uniform magnetic field and Landau levels Crystal electrons in a static B-field Effective mass and real-space orbits Quantum oscillations: periodicity in 1/B and the de Haas–van Alphen effect in metals

12 Fundamentals of transport phenomena in solids 12.1 12.2 12.3 12.4

Elementary treatment of magnetoresistance and the Hall effect The integer quantum Hall effect The Boltzmann equation formalism and transport in real materials Electrical and thermal transport with the linearized Boltzmann equation

Part III Problems

185 185 189 192 196 201

220 220 224 229

235 235 237 239 241

248 248 257 264 271

278

Part IV Many-body eﬀects, superconductivity, magnetism, and lower-dimensional systems 13 Using many-body techniques 13.1 General formalism 13.2 Interacting Green’s functions 13.3 Feynman diagrams and many-body perturbation theory techniques

14 Superconductivity 14.1 Brief discussion of the experimental background 14.2 Theories of superconductivity 14.3 Superconducting quasiparticle tunneling

287 287 291 298

305 305 311 349

Contents

x

14.4 Spectroscopies of superconductors 14.5 More general solutions of the BCS gap equation 14.6 Field theoretical methods and BCS theory

15 Magnetism 15.1 15.2 15.3 15.4 15.5 15.6

Background Diamagnetism Paramagnetism Ferromagnetism and antiferromagnetism Magnetism in metals Magnetic impurities and local correlation effects

16 Reduced-dimensional systems and nanostructures 16.1 16.2 16.3 16.4 16.5 16.6

Density of states and optical properties Ballistic transport and quantization of conductance The Landauer formula Weak coupling and the Coulomb blockade Graphene, carbon nanotubes, and graphene nanostructures Other quasi-2D materials

356 360 368

372 372 372 374 377 386 389

393 393 399 404 406 409 421

Part IV Problems

424

References Index

434 440

Preface

The field of condensed matter physics is the largest branch of physics worldwide and probably the most diverse. Undergraduate courses in this area are ubiquitous and most research universities offer graduate courses. Over the past 50 years, the undergraduate course has been open to physicists, chemists, materials scientists, engineers, and, to a smaller extent, biologists. The graduate course slowly evolved in many institutions from a course for theorists to one that welcomed students interested in a career in experimental condensed matter physics and materials research. In recent years, the proportion of chemists, materials scientists, engineers, and researchers in nanoscience has increase significantly in graduate courses in condensed matter physics. There are numerous undergraduate texts. The prime example is Introduction to Solid State Physics (ISSP) authored by C. Kittel. At the graduate level, no single text has emerged as the canonical choice. N. Ashcroft and N. D. Mermin’s book Solid State Physics is sometimes chosen since it contains advanced topics going beyond Kittel’s ISSP, although Ashcroft & Mermin is often used as an undergraduate text. J. Ziman’s Principles of the Theory of Solids is at roughly the same level as Ashcroft & Mermin, with excellent physical examples and discussions of concepts. C. Kittel’s Quantum Theory of Solids, which was written for the graduate course at the University of California, Berkeley, at a time when students taking the course were predominantly theorists, is somewhat limited in scope and generally considered difficult by graduate students not intent on a career in theoretical condensed matter physics. Other texts, such as those by J. Callaway, O. Madelung, M. Marder, and J. Patterson and B. Bailey, are considered to be at the right level and suitable. Many others are in the recommended, but not required, category and are useful when specific subjects are considered. Examples include those authored by E. Kaxiras, R. Martin, M. Balkanski and R. Wallis, P. Yu and M. Cardona, and M. Cohen and J. Chelikowsky for electronic and optical properties of solids; M. Tinkham, P. de Gennes, and R. Schrieffer for superconductivity; G. Mahan for many-particle physics; and P. Chailken and T. Lubensky for phase transitions and soft matter systems. There are also many other excellent texts on specific subjects in this field. The present text, Fundamentals of Condensed Matter Physics, is intended to cover the “mainstream” subjects in this field at the graduate level. It is probably impossible to produce a book that fills the complete bill for a course, as J. D. Jackson’s E&M text has done for electricity and magnetism, because the range of topics is so broad. To cover the whole field would require many volumes. Hence the intent here is to write a text that covers the central topics on a level that will prepare a student to enter research, and that can serve as a higher-level source to sit alongside undergraduate texts for researchers in this field. xi

xii

Preface

This text is based on lectures given as part of the condensed matter physics graduate course at Berkeley since 1965. The course, called Physics 240A and B, is a two-semester (or three-quarter) course covering 90 hours of lectures. In addition, there is a weekly discussion section for going over problem sets. Over the decades, this course was taught by one of the authors, either Marvin L. Cohen or Steven G. Louie, with guest lecturers from time to time. Student evaluations of the course have been high. The class size has typically been 20–30 students plus auditors. Of the more than one thousand students who took this course, a fair number have taken academic positions and have reported back that they have used their course notes successfully to teach similar courses in various departments including physics, chemistry, materials science, and engineering. The book is divided into four main parts. Part I is devoted to the development of basic concepts. It begins with an introduction to the modern conceptual models of a solid from the points of view of (i) interacting atoms and (ii) elementary excitations, and then develops a thorough grounding on the basic elements needed to understand many of the properties of solids and the methods used to calculate them. Part II concerns the fundamentals of electron interactions, electron dynamics, and response functions, that control and exhibit the properties of and phenomena in condensed matter. Parts III and IV focus on the different properties and phenomena that are central to modern condensed matter and materials research. These include vibrational, thermal, optical, and transport properties, superconductivity, magnetism, and lower-dimensional systems, with emphasis on developing a physical understanding of real material systems. A range of theoretical techniques is developed as needed. The mathematical level varies, as does the degree of detail, in a manner similar to what one would experience in the world of research. Topics and techniques, such as band structure methods, pseudopotentials, density functional theory, effective Hamiltonians, electron dynamics, dielectric functions, electron–electron and electron–hole interactions, Berry’s phase, Boltzmann transport theory, optical response, cooperative phenomena, many-body Green’s functions, and diagrammatic and quasiparticle approaches, are explored and motivated by “real problems” associated with understanding and calculating material properties. Experimental techniques are described but not in detail. Because of the breadth of the field and the limitation to one volume, some subjects are not treated in depth and others are left out completely. However, the success of the course at Berkeley, and hopefully this text, is that it takes a student through the concepts and techniques for many central areas of condensed matter physics, and establishes the level needed to start current research. Hence, the intent is to take students with a good knowledge of graduate quantum mechanics and undergraduate condensed matter physics to a level where they can do cutting-edge research. The book is suitable for a one-semester course (covering most of Parts I and II and some selected topics in Parts III and IV) or a two-semester course (covering essentially all of Parts I–IV with the option of omitting some topics as desired by the instructor). This book would not have been possible without help from many people. We would especially like to thank Ms. Katherine de Raadt for her help with editorial matters and for producing the manuscript. We would like to acknowledge Cheol-Hwan Park for some of his class notes from the Berkeley course, David Penn for suggestions and critical readings

xiii

Preface

of part of the text, Felipe Jornada and Sangkook Choi for producing most of the figures and for useful suggestions, and Meng Wu for his contributions in producing the problem sections. We profited from helpful corrections of the various chapters of the text by Gabriel Antonius, Brad Barker, Ting Cao, Sinisa Coh, Zhenglu Li, Jamal Mustafa, Chin-Shen Ong, Diana Qiu, Liang Tan, and Derek Vigil-Fowler. Finally, we thank Simon Capelin of Cambridge University Press for his guidance and patience. Marvin L. Cohen Steven G. Louie Berkeley, CA, USA Spring, 2016

PART I

BASIC CONCEPTS: ELECTRONS AND PHONONS

1

Concept of a solid: qualitative introduction and overview 1.1 Classiﬁcation of solids Condensed matter physics and solid state physics usually refer to the same area of physics, but in principle the former title is broader. Condensed matter is meant to include solids, liquids, liquid crystals, and some plasmas in or near solids. This is the largest branch of physics at this time, and it covers a broad scope of physical phenomena. Topics range from studies of the most fundamental aspects of physics to applied problems related to technology. The focus of this book will be primarily on the quantum theory of solids. To begin, it is useful to start with the concept of a solid and then describe the two commonly used models that form the basis for modern research in this area. The word “solid” evokes a familiar visual picture well described by the definition in the Oxford Dictionary: “Of stable shape, not liquid or fluid, having some rigidity.” It is the property of rigidity that is basic to the early studies of solids. These studies focused on the mechanical properties of solids. As a result, until the nineteenth century the most common classification of solids involved their rigidity or mechanical properties. The Mohs hardness scale (talc – 1; calcite – 3; quartz – 7; diamond – 10) is a typical example. This is a useful but limited approach for classifying solids. The advent of atomic theory brought more microscopic concepts about solids. Solids were viewed as collections of more or less strongly interacting atoms. From the point of view of atomic theory, a gas is described in terms of a collection of almost independent atoms, while a liquid is formed by atoms that are weakly interacting. This picture leads to a description of the formation of solids, under pressure or by freezing, in which the distances between atoms are reduced and, in turn, this causes them to interact more strongly. Molecular solids are formed by condensing molecular gases. Hence, the development of atomic physics and chemical analysis led to a more detailed classification of solids according to chemical composition. Although for most studies of solids it is necessary to establish the identity of the constituent atoms, such a scheme provides limited insight into many of the basic concepts of condensed matter physics. Solids can also be classified according to their crystalline structure. This monumental feat has occupied crystallographers and applied mathematicians for over a hundred years. The discovery of X-ray crystallography added an important component to the atomic model. The chemical view of a crystalline solid as a collection of strongly interacting atoms can be expanded by adding that the atoms arrange themselves in a periodic structure. This

3

4

1 Concept of a solid: qualitative introduction and overview

Table 1.1 Classiﬁcation of solids using resistivity. Class

Typical resistivity ( cm)

Example

metal semimetal semiconductor insulator

10−6 10−3 10−2 –109 1014 –1022

copper bismuth silicon diamond

would not be true for non-crystalline solids such as window glass. For most modern studies of solids, it is usually assumed that the structure and chemical composition are known and that information of this kind is the starting point for most investigations. When new materials are discovered, chemical and structural analyses are often the first steps in the characterization process. Properties other than mechanical, chemical, and structural can be used to classify solids. Electromagnetic and thermal characteristics are commonly used. In particular, the resistivity ρ is the most used property, since it involves a single scalar quantity or a symmetric tensor with a range of values for different substances that varies at room temperature by about 28 orders of magnitude. For many materials ρ can be measured with great precision. Even though this approach focuses on a macroscopic property, with some theoretical analysis, it provides considerable insight into the microscopic nature of solids. Table 1.1 lists the classification according to resistivity of the four classes of solids: metals, semimetals, semiconductors, and insulators. Typical resistivities and examples for each class are also given. Although the divisions between classes are approximate, this classification of solids is extremely useful for a wide variety of studies and applications. The chemical and structural classifications lead naturally to a model of crystalline solids based on interacting atoms. This is a fruitful approach and suggests that it may be possible to explain and predict the properties of solids through an adjustment or perturbation of the properties of atoms. The use of the resistivity for the classification of types of solids suggests another view, where the responses of a solid to external probes are used to classify solids. Electromagnetic, thermal, or mechanical probes can give rise to responses that may arise from the collective nature of the interacting particles in solids. However, viewing the solid as perturbed atoms may not lead naturally to an interpretation of its properties in terms of collective or cooperative effects. The interacting atoms approach is convenient for describing ground-state properties, whereas collective effects are best explained in terms of a model based on the excitations of the solid. Both models are discussed in more detail below.

1.2 A ﬁrst model of a solid: interacting atoms Consider aluminum metal. It is a relatively soft solid with hardness between 2 and 2.9 on the Mohs scale and it is composed of a single element. It crystallizes in the face-centered

1.2 A ﬁrst model of a solid: interacting atoms

5

nucleus: +13 e

Figure 1.1

core electrons: –10 e

valence electrons: –3 e

Schematic drawing of a solid consisting of atoms with atomic number z = 13 containing cores and valence electrons. Here e denotes the charge of a proton.

˚ it is a reasonably good conductor cubic structure with cubic lattice constant a = 4.5 A, (ρ = 2.8 × 10−6 cm at 20◦ C), and it becomes a superconductor at Tc = 1.19 K. What model can be used as a basis for explaining these properties? Why is aluminum different from copper, solid argon, solid oxygen, silicon, sodium chloride, or anthracene? The most straightforward approach is to start from the chemical and atomic descriptions and to consider aluminum metal as a collection of interacting aluminum atoms. Each aluminum atom is composed of a nucleus with atomic number Z = 13. Hence in the neutral atom, there are 13 protons and 13 electrons. The electronic configuration can be easily divided into 10 core electrons, denoted by principal and angular momentum quantum labels as [(1s)2 (2s)2 (2p)6 ], and three outer valence electrons [(3s)2 (3p)1 ]. One picture of solid aluminum is a collection of cores with each core composed of a nucleus plus the tightly bound core electrons. Because of the cancellation of charge of 10 protons by the core electrons, the core has an effective charge Zeff = 3. Moving around the cores and between them is a collection of itinerant, nearly-free electrons; there are three per core. A schematic drawing is given in Fig. 1.1. Cores and valence electrons move in a potential set by their mutual interactions. The laws of motion are well known and are described by quantum mechanics. The Schr¨odinger equation is sufficient in most cases; however, the Dirac equation may be necessary if relativistic effects are to be incorporated. The forces are also known; only electromagnetism plays a role. Gravity and weak

6

1 Concept of a solid: qualitative introduction and overview

interactions are too feeble, and strong interactions are too short-ranged. However, the problem is not an easily solvable one since there are of the order of 1023 interacting particles in solids per cm3 . Approximate methods must be used and simpler models developed. These will be discussed in Chapter 2.

1.3 A second model: elementary excitations A drastically different approach to studying condensed matter systems is also in common use. In quantum mechanics and quantum field theory, it is often convenient to change the description of a system when discussing its excited states. This picture is based on the excitations that can emerge when a system is not in its ground state. A standard example is a harmonic oscillator of mass m moving in a quadratic potential 12 mω2 x2 . This system has an energy spectrum defined by a quantum number n, En = (n+ 12 )hω, ¯ which can be viewed 1 as a ground state having energy E0 = 2 hω, ¯ and higher-energy states in which quanta of excitation energy hω ¯ can be created and subsequently destroyed in any non-negative integral number n. Another example is the electromagnetic field, which can can be viewed as a collection of quantized particle-like excitations, the photons, each one characterized by a wavevector k, a polarization direction ˆ , and energy hω where c is the velocity ¯ = hc|k|, ¯ of light. The examples above give an operational definition of a quantum system that is described by its excitations, each one defined by its energy and other specific physical characteristics. Once the excitations are identified, the next task is to study the interactions between various excitations and the manner in which these excitations appear, disappear, or are modified when the external conditions of the quantum system change. In the end, the quantum system will be characterized by its elementary excitations when probes are used to study its properties. The elementary excitations of a solid can often be divided into two classes: quasiparticles and collective excitations. Quasiparticles are usually fermions and resemble well-defined excited states of the non-interacting real particles of the solid. Collective excitations are usually bosons and do not resemble their constituent real particles. In the majority of cases, collective excitations are associated with macroscopic collective motions of the system, which in turn are described by quanta of generalized harmonic oscillators that can be created or destroyed in an integral number n. Each quantum provides an excitation energy h¯ ω. The language of second quantization is the natural one to use for this model. Since elementary excitations can be created and destroyed, and since symmetric (Bose–Einstein) or antisymmetric (Fermi–Dirac) conditions must be satisfied, creation and destruction operators, with their attendant commutation and anticommutation rules, are among the fundamental descriptive tools of this approach. To explain the properties of a solid, it is advantageous to define the elementary excitations of the solid, to describe their properties and characteristics, to evaluate their interactions, and to determine how they respond to external probes.

7

1.4 Elementary excitations associated with solids and liquids

1.4 Elementary excitations associated with solids and liquids Quasielectrons. Quasielectrons (or electrons for short) are quasiparticles that behave like non-interacting electrons in low-lying excited states. They are fermions that are characterized by energy and quantum numbers, such as their wavevectors and spin orientations. Their properties include the effects of the environment in which they move. An important example is that of an electron experiencing the interaction with other electrons that can change its free electron mass m to an effective mass m∗ > m. The resultant quasielectron can be described by one-particle states of spin 12 and charge −|e|. Typical excitation energies for quasielectrons are of the order of the Coulomb interaction energy between 2 two electrons separated by a crystal lattice parameter a: ea ∼ = 5 eV. Typical velocities e2 1/2 ∼ 8 ∼ associated with quasielectrons are v = ( ) = 10 cm/s. am

Hole. The removal of an electron from an orbital that is normally occupied in the ground state is called a hole. The analogy is made with the Dirac theory of positrons. A hole is a quasiparticle that has charge +|e|, spin 12 , and energies and velocities similar to quasielectrons. When electrons are injected into or removed from a solid in processes such as those associated with quantum tunneling phenomena and electron emission, they are often treated as single particles without any reference to the holes left behind. The holes are usually studied separately. Phonon. A phonon is a collective excitation (boson) associated with lattice vibrations or sound waves. It is defined by a wavevector q, a branch or polarization mode index α, and an energy h¯ ω. Typical energies are of the order of kB TD , where kB is Boltzmann’s constant and TD is the Debye temperature. Since TD is of the order of room temperature (∼300 K), a typical phonon energy is hω = 0.025 eV. ¯ ∼ Plasmon. A plasmon is a collective excitation (boson) associated with the collective motion of the electronic charge density. It is characterized by a wavevector q and an energy of the order of the classical plasma energy (in three dimensions) 1 4π ne2 2 , hω ¯ p = h¯ m

(1.1)

where n is the density of valence electrons per unit volume. For typical solids, hω = 10 ¯ p∼ eV. This value can be smaller by an order of magnitude or more in low-density electron or hole systems such as those found in semimetals and degenerate semiconductors. Magnon. A magnon is the collective excitation (boson) associated with spin waves or spin excitations, resulting from the occurrence of spin reversals in an ordered magnetic system. Typical energies are of the order of the ordering temperatures (Curie or N´eel). These can be as high as 10−1 eV, but are usually much lower (∼ 4 × 10−5 eV). Polaron. A polaron is a special type of quasielectron that exists in crystals. It can be regarded as an electron or a hole moving through a crystal and carrying a lattice deformation or strain with it. If the strain is expressed in terms of excitations of phonons, this leads to the view of a polaron as an electron accompanied by a cloud of phonons. The terms

8

1 Concept of a solid: qualitative introduction and overview

“polaron” and “polaron effects” are often used to describe changes in electron properties arising from electron–phonon interactions in general. Exciton. An exciton is a bound or quasibound state of a quasielectron and a hole. This elementary excitation is similar to positronium, and it often behaves as a boson which can be decomposed into its two component fermions or radiatively annihilated. Excitons are usually observed in insulators and semiconductors. Typical binding energies are ∼0.025 eV in three-dimensional systems. Superconducting quasiparticles. Superconducting quasiparticles are fermions that describe the electronic excited states of a superconductor. They are sometimes called Cooper particles (not Cooper pairs) or Bogoliubons. Because of the physics inherent in the description of the superconducting ground state, these quasiparticles are viewed as a linear combination of quasielectrons and holes. Typical energies are of the order of the superconducting transition temperature between 10−5 eV and 10−2 eV, depending on the material. Roton. A roton can be viewed as a special phonon associated with a local energy minimum in the dispersion relation at a finite wavevector. This description usually applies to liquid He4 . Typical roton energies in helium are of the order of 10−3 eV.

1.5 External probes Knowledge about the properties of solids is obtained from measurements done under welldefined conditions. These are either equilibrium situations, in which the temperature and externally applied static electric and magnetic fields are predetermined, or dynamical situations in which energy, momentum, angular momentum, and other dynamical quantities are exchanged with the environment. In the latter case, the agents that effect this exchange are also microscopic quanta, the so-called test or probe particles. Some of these are listed below. Photons. Electromagnetic probes are the most commonly used probes in solids, for example, they are used in absorption spectra, reflectivity spectra, and photoemission spectra. The energy range of the useful photons spans the available electromagnetic spectrum, from radio frequency studies of metals (hω = 2 × 10−8 eV) to γ -radiation studies of the ¯ ∼ 6 ∼ M¨ossbauer effect (hω ¯ = 2 × 10 eV). Electrons. Electrons are used to probe solids in a variety of ways. They are injected and extracted through electrical contacts and tunneling junctions, or used as scattering particles in electron beams. Typical energies vary with the experiment: ∼1 meV for superconductive tunneling; ∼1 eV for semiconductor tunneling; ∼ 10−2 to 2 eV for scanning tunneling microscope investigations of surfaces; ∼ 10 to 100 eV for low-energy electron diffraction at solid surfaces; and ∼100 keV to 1 MeV for high-energy electron microscopy. Positrons. Positron annihilation in solids arising from electron–positron interactions provides useful information for investigating the electronic properties of solids – primarily metals. Photons are emitted when the annihilation occurs and studies of the emitted radiation give information about the electronic structure.

1.6 Dispersion curves

9

Neutrons. Neutron scattering has become the standard and preferred technique to study magnetic structural properties and properties of phonons, magnons, and other collective excitations in solids, owing to the fact that a neutron is a neutral particle with a magnetic moment. Muons and pions. Muons and pions are used as probes, but they are not as commonly used as most of the other particles discussed here. Muons are more versatile than pions because of their similarity to heavy electrons. Their magnetic moments and decay modes can give information not obtained with other methods. Protons. Protons can be used to study the structures of crystalline solids, primarily by examining their trajectories in solids. Atoms. Light atoms and ions are usually employed to study surfaces; sometimes they can be used to probe deeper into solids. Their role is often similar to that of electrons in scattering experiments.

1.6 Dispersion curves All the probe particles can be characterized by a momentum (or wavevector or wavelength) and an energy (or frequency). The particles are assumed to exist in free space or vacuum. For massive particles with mass m, the dispersion curve, which is the functional relation between the energy E and the momentum p or wavevector k, is given by E=

h¯ 2 k2 p2 = , 2m 2m

(1.2)

or, in the relativistic limit, by E = (h¯ 2 k2 c2 + m2 c4 )1/2 − mc2 ,

(1.3)

where c is the speed of light. The probing photon in free space (a massless particle) is described by the dispersion curve, connecting the frequency ω and wavevector k, ω = ck. These dispersion curves are illustrated in Fig. 1.2. In a solid or liquid, most elementary excitations are also defined by a wavevector and an energy or frequency. The functional dependence of the energy on the wavevector, that is, the dispersion curve, constitutes one of the most fundamental properties of the excitations to be determined. The quasielectron dispersion curve can be used to distinguish the various types of solids: metals – no gap in the spectrum and the existence of a Fermi surface; semiconductors and insulators – an electronic energy gap of order 0.1 to 10 eV, caused by the ion core potential and uniquely related to specific k-space locations; and superconductors – an energy gap for creating a quasielectron and quasihole pair of order 2 < 10−1 eV caused by dynamic interactions of the electrons. Some examples of dispersion curves for quasiparticles are shown in Fig. 1.3. The quasielectrons and holes in metals (Fig. 1.3(a)) have excitation energies which start from zero. Excitations with zero energy define a surface in k-space known as the Fermi surface. For

1 Concept of a solid: qualitative introduction and overview

10

Energy E

(b)

Energy E

(a)

Wavevector k

Figure 1.2

Wavevector k

Dispersion curves for probe particles. (a) Free particle of mass m. (b) Photons in vacuum.

semiconductors, the excitation spectrum has a different starting value for electrons and holes, which depends on the chemical potential μ (or EF ) of the system. Silicon is used as an example in Fig. 1.3(b). The lowest-energy electron excitation is at a well-defined k-vector, k = kcb , and the lowest-energy hole state is at k = kvb . For the silicon example, kvb = 0, while kcb has a finite value along the (100) direction of k-space, and the minimum energy required to create a quasielectron and a hole is 1.1 eV. This is the minimum bandgap Eg for silicon. Superconducting quasiparticle spectra also exhibit an energy gap. The minimum energy for creating both a superconducting quasielectron and quasihole requires an energy of 2. This is usually a much smaller gap than in semiconductors (2 = 0.3 meV in aluminum), and it appears at what, in the normal state, was the Fermi surface of the metal. The semiconducting and superconducting gaps are of very different natures; their characteristics are discussed in subsequent chapters. It is often convenient to choose a specific form for the dispersion curve near local minima or maxima and in other regions where quadratic approximations are appropriate. For example, in the case of an electron or hole at a band minimum with wavevector k0 , it is convenient to write (1.4) E(k) = 12 h¯ 2 (k − k0 ) · A · (k − k0 ), where the tensor Aij ≡ 1/m∗ij can be interpreted as an inverse effective mass tensor. For a free electron, the relation (Eq. (1.4)) holds exactly with Aij = m−1 δij ,

(1.5)

where m is the free electron mass (see Eq. (1.2) and Fig. 1.2). In solids, effective masses may differ substantially from the free electron mass. For example, m∗ ∼ = 0.01m for quasielectrons near the conduction band minimum in InSb. This small m∗ value is caused by the static crystal potential, which is also responsible for the existence of the energy gap. In sodium metal, where the Fermi surface is, to a very good approximation, a sphere of radius

1.6 Dispersion curves

11

(a) E

(b) E

EF

EF

Eg k kcb

kBZ

k 0

kF

kvb = 0

kBZ

Energy E

(c)

Δ

EF

k 0

Figure 1.3

kF

kBZ

Dispersion curves. (a) Quasielectrons and holes in a simple metal, for example, an alkali metal. Quasielectrons are excited into states E > EF , k > kF , where EF and kF are the Fermi energy and wavevector and kBZ is the wavevector for the Brillouin zone edge. Hole states are by convention often plotted by the dispersion curve for E < EF and k < kF . However, since it costs energy to remove an electron to create a hole, the hole branch of the dispersion curve should be inverted and the energies measured positively with hole energies between zero and EF . (b) Quasielectrons and holes in a semiconductor. For the case illustrated, the lowest-energy quasielectron wavevector is centered at kcb at the conduction band minimum, while the lowest-energy hole wavevector is at the valence band maximum centered near kvb = 0. These two kinds of states are separated by energy gap Eg . As in (a), the hole branch of the dispersion curve should be inverted, with the energies measured positively. (c) Quasiparticles in a superconductor. Here the quasielectron and hole branches of (a) are combined. The superconducting gap for creating a single quasiparticle appears at kF . kF , the quasiparticle dispersion curve is given by E(k) =

h¯ 2 2 |k − k2F |. 2m∗

(1.6)

Equation (1.6) is valid for both quasielectrons (|k| > kF ) and holes (|k| < kF ) with an effective mass of m∗ ∼ = 1.25m. This enhancement of 25% over the free electron value is not caused by the static crystal potential. It arises from the dynamic interactions between electrons and phonons and interactions among the electrons. In Fig. 1.4, examples of dispersion curves for collective excitations are given. The specific properties related to features of particular curves are discussed in later chapters.

1 Concept of a solid: qualitative introduction and overview

12

(a)

Phonons

ω

(c)

ω

Plasmons

Optical ωp Acoustic

π – a

0

q

Phonons

(b)

q

0

(d)

ω

ω Rotons LA

TA2

TA1 0

Figure 1.4

Phonons π – a

q

q 0

Dispersion curves (schematic) for collective excitations. (a) Phonons in a one-dimensional solid with lattice constant a and two masses per unit cell. (b) Phonons in a three-dimensional solid with one atom/cell. LA, TA1 , and TA2 refer to the longitudinal acoustical mode and the two transverse acoustical modes, respectively. (c) Plasmons in a three-dimensional metal where ωp is the classical plasma frequency. (d) Phonons and rotons in liquid He-4.

In restricted regions of given spectra, useful analytic approximations are commonly made. For instance, for each mode α of the acoustic phonon dispersion relation near q = 0, it is possible to write hω ¯ α |q|, ¯ α = hv

(1.7)

where vα is the speed of sound propagation for mode α. The determination and interpretation of the dispersion curves for the elementary excitations can be complex. However, a scheme or investigational approach can be outlined. This approach consists of: (1) defining the bare elementary excitation by means of a Hamiltonian formalism; (2) solving the equations of motion to determine the dispersion curves for the “bare” elementary excitations; (3) solving for the “final” spectrum of the excitations after including the necessary interactions among the excitations; (4) including the effects of the external probes and their interactions with the excitations; and (5) solving the new coupled equations to determine the response functions for the condensed matter system. In the above scheme, steps (1) and (2) are usually handled by ordinary quantum mechanical methods, using the Schr¨odinger equation appropriate for one body in an external potential. Steps (3), (4), and (5) are concerned with the many-body aspects that can be

13

1.8 Interactions among particles

electron hole photon phonon plasmon magnon

Figure 1.5

Diagrammatic representation of some elementary excitations and probe particles. Spin and polarization indices (not shown) can be added to the wavevector to specify a state.

evaluated using second quantization and Green’s function techniques, which will be discussed later. In these steps, it is convenient to have a convention to express the physical processes in graphical form. A standard and very convenient choice is the use of Feynman diagrams.

1.7 Graphical representation of elementary excitations and probe particles Elementary excitations, probe particles, and their interactions can be represented graphically (Feynman diagrams). When describing physical processes, it is often assumed that time develops from the left to the right, or from the bottom to the top of the diagram used to describe the process. Each elementary excitation or probe particle is depicted by a line (a different type of line for each type of excitation) and a label that characterizes its quantum numbers. Some graphic representations are shown in Fig. 1.5.

1.8 Interactions among particles In order to accomplish the last three parts of the scheme designed to explain the properties of condensed matter systems using elementary excitations, it is necessary to describe how the elementary excitations interact with one another and with the probe particles. The interactions of interest are given in Table 1.2. It is helpful to develop interactive Hamiltonians that can be analyzed by means of diagrams and use these to give a physical picture of the processes involved.

Table 1.2 Important interactions between excitations and between excitations and probe particles. Elementary Excitations

Probe Particles

Electron Hole Photon Plasmon Magnon Polaron Exciton Superconducting Roton Photon Electron Positron quasiparticle Electron Hole Photon Plasmon Magnon Polaron Exciton Superconducting quasiparticle Roton

x x x x x

x x x x x

x

x

x

x

x x x x x x x x x

x x x x x

x x x x x

x

x x x

x x x

x

x x x x

x x x x x x x

x x x x

x x

x

Neutron

x x x x x

x

x

1.8 Interactions among particles

15

(a) –q

k

k+q

(b)

q

k

k+q

(c) –q

k+q

k

(d) q

k+q

k

(e) k+q q

k (f)

k q k+q

Figure 1.6

Diagrams representing some electron–photon and hole–photon processes. The individual processes are discussed in the text. The electron is represented by the wavevector k and a right-pointing arrow, and a hole is represented by a left-pointing arrow and its wavevector is given by the negative of the electron wavevector k or k + q used in this ﬁgure.

1.8.1 Quasiparticle–boson interactions Many physical processes in condensed matter systems involve the interactions of quasiparticles with bosons. The bosons may correspond to the collective excitations of the system

16

1 Concept of a solid: qualitative introduction and overview

(a) q

k

(b)

k–q

q

k

(c)

q

k

Figure 1.7

k–q

k–q

Some possible quasielectron–boson interactions. (a) Electron–photon. (b) Electron–phonon. (c) Electron– plasmon.

or to the probe particles. Some examples are given in Fig. 1.6, where electrons and holes are used as the prototypes for the quasiparticles, and photons represent bosons. The following cases are given graphically in Fig. 1.6: (a) an electron having wavevector k emits a photon of wavevector −q and is scattered into a state described by wavevection k + q; (b) an electron with wavevector k absorbs a photon of wavevector q and is scattered into a state k + q; (c) a hole with wavevector −k− q emits a photon at wavevector −q and is scattered into the state −k; (d) a hole of wavevector −k − q absorbs a photon of wavevector q and is scattered into the state −k; (e) the creation of an electron of wavevector k + q and a hole of wavevector −k by a photon of wavevector q; and (f) the annihilation of an electron of wavevector k+q and a hole of wavevector −k to produce a photon of wavevector q. The photon representing the boson in Fig. 1.6 can be replaced by other bosons. Examples of common electron–boson interactions are shown in Fig. 1.7. These include the electron–photon interaction and others, such as the electron–phonon interaction and the electron–plasmon interaction. In each of these examples an electron with wavevector k emits a boson of wavevector q and is scattered into a state described by wavevector k − q. The examples above are the fundamental interactions for a large number of physical phenomena. For example, the electron–photon interaction is basic to the processes involved in optical absorption and emission, electron photoemission, X-ray scattering, Compton scattering, Raman scattering, cyclotron resonance, and many other physical phenomena. The electron–phonon interaction is responsible for electrical and thermal resistance, ultrasonic attenuation, polaron formation, and superconductivity. Electron–plasmon interactions dominate electron energy loss in many systems when fast or high-energy electrons

1.8 Interactions among particles

17

q

(a)

k

k–q q

(b)

k

(c)

k

k–q

k–q

k

k + q q

k (d)

k

k–q

k + q q

k

k

(e)

k – q

k–q q

k

Figure 1.8

k

(a) Electron self-energy diagram involving phonon emission and absorption by the same electron. (b) Electron self-energy diagram involving plasmon emission and absorption. (c) Electron–electron Coulomb interaction or photon exchange. (d) Electron–electron interaction via phonon exchange. (e) Electron–hole Coulomb interaction.

pass through solids. Finally, electron-magnon interactions determine magnetic resonance phenomena and transport properties of magnetic materials.

1.8.2 Quasiparticle–quasiparticle interactions Because the quasiparticle concept is only an approximation, all quasiparticles interact directly, in most cases weakly, with one another via residual interactions, or indirectly via the exchange of a collective excitation. These processes can be described using Feynman diagrams, as shown in Fig. 1.8, and are discussed below.

18

1 Concept of a solid: qualitative introduction and overview

Electron and hole self-energies. The emission and reabsorption of a boson “dresses” what would otherwise be a “bare” quasiparticle. This process produces changes in the energy and the quasiparticle effective mass, and for electrons can lead to the formation of a polaron (Fig. 1.8(a)) or a plasmonic polaron (Fig. 1.8(b)). Electron–electron and hole–hole interactions. This interaction leads to ordinary quasiparticle–quasiparticle scattering via the residual Coulomb interaction, which can also be viewed as the exchange of a photon (Fig. 1.8(c)) or, for appropriate cases, the exchange of a phonon (Fig. 1.8(d)), a magnon, or a plasmon. In particular, the phonon exchange (Fig. 1.8(d)) can lead to an effective attraction between quasielectrons, which can result in a transition to the superconducting state. Electron–hole interaction. Electrons and holes can interact via the Coulomb interaction (Fig. 1.8(e)) through the exchange of photons. They can also interact via phonons, plasmons, or magnons. These processes are responsible for the formation of excitons, for screening, and other many-body effects.

1.8.3 Collective excitation interactions Because second quantization can be used to view collective excitations in terms of quanta of harmonic oscillators, any anharmonicity in the original Hamiltonian leads to direct interactions between collective excitations of the same type. This anharmonicity causes a renormalization of the frequencies (“dressing”) of the excitations as well as the decay of the modes into a multiplicity of other modes (“lifetime” effects). A typical example of an anharmonic effect is shown for phonons in Fig. 1.9(a). Ferroelectricity and the thermal expansion of solids are consequences of this interaction.

(a)

–q

q q + q

(b) k+q

q

q k

Figure 1.9

Examples of interactions among collective excitations. (a) Phonon–phonon scattering. (b) Phonon self energy caused by electron–hole pair creation and destruction.

1.8 Interactions among particles

19

(a)

(b) ω

Photon

Frequency ω

LO phonon

Plasmon ωp

Wavevector k

Figure 1.10

LO phonon

TO phonon

Wavevector k

Coupled modes (solid line) formed from bare collective excitations (dashed lines). (a) An optical phonon–photon complex (also called a polariton). The longitudinal optical (LO) and transverse optical (TO) phonon dispersion curves are assumed to be ﬂat near k = 0. (b) A longitudinal optical phonon–plasmon complex. Collective excitations can also be “dressed” by the creation of virtual quasielectron–hole pairs, as shown in Fig. 1.9(b). This process leads to the softening of the frequency of the modes, which can also be responsible for phase transitions. The interaction between two different types of collective excitations is a good example of mode coupling. We can have optical phonon–photon coupled excitations (polaritons), optical phonons–plasmon coupled excitations, exciton–photon coupled excitations, magnon–phonon coupled excitations, magnon–photon coupled excitations, and so forth. If the dispersion curves for any two of these modes intersect, that is, there is a point of common excitation energy and wavevector, the interaction becomes paramount in the neighborhood of the crossover point. There the two modes can be mixed in approximately equal amounts, and each of the original collective excitations loses its identity. Examples for the polariton and the longitudinal optical phonon–plasmon complex are shown in Fig. 1.10.

2

Electrons in crystals

The “scheme” described in Chapter 1 will now be applied to determine the properties of electrons (and holes) in crystals. The first step is to use an appropriate Hamiltonian and then make approximations that exhibit the quasiparticles and allow calculations of their dispersion curves. Next, interactions among the electrons and between electrons and other elementary excitations or test particles will be introduced. The physical properties of the solid, such as the optical properties, can then be described in terms of response functions, such as the dielectric function, that measure the responses of the solid to external probes.

2.1 General Hamiltonian The starting point is based on the first model of a solid described in Chapter 1: a collection of ion cores and itinerant valence electrons. We assume that the electronic core states are atomic-like in character, undeformable, and tightly bound to the nuclei. Therefore, for many applications, each core, which consists of the nucleus and core electrons, can be treated as a single particle. There is a Coulomb attraction between the positive cores and the valence electrons. Near a nucleus, a negative test charge would experience an attractive potential corresponding to all the protons in the nucleus. However, outside the core, the effective charge of the core is reduced by the number of core electrons. For example, in silicon the charge near the nucleus is +14|e|, while the core charge is +4|e|, where e is the charge of an electron. The total Hamiltonian HT for the system of cores and valence electrons is HT =

p2 p2 1 Zn Zn e2 1 e2 n i + + + + Vn (ri − Rn ) + HR , 2m 2Mn 2 |ri − rj | 2 |Rn − Rn | n i

ij

nn

n,i

(2.1) where the first right-hand term is the kinetic energy of the valence electrons, the second term is the kinetic energy of the cores, the third term is the Coulomb interaction between electrons, the fourth term is the Coulomb interaction between cores, the fifth term is the interaction between electrons and cores, and the final term represents the relativistic corrections, including spin–orbit coupling. In Eq. (2.1), the primed summation indicates either i = j or n = n ; ri , pi , e, and m are the electron position, momentum, charge, and mass, while Rn , pn , Zn , and Mn are the core position, momentum, charge, and mass. A straightforward approach for solving Eq. (2.1) is not practical since an exact solution would imply the handling of ∼1023 quantum numbers 20

2.2 The Born–Oppenheimer adiabatic approximation

21

to describe the system. Even if available, these quantum numbers would be too numerous for practical applications, and most of them are likely to have obscure or non-useful physical meaning. Approximations are a necessity and must be introduced from the start. Three basic approximations are described below.

2.2 The Born–Oppenheimer adiabatic approximation The cores are much heavier than the electrons; for example, M ∼ 5 × 104 m for aluminum. At densities corresponding to typical solids, the cores behave like classical particles, but the electrons form a degenerate electron gas, leading to a difference of orders of magnitude in the kinetic energy of the two species. This difference in mass and kinetic energy implies that the cores are significantly more sluggish than the electrons; therefore the electrons can react almost instantaneously to any motion of the cores. For most systems, it can be assumed that the electrons feel the instantaneous potential produced by the cores in their “frozen” or “fixed” positions. Therefore, we define an electronic Hamiltonian for fixed cores, He =

p2 i

i

2m

+

n

1 e2 + HR , Vn (ri − Rn ) + 2 |ri − rj |

(2.2)

ij

and determine its energy spectrum Ele ({Rn }), where l labels the ith excited state which depends implicitly on the core positions {Rn }. In particular, with the electronic system in the ground state, the energy E0e ({R}) defines the potential Vec ({R}) within which the cores move. Remaining contributions of Eq. (2.1) can be assigned to the core part of the Hamiltonian, p2 1 Zn Zn e2 n + Vec ({Rn }). + (2.3) Hc = 2Mn 2 |Rn − Rn | n nn

The term Vec ({Rn }), which is E0e ({Rn }), represents an electron–core term which can be evaluated once Eq. (2.2) is solved and then used in Eq. (2.3) to determine the energy specturm for the cores. The procedure described above is the Born–Oppenheimer1 adiabatic approximation. It provides the important step of separating the electronic and core degrees of freedom. The electronic part (Eq. (2.2)) leads primarily to the determination of the properties of the electrons, holes, excitons, plasmons, and magnons. The core part (Eq. (2.3)) is used to describe the core motions and phonons. When the phonons are coupled to the electrons, including terms in Eq. (2.1) that go beyond Eqs. (2.2) and (2.3), one can examine polarons, superconductivity, resistivity, and other properties of solids. At this point, we restrict ourselves to the electronic Hamiltonian (Eq. (2.2)). 1 M. Born and J. R. Oppenheimer, “Zur Quantentheorie der Molekeln,” Ann. Physik 84(1927), 457.

2 Electrons in crystals

22

2.3 The mean-ﬁeld approximation Even though the Hamiltonian (Eq. (2.2)) does not include the cores as dynamical variables, it still contains a very large number of particles, namely, all the valence electrons in the solid. Another approximation is needed. The simplest commonly employed one is the Hartree2 mean-field approximation, which assumes that each electron moves in the average or mean field created by the cores together with all the other electrons. In the Hartree approach, one assumes that the electronic wavefunction of all the valence electrons is approximated by a product of one-electron wavefunctions, and each one is characterized by some one-electron spatial and spin quantum numbers. The effects of the Pauli exclusion principle are taken into account by requiring that no pairs of one-electron wavefunctions (orbitals) in the product have an identical set of quantum numbers. As discussed in standard quantum textbooks, demanding that the ground state has the lowest energy for the electronic system results in a set of self-consistent Euler–Lagrange equations (the Hartree equations) for the one-electron orbitals and energies with potential V(r, {Rn }). The Hartree mean-field approximation accomplishes the important task of separating the Hamiltonian (Eq. (2.2)) into a sum of one-electron Hamiltonians H(ri , {Rn }), (2.4) He = i

where

p2 (2.5) + V(r, {Rn }). 2m Another approach involves the Hartree–Fock approximations, which is also a meanfield approach for the electronic ground state. The Hartree–Fock method approximates the wavefunction by a determinant of one-electron orbitals, and thus automatically satisfies all the symmetry requirements of the Pauli principle. However, although more accurate, this approach has several complicating features which often make it inconvenient for many applications. Further discussion of this point appears in Chapter 6. H(r, {Rn }) =

2.4 The periodic potential approximation The potential V(r, {Rn }) of Eq. (2.5) is a one-electron potential that describes the forces acting on the electron labeled by the coordinate r. However, it depends on the one-electron states occupied by all the other electrons, a consequence of the Hartree approximation; it also depends parametrically on the “fixed” position of all the cores {Rn }. Even though the problem has been reduced to solving for the wavefunction of one electron at a time, this calculation must be accomplished self-consistently, since each electron state depends on the states of all the other electrons for an arbitrary core configuration. 2 D. R. Hartree, The Calculation of Atomic Structures (New York: Wiley, 1957).

23

2.5 Translational symmetry, periodicity, and lattices

Again, a straightforward calculation is extremely complicated and another approximation is needed. At this point, we rely on experiment which tells us that, in a crystalline solid, the cores form, to a very good approximation, an ordered periodic array. We thus take as a starting point a perfect crystal with core position {Rn } determined by X-ray crystallography or other means. We also assume at this stage that there are no defects or surfaces, and we assume, temporarily, an infinite number of atoms in the crystal. With {Rn } fixed, we may then write V(r, {Rn }) = V(r),

(2.6)

where V(r) has the symmetry of the periodic crystal arrangement. Because of the periodicity, an electron at point r experiences the same potential at all points r which are related to r through the periodicity and symmetry of the crystal. This potential V(r) now contains an enormous amount of information: the chemical composition of the crystal, the crystal structure and all its relevant parameters, the equilibrium positions of the cores, and the averaged potential acting on an electron produced by all the others. We have now arrived at the one-electron periodic potential model. The use of this model enables us to determine the spectrum of electrons and, with it, to answer approximately an amazingly large number of questions about the properties and behavior of electrons in solids at a mean-field level.

2.5 Translational symmetry, periodicity, and lattices The crystal potential V(r) describes the ideal crystal, that is, a collection of electrons and static cores in a perfectly periodic arrangement. Given an arbitrary point r in the crystal, there is an infinite array of points {r + Rn } such that, without change of orientation, the crystal appears exactly the same regardless of which point the arrangement is viewed from. This means that (2.7) V(r + Rn ) = V(r). This collection of all vectors {R} constitutes a set of discrete points which is called a Bravais lattice. In three dimensions, any periodic lattice {R} can be written as Rn = Rn1 n2 n3 = n1 a1 + n2 a2 + n3 a3 ,

(2.8)

where the three vectors ai are not coplanar, (a1 × a2 ) · a3 = 0,

(2.9)

and where n1 , n2 , n3 = 0, ±1, ±2, ±3, . . . Lattice vectors. The vectors Rn are called lattice vectors or translation vectors; the three vectors ai are called primitive lattice vectors or primitive translation vectors. The

24

2 Electrons in crystals

parallelepiped defined by the three primitive lattice vectors a1 , a2 , and a3 has a volume p given by p = |(a1 × a2 ) · a3 |,

(2.10)

and the lattice points in a Bravais lattice have a density (1/p ). Several important concepts follow. Primitive cell. A primitive cell is a region of space that, when translated by “all” the vectors in a Bravais lattice, exactly fills all of the space of the crystal without either voids or overlaps. Each primitive cell contains only one lattice point. The volume of a primitive cell is p , and the parallelepiped defined above is one possible kind of primitive cell. Although the volume of a primitive cell is constant and equal to p , its shape is largely arbitrary, and, in principle, it can consist of several disconnected parts. Unit cell. A unit cell is a region of space which, when translated by a subset of vectors of the Bravais lattice, exactly fills the space of the crystal with no voids or overlaps. Hence the volume of any unit cell u satisfies the condition u ≥ p . In fact, u = υp ,

v = 1, 2, 3, . . .

(2.11)

A primitive cell can now be redefined as a unit cell of minimum volume. Basis. A basis is the set of atoms and their coordinates within the unit cell which form the crystal. The basis for a primitive cell is smaller than the basis for a unit cell, and it is a minimal basis when related to a primitive cell. A basis must contain an integral number of the formula units that characterize the crystal. In more mathematical terms, a basis is given by a finite (and usually small) set of vectors {τ μ }, μ = 1, 2, . . . , Nb , where Nb is the number of atoms in the basis. Because the origin of a unit cell is arbitrary, two bases, which differ by a constant displacement, {τ μ } and {τ μ + τ 0 } for all μ, define the same crystal. Also, the change of any basis vector τ μ by a translation vector (τ μ + Rn ) yields a different basis and a different unit cell, but it still describes the same crystal. The most convenient way to define a crystal is to give its Bravais lattice and one primitive-cell basis. In some cases, to illustrate symmetries that are not obvious, the crystal is defined by a nonprimitive-cell basis and the corresponding subset of translation vectors. A two-dimensional example for a triangular crystal of formula AB2 is given in Fig. 2.1. Shown there are the Bravais lattice and a basis of three atoms. Wigner–Seitz cell. The Wigner–Seitz cell is a special primitive cell. It is built by drawing a line from the origin of the Bravais lattice to nearest-neighbor lattice points, and then constructing all the planes that bisect and are perpendicular to the lines, as illustrated in Fig. 2.2 for one and two dimensions. The smallest polyhedron that remains at the origin is the Wigner–Seitz cell. It is the most compact of all primitive cells and exhibits the maximum possible symmetry of the lattice. In the examples of Wigner–Seitz cells given in Fig. 2.2, (a) is a one-dimensional lattice, (b) is a two-dimensional square lattice, and (c) shows a two-dimensional hexagonal Wigner–Seitz cell for a triangular lattice. Reciprocal lattice. The reciprocal lattice is a mathematical construction of great importance in the study of the quantum mechanical properties of solids. Given a crystal and its

2.5 Translational symmetry, periodicity, and lattices

25

Figure 2.1

A two-dimensional lattice with a basis. The shaded circles represent diﬀerent atoms. (a)

(b)

Figure 2.2

(c)

(a) One-dimensional Wigner–Seitz cell. (b) and (c) Two-dimensional Wigner–Seitz cells.

Bravais lattice (Eq. (2.8)) defined by the three primitive translation vectors a1 , a2 , and a3 , we define a reciprocal lattice Gm ≡ m1 g1 + m2 g1 + m3 g3

(m1 , m2 , m3 = integers),

(2.12)

such that, for any translation vector Rn , Gm · Rn = 2π v

(v = integer)

(2.13)

for any m1 , m2 , m3 . It can easily be shown that gi = 2π

aj × ak , (a1 × a2 ) · a3

(2.14)

2 Electrons in crystals

26

where (i → j → k) = (1 → 2 → 3), in cyclic order, satisfies the requirements with v = n1 m1 + n2 m2 + n3 m3 . ˚ or Given the fact that the magnitude of ai is measured in units of length, typically A Bohr radii a0 , the magnitudes of the gi , |gi |, are measured in units of inverse length such as ˚ −1 or a−1 A 0 . This space of “inverse length” where we define the reciprocal lattice is called “reciprocal space.” Periodic functions. Any function u(r) that has the periodicity of the lattice u(r + Rn ) = u(r) can be expressed in a “discrete” Fourier expansion u(r) = bm eiGm ·r ,

(2.15)

(2.16)

m

where Gm are reciprocal lattice vectors as given by Eq. (2.12). Brillouin zone. Since the reciprocal lattice is a lattice, we may define unit cells and primitive cells for it in a manner similar to that was done for the real-space lattice. In particular, if we build a primitive cell following the same construction described for the Wigner–Seitz cell in the Bravais lattice, we obtain a polyhedron in reciprocal space. This important cell is called a Brillouin zone, and it is used extensively. Figure 2.2 can equally be used to represent one-dimensional and two-dimensional Brillouin zones, but the units are in inverse lengths, as described previously. For three dimensions, the Brillouin zone ˚ −3 or a−3 volume is usually measured in units of A 0 , and is given by BZ = |(g1 × g2 ) · g3 |.

(2.17)

The use of Eq. (2.14), some simple vector algebra, and Eq. (2.10) yields BZ =

8π 3 8π 3 = . |(a1 × a2 ) · a3 | p

(2.18)

A second and higher Brillouin zone can be defined by regions in space between the bisecting planes. These regions are mapped back into the first Brillouin zone by mapping reciprocal lattice vectors. The mapping is k → k − Gm .

(2.19)

This is shown for the square lattice and the construction of the higher Brillouin zones in Fig. 2.3. Periodic boundary conditions. All crystals, even the ideal, perfect ones, are finite. Their finiteness is essential for defining a crystal volume x , and the finiteness has important physical consequences. The presence of a crystal surface or boundary destroys the periodicity of the crystal, and many of the concepts defined above lose their meaning. This unsatisfactory situation is resolved with the aid of a mathematical device that in some sense makes the crystal finite and periodic. This is the concept of “periodic boundary

2.5 Translational symmetry, periodicity, and lattices

27

(a)

(b)

0 First BZ 5

6

1

12

7

0 2

3 4

4

2 1

8

11 10

3

Second BZ 9 7 12 10 5

9 8 11

6

Third BZ

Figure 2.3

(a) Construction of the two-dimensional Brillouin zones. (b) The ﬁrst, second, and third Brillouin zones in two dimensions.

conditions.” These conditions state that the crystal closes onto itself and that the last atom on the right is followed, without a loss of periodicity, by the first atom on the left. Similar conditions apply to other dimensions for an n-dimenional crystal. (This corresponds to replacing a line by a circle, a plane by a torus, and the whole crystal by a “super torus.”) The details of this approach will be dealt with later. For now, we eliminate finite crystal effects and consider a crystalline solid of volume x containing N primitive cells. Hence, for Ni primitive cells in the ai -direction (i = 1, 2, 3 in three dimensions), any translation of the form Rv1 N1 ,v2 N2 ,v3 N3 , where vi = integer, takes the crystal back into itself and leaves the crystal invariant. Therefore, there are N ≡ N1 · N2 · N3

(2.20)

primitive cells in the crystal, and the crystal volume is x = Np .

(2.21)

Bloch’s theorem. We now return to the one-electron-in-a-periodic-potential problem. The Hamiltonian (Eq. (2.5)) in the periodic potential approximation yields the Schr¨odinger equation h¯ H(r)ψ(r) ≡ − ∇ 2 + V(r) ψ(r) = Eψ(r), 2m

(2.22)

2 Electrons in crystals

28

where V(r) satisfies Eq. (2.7). Because of the periodic symmetry of the potential, the wavefunctions that satisfy Eq. (2.22) have distinct properties and are called Bloch3 wavefunctions. The theorem that states or illustrates the properties of Bloch wavefunctions is referred to as Bloch’s theorem or the Bloch condition. Three standard ways of stating Bloch’s theorem or the Bloch condition are described below. (1) The solutions of Eq. (2.22) can be expressed as a planewave eik·r times a function having the periodic symmetry of the lattice; hence, k (r) = uk (r)eik·r ,

(2.23)

uk (r + Rn ) = uk (r).

(2.24)

where The condition (Eq. (2.24)) is the same as that for the potential (Eq. (2.7)). At this point, the wavevector k is used as a quantum number to label the electronic state. Later we will show that energy levels group into bands. This is expected because of the existence of unit cells which confine electrons in the sense of Eq. (2.24). The bands will be indexed by the letter n. Hence, a specific state will be assigned the label (n, k), where n indicates the band and k specifies a particular state in that band. We suppress the band index n for now. (2) Bloch functions satisfy the periodic translational symmetry condition k (r + Rn ) = eik·Rn k (r).

(2.25)

This condition, which relates a lattice translation to a wavefunction phase factor, is very useful for illustrating the consequences of lattice periodicity on the wavefunction and matrix elements involving Bloch functions. (3) Since functions having the periodicity of the lattice can be expressed in a discrete Fourier sum (Eq. (2.16)), the periodic part of the Bloch function can be written as uk (r) =

bk (G)eiG·r .

(2.26)

G

This results in a useful and common form for the Bloch wavefunction ψk (r) = bk (G)ei(k+G)·r .

(2.27)

G

It is possible to use any of the three descriptions above to obtain the benefits of periodic translational symmetry via Bloch’s theorem. The above three statements describe the same physical properties. One-dimensional proofs of Bloch’s theorem, also called Floquet’s theorem, appear in most introductory texts on solids. Below we give a proof of Eq. (2.25). We begin by defining a set of translation operators {Tn } such that Tn f(r) = f(r + Rn ), 3 F. Bloch, “Uber die Quantenmechanik der Elektronen in Kristallgittern,” Z. Phys. 52(1928), 555.

(2.28)

2.5 Translational symmetry, periodicity, and lattices

29

where f(r) is an arbitrary function and n = (n1 , n2 , n3 ) is a set of integers (here we consider a three-dimensional crystal) where we have dropped the vector sign on n. Hence, Rn is defined as (2.29) Rn = n1 a1 + n2 a2 + n3 a3 . We can describe Tn as an operator that takes r → r = r − Rn and then relabel r = r, where r = (x, y, z) and r = (x , y , z ). If the operator Tn acts on the Hamiltonian H(r) given by Eq. (2.22), H(r) = −

h¯ 2 2 ∇ + V(r), 2m

(2.30)

it leaves H(r) invariant. This is obvious for the second term because of the periodic nature of the potential. To examine the action of Tn on the kinetic energy term, we first look at the x component of r, Tn

∂2 ∂2 ∂2 ∂2 f(r) = f(r ) = f(r + R ) = Tn f(r), n ∂x2 ∂x2 ∂x2 ∂x 2

(2.31)

and similarly for ∂ 2 /∂y2 and ∂ 2 /∂z2 . Therefore, Tn commutes with ∇ 2 and thus with H(r): [Tn , H(r)] = 0.

(2.32)

The action of two translation operators Tn and T on f(r) yields Tn T f(r) = f(r + Rn + R ) = T Tn f(r) = T+n f(r).

(2.33)

Therefore, {Tn } is a set of commuting operators that commute with H(r). Hence, we can diagonalize all Tn and H(r) simultaneously. Choosing θn to represent the eigenvalues corresponding to the action of the translation operator on an eigenfunction of Eq. (2.30), ψn (r), we have Tn ψn (r) = θn ψn (r).

(2.34)

θn θ = θn+ .

(2.35)

Using Eq. (2.33), we have We now break up the translation operator into components:

Tn ≡ T(n1 n2 n3 ) = Tna11 Tna22 Tna33

(2.36)

and θ(n1 n2 n3 ) = θan11 θan22 θan33 .

(2.37)

Since T is a translation operator and the electron wavefunction is normalized, θ can only be a complex number with unity absolute value. Letting θa1 = eiα1 ;

θa2 = eiα2 ;

θa3 = eiα3

(2.38)

2 Electrons in crystals

30

yields

θn = θ(n1 n2 n3 ) = ei(n1 α1 +n2 α2 +n3 α3 ) .

(2.39)

Since, from Eqs. (2.12)–(2.14), gi · Rn = 2π ni ,

(2.40)

θn = eik·Rn ,

(2.41)

we may write with k≡

α 1

2π

g1 +

α 2

2π

g2 +

α 3

2π

g3 .

(2.42)

We note here, since the αi ’s are defined only in the range 0 ≤ α ≤ 2π , that k is a vector in reciprocal space and may be taken to be confined to within the first Brillouin zone. We then can use k as a quantum number, labeling the eigenstates that simultaneously diagonalize H and all the Tn ’s. Equation (2.34) becomes Tn ψk (r) = eik·Rn ψk (r),

(2.43)

which gives one of the standard forms of Bloch’s theorem: ψ(r + Rn ) = eik·Rn ψk (r).

(2.44)

Arbitrariness of the k-vector and reduction to the Brillouin zone. Because of the properties of Bloch functions, we can write ik·r ik·r iG·r i(k−G0 )·r i(G+G0 )·r =e bk (G)e bk (G)e ψk (r) = e uk (r) = e i(k−G0 )·r

=e

G

iG ·r

bk (G − G0 )e

G i(k−G0 )·r

=e

(2.45)

uk−G0 (r) = ψk−G0 (r),

G

where G0 is any specific reciprocal lattice vector, G = G + G0 , and uk−G0 is a periodic function with properties similar to those of uk (r). Equation (2.45) states that both k and k − G0 are equally acceptable labels for describing the translational properties of ψ. In other words, any vector k in reciprocal space that differs from k by a reciprocal lattice vector G (Eqs. (2.12)–(2.14)) can be chosen to represent the “planewave” part of a Bloch function; the choice is arbitrary. Mathematically, this is because, in Eq. (2.44), (k − G0 ) · Rn = k · Rn − 2π ν, with ν an integer, and therefore the G0 term has no physical consequences. This indeterminacy is normally resolved by imposing extra conditions on k. The most common one is to require that the magnitude |k| of the k-vector is the smallest possible one. This condition restricts k uniquely to the interior of the Brillouin zone, and it leaves at most a small number of possible choices if k is on the Brillouin zone boundary. In this last case, the choice is left to the individual. For example, in one dimension where Gn = (2π/a)n, the label k is restricted to −(π/a) < k ≤ (π/a).

3

Electronic energy bands

In Chapter 2, the complex problem of calculating the properties of electrons in perfect crystals is reduced (through a series of approximations) to an investigation of a oneelectron Hamiltonian, which we now attempt to solve. Bloch’s theorem and symmetry considerations will be used to simplify the computation. At this point, the construction of the potential itself will not be described, and it will be assumed that a periodic potential consisting of electron–electron and electron–core contributions has been formulated. We begin by considering a free electron model to introduce the approach and to develop a framework for the discussion. After a description of some of the consequences of symmetry principles, a potential will be considered to demonstrate the existence of energy bands and energy bandgaps. Initially, the examples chosen will be one-dimensional. Most of the conclusions based on the one-dimensional cases are general, or at least suggestive of what can be expected for two and three dimensions.

3.1 Free electron model We first consider the one-electron Schr¨odinger equation

p2 + V(r) = E , 2m

(3.1)

with V(r) = V(r+R), and explore the case where V(r) is much less than the kinetic energy p2 /2m. The translational boundary conditions on the electronic wavefunction are enforced; that is, we still have Bloch waves, but beyond this, it is assumed that the potential has only a slight effect on the electrons. Let us begin by examining electrons in a one-dimensional box of length L, and as a first approximation to a weak potential, we set V(x) = 0. This is the free electron model or free electron gas. The Schr¨odinger equation is p2 0 = E0 (k) k0 , 2m k

(3.2)

and its solution is straightforward, consisting of planewaves k0 and energy E0 (k) for a given k, where 1 k0 = √ eikx L 31

(3.3)

3 Electronic energy bands

32

and E0 (k) =

h¯ 2 k2 . 2m

(3.4)

The wavevector k is not restricted, and k goes from −∞ to +∞, that is, no potential and no Brillouin zone. If we plot E0 (k), it has the form shown in Fig. 3.1(a). Plotting E0 (k) with no restriction on k is referred to as using the “extended zone scheme.” When the E0 (k) curve is mapped back into the first Brillouin zone, this is called the “reduced zone scheme.” The extended zone scheme is appropriate for free electrons, since the Brillouin zone has no real significance here because the lattice periodicity does not exist for this case. In the reduced zone scheme, the E0 (k) of the free electron model is mapped into the first Brillouin zone in anticipation of turning on the potential. The prescription for the mapping, based on the result of Eq. (2.45), is k = k −

2nπ , a

(3.5)

with n equal to an integer, or k = k − G.

(3.6)

This gives a mapping for k0 and E0 (k) as

2nπ . E0 (nk ) = E0 k + a

(3.7)

There is now another quantum number n in addition to k that is restricted to the first Brillouin zone. Figure 3.1(b) contains the dispersion curve or band structure (because of the appearance of “bands” of energy) for the free electron model when it is mapped into the first Brillouin zone. It will be shown presently that a periodic potential can introduce energy gaps between energy bands that are degenerate at the k-points, k = 0 and k = ±π/a. Before demonstrating this feature, we will assume that it is plausible and discuss the influence of some symmetry principles on the form of E0 (nk). E0

(a)

(b)

e

f c

– 3π a

Figure 3.1

–π a

e f

d a

b 0

π a

E0

3π a

k

d c a b –π 0 π a a

Energy bands for a free electron model. (a) Extended zone scheme. (b) Reduced zone scheme.

k

3.2 Symmetries and energy bands

33

3.2 Symmetries and energy bands We begin by discussing some general features of symmetry that are applicable in one, two, or three dimensions, and then focus on a few features of one-dimensional energy bands. Translational symmetry led to Bloch functions and Bloch’s theorem. If the Bloch form is assumed for the wavefunction (Eq. (2.23)) and inserted into the one-electron Hamiltonian (Eq. (2.22)), we arrive at the equation for the uk (r) part of the Bloch wavefunction

1 2 2 2 p + 2hk + V(r) un,k (r) = En (k)un,k (r) . · p + h k ¯ ¯ 2m

(3.8)

Since this is an eigenvalue problem with periodic boundary conditions, the eigenvalues take on discrete values labeled by n. Once the above equation is solved, the band structure En (k), giving the electronic energy for each state labeled by the band index n and wavevector k, is obtained. The full Bloch wavefunction nk can be constructed using the periodic part obtained from the solution of Eq. (3.8) using Eq. (2.23). The label n is the band index described earlier. A lattice can have other symmetries in addition to periodic translations. For example, it can be invariant to rotations through a specific angle. The group of rotations, reflections, and combinations of the two is called the point group. These are the symmetries obtained by keeping one point fixed, and like periodic translational symmetries, the point group symmetries can be exploited. (The point group operations together with translation symmetry operations form the space group of the crystal. For some crystals, there are also operations that involve point group operations plus a translation that is not a translation vector, leaving the system invariant. These are called nonsymmorphic operations.) In particular, it can be shown that the energy bands given by En (k) have the same symmetry as the crystal. To describe what this implies, consider the operator θ , which can be a rotation such that r = θ r.

(3.9)

En (k) = En (k ),

(3.10)

In order to show that

where k = θ k, we apply θ to the wave equation for uk (r) (Eq. (3.8)). Since scalar products are invariant under rotation, p2 = (θ p · θ p) = p2 ,

k2 = k2 ,

k · p = k · p .

(3.11)

Therefore,

1 2 2 2 p + 2hk ¯ · p + h¯ k + V(r) un,k (θ r) = En (k )un,k (θ r), 2m

(3.12)

3 Electronic energy bands

34

and unk (θ r) satisfies the same equation as unk (r). Hence, a situation similar to Eq. (2.44) exists, and a band index n can be chosen such that En (k ) = En (k),

where k = θ k.

(3.13)

Schematically, θ En (k) = En (k ), and En (k) possesses the full rotational symmetry of the crystal structure. Operationally, the translational symmetry is assured by the Brillouin zone scheme, and beyond this, En (k) is taken to have the space group symmetry. We consider inversion separately because its consequences are related to those of timereversal symmetry. All Bravais lattices (i.e. structures) without a basis have inversion symmetry. In some cases, inversion symmetry remains even after the inclusion of a basis. Using the above arguments, since V(r) = V(−r), then En (k) = En (−k). However, even without inversion symmetry, if the system being considered contains no magnetic fields and the forces are time-reversal invariant, such as the Coulomb force, it can be shown that En (↑ k) = En (↓ −k), where ↑ and ↓ denote spin configurations that are related by time reversal symmetry. The proof for the case without spin–orbit interaction comes from taking complex conjugates of both the wave equation and wavefunctions, and this is essentially equivalent to a time-reversal operation. Applying the complex conjugate operator to a Bloch function ∗ (r) = ei(−k)·r u∗n,k (r), n,k

the wave equation for Eq. (3.8) becomes 1 2 2 2 ∗ ∗ p − 2hk ¯ · p + h¯ k + V(r) unk (r) = En (k)unk (r). 2m

(3.14)

(3.15)

So u∗n,k (r) and un,k (r) satisfy the same equation if k is replaced by −k, and we can choose u∗n,−k = un,k

(3.16)

and En (↑ k) = En (↓ −k) by the same approach used before. This degeneracy is called the Kramers degeneracy. When discussing states and bands in the first Brillouin zone, there are some definitions that are commonly used. Degeneracy implies more than one state with the same k, and E. In cases where we consider n,k and n,k such that k = θ k and in the cases where we consider n,k and n,k+G , we do not call these states degenerate. In the latter case, the states are considered identical. Most degeneracies result from symmetries, while others are called accidental. The symmetry considerations discussed here can save considerable effort in computing energy bands. For example, if En (k) is needed throughout the Brillouin zone for a facecentered cubic lattice, the calculation need only be done in 1/48 of the Brillouin zone because of space group symmetry and the condition En (k) = En (−k). Other states in the full Brillouin zone are identical in energy to those in the 1/48 section and can be obtained by a mapping.

3.2 Symmetries and energy bands

35

3.2.1 Symmetries and energy bands in one dimension Several features of E(k) with k confined to the Brillouin zone defined by −π/a < k ≤ π/a are easily deduced from symmetry principles for a strictly one-dimensional crystal with lattice constant a. It is possible to show that (1) E(k) is non-degenerate; (2) E(k = 0) is a maximum or a minimum; (3) E(k) approaches k = ±π/a with zero slope; and (4) E(k) has a maximum or a minimum only at k = 0 and ±π/a for a lattice with a center of symmetry. E(k) is non-degenerate. For one dimension, the one-electron Schr¨odinger equation (3.1) is just an ordinary homogeneous linear differential equation, so there are at most two independent solutions (x) for a given energy E, which are labeled by the pair of quantum numbers nk. For a system without spin, time reversal and inversion both require E(k) = E(−k), but we exclude the k and −k pair of states from our definition of degeneracy. One-dimensional bands are therefore, non-degenerate and do not “overlap.” E(k = 0) is a maximum or a minimum. Since E(k) = E(−k), and assuming the derivative can be defined, then

E(δk) − E(−δk) dE(k)

= 0. = lim dk k=0 δk→0 2δk

(3.17)

Therefore, E(k) is a maximum or minimum at k = 0. E(k) approaches k = ± πa with zero slope. Translational symmetry requires that π 2π π π =E + δk . E − + δk = E − + δk + a a a a

(3.18)

Since from time-reversal symmetry, π π E + δk = E − − δk , a a then π π

E ± + δk − E ± − δk a a dE(k)

= 0. = lim

dk k=±π/a δk→0 2δk

(3.19)

So, E(k) is a maximum or minimum at k = ±π/a. E(k) has a maximum or minimum only at k = 0, ± πa . This means that the E(k) curve can have the form shown in Fig. 3.2(a) but not Fig. 3.2(b). If another maximum or minimum existed, then, as the figures show, we would have a situation where E(k1 ) = E(k2 ) with k1 = k2 . This condition would exceed the maximum number of degenerate solutions that the differential equation (3.1) could have. Because of the above restriction, one-dimensional conductors have hole or electron states only at k = 0 and k = ±π/a. The proofs given neglect the spin degree of freedom and assume inversion or timereversal symmetry, and that the system is not a one-dimensional structure embedded in three dimensions with internal symmetries. For example, if our system consists of an array of atoms with special symmetry properties, these would have to be considered.

3 Electronic energy bands

36

(a)

–

Figure 3.2

E

π a

0

π a

(b)

E

π a

0

k –

k1

k2

π a

k

(a) Possible one-dimensional E(k) with maxima and minima at k = 0, ±π/a. (b) One-dimensional E(k) with minima not at k = 0, ±π/a. This case is not allowed.

3.2.2 Energy bands and gaps: the Kronig–Penney model In the previous discussion, we anticipated the existence of separated energy bands and bandgaps. The gaps are regions of energy where electronic states do not exist; these gaps separate the states into bands. It is the interaction of the electrons with the periodic crystalline potential that gives rise to the bandgaps if we neglect strong electron correlation effects. There is a one-dimensional model of a periodic potential that is exactly solvable and demonstrates the existence of separated energy bands and bandgaps. This Kronig– Penney1 model can be solved easily, and it provides a good example of the consequences of a periodic potential. It is also a useful starting point for many other calculations; hence, it is often used instructionally and as a research tool. We begin by considering an infinite periodic array of δ-function potentials of integrated strength aV separated by a distance a. The potential can be written as V(x) = aV

∞

δ(x − na).

(3.20)

n=−∞

This potential represents the simplest periodic, one-dimensional model. Consider two adjacent regions (labeled 1 and 2) on either side of a δ-function that is placed at x = 0. In these regions, V = √ 0 and the eigenfunctions are linear combinations of planewaves with momentum hk ¯ 0 = 2mE, 1 or 2 = A1 or 2 eik0 x + B1 or 2 e−ik0 x ,

(3.21)

and the energy of the electron E is composed of the kinetic energy term only. Continuity of the wavefunction yields 1 (0− ) = 2 (0+ ),

(3.22)

A1 + B1 = A2 + B2 .

(3.23)

1 R. D. Kronig and W. G. Penney, “Quantum mechanics of electrons in crystal lattices”, Proc. R. Soc. Lond. A

130(1931), 499.

3.2 Symmetries and energy bands

37

Near x = 0, by integration of the Schr¨odinger equation, −

h¯ 2 (0+ ) − (0− ) + aV (0) = 0. 2m

(3.24)

This equation gives a discontinuous slope for the wavefunction that results from the singularities in the potential and yields the following condition: −

ih¯ 2 k0 (A1 − B1 − A2 + B2 ) + aV(A1 + B1 ) = 0. 2m

(3.25)

Also, Bloch’s theorem requires 2 (a) = eika 1 (0);

2 (a) = eika 1 (0).

(3.26)

Hence, A2 eik0 a + B2 e−ik0 a = eika (A1 + B1 )

(3.27)

A2 eik0 a − B2 e−ik0 a = eika (A1 − B1 ).

(3.28)

and

Simultaneous solution of Eqs. (3.23), (3.25), (3.27), and (3.28) gives cos ka = cos k0 a +

Vma2 sin k0 a . k0 a h¯ 2

(3.29)

The solution of Eq. (3.29) yields E(k), but since E(k) is not in an explicit form, the equation must be solved numerically or graphically. Before considering the solution, we will change notation. Let P=

Vma2 h¯

2

, K = ka, and α 2 = k20 a2 =

2mEa2 h¯ 2

.

(3.30)

The right- and left-hand sides of Eq. (3.29) become, respectively, f(α) ≡ cos α + P

sin α α

and g(K) ≡ cos K. Equation (3.29) is equivalent to f(α) = g(K).

(3.31)

We begin an analysis of Eq. (3.31) by considering a repulsive potential. The attractive potential case will be discussed later. For the repulsive case, P > 0, which means that the energy E > 0 and α 2 > 0. So α is real. We take α > 0 and solve Eq. (3.31) graphically.

3 Electronic energy bands

38

f (α)

f (α0) 1

α

π

2π

3π

4π

–1 n=1

Figure 3.3

n=2

n=3

n=4

n=5

Graphical solution of a Kronig–Penney model of δ-functions.

Since |g(K)| ≤ 1, the only values of α that satisfy Eq. (3.31) are those consistent with |f(α)|≤ 1. Graphically, this can be solved as shown in Fig. 3.3. The acceptable α’s are given by the shaded regions; the rest are forbidden. For a given k, there exists an infinite set of solutions for f(α) given by the intersection of the value cos K and f(α). As α → ∞, the forbidden regions get smaller, then f(α) → cos α, K → α, and k → k0 . This means that, as expected, the potential has less of an effect on the particle as the energy of the particle becomes very large. The regions containing acceptable values for α can be labeled by a band index n. Using the expression α 2 = 2mEa2 /h¯ 2 , the acceptable values for α(k) yield separate acceptable values for E(k), and hence we have demonstrated the existence of energy bands. Symmetry properties are preserved. Since cos K = cos(−K), then α(k) = α(−k) and En (k) = En (−k); also, the solution for cos(K + 2nπ ) is the same as the solution for cos K, and we need only take −π < K ≤ π or π/a < k ≤ π/a. This is just the first Brillouin zone. If we solved for α(k) or E(k), we would get energy bands that are consistent with the restrictions discussed earlier for a one-dimensional E(k). A schematic E(k) curve for the first three bands of the Kronig–Penney model is given in Fig. 3.4. The first band has its lowest energy at E(k = 0) = E0 , a constant that depends on the value of the potential. At the Brillouin zone edge, ka = π , α = π , and E(k) = h¯ 2 π 2 /2ma2 , which is the free electron value for this value of k. In fact, for this model, the Kronig–Penney energy reduces to the free electron value at k = nπ at the top of a band, since the potential term in Eq. (3.31) is inoperative at these points. The nth gap, therefore, starts at ka = nπ and f(nπ ) = (−1)n . Using this fact, it is possible to find the size of the gap for large n when the potential energy is small compared to the kinetic energy, that is, for a “nearly-free electron” system. Suppose the nth gap starts at α = nπ and ends at α = nπ + α, where α is small. Using Eq. (3.31) and the fact

3.3 Nearly-free electron model

39

E 9ħ2π 2 / (2ma2)

4ħ2π 2 / (2ma2)

ħ2π 2 / (2ma2)

π – a

Figure 3.4

π a

Wavevector k

E0

Schematic E(k) for the Kronig–Penney model. that f does not change much with the small variation in α, we have (−1)n = cos(nπ + α) + P

sin(nπ + α) . (nπ + α)

(3.32)

Expanding, we get α =

2P , nπ

(3.33)

and the energy gap becomes E = E(nπ + α) − E(nπ ) =

2h¯ 2 P = 2V. ma2

(3.34)

This is a well-known result for the bandgap Eg for a nearly-free electron; however, it is usually obtained using perturbation theory on a free electron model, as will be shown next.

3.3 Nearly-free electron model The model of electrons interacting with a weak potential is an excellent one for representing the electronic structure of many solids. In many metals, the electrons can be considered as almost free, so their energies and wavefunctions are not expected to differ much from the results obtained for a free electron model (FEM). The standard approach is to use perturbation theory on the FEM to obtain results for the nearly-free electron model (NFEM) rather than using the Kronig–Penney method. Because of the appropriateness of the model for real systems, the model also illustrates many of the general features of band structures. Since the extension of the FEM and the NFEM to the three-dimensional case is straightforward with no fundamental complication, we proceed directly to three dimensions.

3 Electronic energy bands

40

Letting V(r) = 0 (but weak), we can obtain E(k) via standard perturbation theory. This gives to second order E(k) = E0 (k) + Vkk +

|Vk k |2 , E0 (k) − E0 (k )

k=k

(3.35)

with Vk k =

1 x

ei(k−k )·r V(r)dr

(3.36)

V(r)dr = V0 ,

(3.37)

and Vkk =

1 x

where E0 (k) is the FEM energy, x is the crystal volume, which for convenience can be set to unity, V0 is the average potential, and the Vkk are matrix elements of the potential eik·r . The constant V0 shifts all the between FEM states k0 and k0 , where k0 (r) = √ x energies irrespective of their k-values; hence, it is used just to set the zero of energy. Since V(r) is periodic with lattice periodicity, it can be expanded in the reciprocal lattice V(r) =

V(G)eiG·r ,

(3.38)

e−iG·r V(r)dr.

(3.39)

G

where (with x = 1) V(G) =

This expansion simplifies the expression for Vkk , that is, Vk k =

V(G)

ei(k−k +G)·r dr =

G

V(G)δk ,k+G .

(3.40)

G

The energy becomes E(k) = E0 (k) + V0 +

G=0

|V(G)|2 . E0 (k) − E0 (k + G)

(3.41)

The “second-order” term is usually small, since for most k’s it is essentially the square of the potential energy divided by the kinetic energy difference. The whole scheme breaks down when E0 (k) = E0 (k+G). At these k-points, we need degenerate perturbation theory. We note that at these k-points, 2k · G + G2 = 0,

(3.42)

3.3 Nearly-free electron model

41

which is the famous Bragg condition used in X-ray scattering from crystals. It is also the condition that determines the Brillouin zone boundary. For example, in one dimension, ±2π + 2k a

2π a

2 = 0.

Hence, k=

±π , a

(3.43)

which are the edges of the Brillouin zone. Hence, the unperturbed energies are degenerate at the Brillouin zone boundaries, and degenerate perturbation theory is required to solve the Schr¨odinger equation for k-points near these boundaries. This is done by considering the wavefunction to be a linear combination of the zero-order degenerate states. In one dimension, only one G is involved. We therefore have 0 k = a k0 + b k+G

and p2 + V(r) k = E k . H k = 2m

(3.44)

0 , we get Taking matrix elements of the Hamiltonian between k0 and k+G

aHkk + bHk,k+G = Ea

(3.45)

and aHk+G,k + bHk+G,k+G = Eb, where Hkk = [E0 (k) + V0 ]δkk + Vkk . Since

(3.46)

Vk,k+G = V∗k+G,k = V(−G)

and E0 (k) = E0 (k + G),

(3.47)

solving for Eq. (3.44), we have E(k) = E0 (k) + V0 ±

V(G) 2 .

(3.48)

3 Electronic energy bands

42

(a)

π – a

Figure 3.5

(b)

E

π a

k

E

π – a

π a

k

Nearly-free electron model. (a) Extended zone scheme. (b) Reduced zone scheme. Setting V0 = 0, we have E(k) = E0 (k) ± |V(G)|.

(3.49)

The degenerate levels are split by 2|V(G)|. A similar result was obtained earlier for the higher gaps in the Kronig–Penney model. For one dimension in the extended zone scheme, the E(k) curve is essentially a parabola with gaps at k = ±nπ/a, as shown in Fig. 3.5(a). In the reduced zone, we have the situation shown in Fig. 3.5(b). If we calculate the wavefunctions near one of these gaps, the existence of the gap can be understood on physical grounds. The solutions for a and b (assuming an attractive potential) are for the lower state 1 a=b= √ 2 and for the upper state 1 a = −b = √ , 2

(3.50)

which give 1 1 ∝ cos Gx 2 and 1 2 ∝ sin Gx. 2

(3.51)

The electronic density | 1 |2 is peaked at the lattice points, while | 2 |2 is peaked between the lattice points. For an attractive potential, the | 1 |2 charge distribution lies lower in

43

3.4 Tight-binding model

energy than that corresponding to | 2 |2 , and the energy difference is 2|V(G)|. Behavior of this kind is expected near bandgaps. In summary, the NFEM yields energy bands, which are almost identical to those of the FEM, except near zone edges. In the NFEM, energy gaps appear, and these can be extremely important in determining the electronic properties of the system.

3.4 Tight-binding model At the other limit relative to the NFEM is the tight-binding model (TBM). This approximation is most appropriate for solids in which the constituent atoms resemble slightly perturbed free atoms. Whereas the NFEM starts with completely free electrons perturbed by a weak potential, the TBM begins with atomic-like states and perturbs them with a potential due to interaction with nearby atoms. The NFEM is appropriate for close-packed solids in which the overlap between electrons from adjacent atoms is large. Hence, metals are particularly suited to this type of analysis. The TBM is more appropriate for wide gap insulators where the overlap between adjacent atoms is small and atomic separations are large. Semiconductors tend to fall in between, and for these cases, both methods have been used. It is possible to begin with the Kronig–Penney model to gain insight into the TBM. For example, consider a situation in which the above Kronig–Penney potential is appropriate for atomic-like systems where the starting point is a set of bound states. For the repulsive potential case considered earlier, it is not possible to get a bound state. This can be seen by examining the Kronig–Penney equation, assuming a bound state with E < 0. The condition E < 0 implies that α is imaginary. Assuming α = iφ, we have cos K = cosh φ +

P sinh φ . φ

(3.52)

This can be solved only if we consider an attractive potential. Now P (Eq. (3.30)) is negative, and one has the possibility that E can be negative. Equation (3.52) can be written as cos K = cosh φ − |P|

sinh φ . φ

(3.53)

This is easily solvable if |φ| 1. Expanding, we find |P| eφ 1− . (3.54) cos K = 2 φ ∼ 0 (or φ = |P| + δφ). Equation Since |cos K| ≤ 1 and eφ is large, we need 1 − |P| φ (3.54) becomes (to lowest order) cos K =

1 |P| δφ δφ |P| e = e 2 φ 2|P|

(3.55)

3 Electronic energy bands

44

and δφ = 2|P|e−|P| cos K.

(3.56)

We can find the energy by using E=−

h¯ 2 φ 2 h¯ 2 |P|2 −|P| 1 + 4e = − cos K + · · · 2ma2 2ma2

(3.57)

−|V|ma2 1 + 4 exp cos ka + · · · . h¯ 2

(3.58)

or E=−

mV2 a2 2h¯ 2

The first term is negative, and it represents the energy of a bound-state in a one-dimensional well; hence, we have bound-state solutions. For large a, the potential wells (negative delta functions in our case) are separated, and N independent potentials give N independent bound states. As a gets smaller, the wells interact, and the level spreads. This spread is given by the second term in Eq. (3.58). The total spread E has the form E =

4mV2 a2 h¯ 2

exp

−|V|ma2 h¯ 2

=

4mV2 a2 h¯ 2

e−a/ ,

(3.59)

2

h¯ is the radius of the bound-state and the spread is small until a ∼ , where ≡ |V|ma electron. The above calculation is similar to a “tight-binding-type calculation.” If atoms are isolated, the energy levels are sharp. As the distance between the atoms gets smaller, the tails of the exponential bound-state wavefunctions “feel” each other and interact. This causes the energy levels to spread out into bands of levels. Summarizing, in the Kronig–Penney model, we are able to find a bound state for a negative potential, and, for N isolated delta functions, this state is N-fold degenerate. As the delta functions are brought closer together, they begin to interact, and the states spread in energy (Fig. 3.6) according to the expression

E = E0 + 4E0 e−a/ cos ka + · · ·

(3.60)

The delta function potentials interact when a ∼ , that is, when the distance between the potentials is of the order of the radius of the bound-state wavefunction. If we now extend this idea to a collection of atoms, we expect the free atom levels to spread as the distance between atoms decreases (Fig. 3.7). The spreading can be so large that the bands corresponding to different levels can overlap. For the case where the overlap is small, the spreading is small, and we expect the wavefunctions to be similar to those in the atomic case. It is then reasonable to expect atomic states to form a good basis set for representing the wavefunctions describing the solid. It is also reasonable to expect the crystal potential to look like a superposition of atomic potentials Va (r − R − τ a ) about

3.4 Tight-binding model

45

One sharp N-fold degenerate level

A band of energy levels N-fold degenerate

0 Inverse lattice constant 1/a

Figure 3.6

Spreading of one N-fold degenerate δ-function level into a band as a function of the inverse of the lattice constant using the Kronig–Penney model.

Energy

Degenerate free atom states

0 Inverse lattice constant 1/a

Figure 3.7

Spreading of atomic levels into bands as the lattice constant a decreases.

the lattice points R and basis vector τ a , i.e. V(r) =

Va (r − Rl − τ a ),

(3.61)

,a

where a labels the basis atoms. The atomic wavefunctions satisfy the equation

p2 + Va (r) φta = Eta φta , 2m

(3.62)

with t labeling the atomic states. We may now form the so-called linear combination of atomic orbitals (LCAOs) to serve as basis functions to expand the electronic states in a

3 Electronic energy bands

46

crystal. An LCAO φkta (r) is defined as 1 ik·Rn e φta (r − Rn − τ a ), φkta (r) ≡ √ N n

(3.63)

where N is the number of unit cells. The phase factor eik·Rn is to ensure that φkta is of the Bloch form. Let r → r+Rm , then 1 ik·Rn φkta (r + Rm ) = √ e φta [r − (Rn − Rm ) − τ a ] . N n

(3.64)

Relabeling R = Rn − Rm , 1 ik·R ik·Rm φkta (r + Rm ) = √ e e φta (r − R − τ a ) N =

(3.65)

eik·Rm φkta (r),

showing that φkta (r) is a Bloch function. For a crystal with weakly interacting atoms, the crystalline electron wavefunctions k (r) can be expanded to a good approximation in terms of the LCAOs. That is, αta (k)φkta (r). (3.66) k (r) = ta

We note that only LCAOs with the same k enter into Eq. (3.66). This is because, from Bloch’s theorem, k is a good quantum number and electronic states do not mix Bloch functions of different k’s, which is a basic consequence of translational symmetry of a crystal. With the form of the wavefunction in Eq. (3.66), the Schr¨odinger equation (H k = E(k) k ) may be written in the form of a generalized matrix eigenvalue equation: ⎛ ⎛ ⎞ ⎞ α1 (k) α1 (k) ⎛ ⎞⎜ ⎜ . ⎟ . ⎟ ⎜ ⎜ ⎟ ⎟ ⎜ ⎜ ⎟ ⎟ ⎝Hij (k)⎠ ⎜ (3.67) . ⎟ = E(k)Sij ⎜ . ⎟, ⎜ ⎜ ⎟ ⎟ ⎝ ⎝ . ⎠ . ⎠ αM (k) αM (k) where (i, j) run over the indices (ta). That is, M in Eq. (3.67), which is equal to the dimension of the matrices H and S, is equal to the sum of the number of relevant atomic states on all of the atoms in the unit cell. The elements of the Hamiltonian matrix H and the overlap matrix S are given by j (3.68) Hij (k) = φki H φk and

j Sij (k) = φki φk .

(3.69)

3.4 Tight-binding model

47

Solutions of Eq. (3.67) lead to a band structure with M bands within this formalism. As a simplest possible illustration, let us consider the case of a crystal with one atom per unit cell; on each atom there is only one relevant atomic state of interest. In this case, M = 1 with

H11 (k) = φk1 (r) H φk1 (r) (3.70) 1 ik·(Rn −Rm ) = e φ1∗ (r − Rm )H(r)φ1 (r − Rn )d3 r. N n,m x Using the factor that H(r) is invariant with respect to a translation vector, we may rewrite Eq. (3.70) (by defining Rp = Rn − Rm ) as 1 ik·Rp e φ1∗ (r)H(r)φ1 (r − Rp )d3 r H11 = N p,m x (3.71) eik·Rp h11 (Rp ). = p

Here we have denoted h11 (Rp ) =

x

φ1∗ (r)H(r)φ1 (r − Rp )d3 r,

(3.72)

which is often called the hopping integral, and we use the fact that the summation over m gives rise to a factor of N. Similarly, eik·Rp φ1∗ (r)φ(r − Rp ) d3 r S11 (k) = x

p

=

ik·Rp

e

(3.73)

s11 (Rp ).

p

The solution to the 1 × 1 matrix eigenvalue problem in Eq. (3.67) becomes (for this simple case) E(k) =

H11 (k) S11 (k) ik·R e p h11 (Rp ) p

= p

eik·Rp s11 (Rp )

(3.74) .

This solution may be transformed to a more intuitive form by dividing H into the atomic part Ha plus the part due to the rest of the crystal H1 = H − Ha . Then Eq. (3.74) becomes

ik·Rp h1 (R ) p pe 11 . ik·R p s11 (Rp ) pe

E(k) = Ea +

(3.75)

3 Electronic energy bands

48

E

Ea

π a

Figure 3.8

k

Schematic E(k) in the kx direction for a tight-binding band for a simple cubic lattice with a single s-orbital on each site.

The first term is the energy of the atomic state, and the second term contains h111 (Rp ), which is negligibly small for p = 0. As an example, consider a simple cubic lattice with only nearest-neighbor interactions. The lattice vectors are (a, 0, 0), (0, a, 0), and (0, 0, a). Assuming the same matrix elements for the six nearest-neighbor sites (which is appropriate for s-like orbitals),

E(k) = Ea + 2h(a, 0, 0) cos kx a + cos ky a + cos kz a .

(3.76)

This result is similar to the Kronig–Penney result in Eq. (3.60). If h(a, 0, 0) is negative, the minimum energy for the simple cubic lattice is Ea + 6h(a, 0, 0), and the width of the band is 12|h(a, 0, 0)|. (See Fig. 3.8 for a schematic example.) The tight-binding method is useful to illustrate how atomic states broaden into bands. It can be used for accurate band calculations in cases where the overlap between neighboring atoms is small and the bands are narrow. This method becomes more accurate as the number of atomic orbits on each atom and further-neighbor interactions are included. The TBM has been exploited with success in calculations on molecules and solids.

3.5 Electron (or hole) velocity in a band and the f-sum rule Once the band structure for a crystal has been computed and the En (k) curve is known, it is possible to evaluate the velocity of an electron (or hole) and the effective mass m∗ characterizing the electron or hole in a band state. In addition, if the energies of the states are known at one k-point, the band structure at neighboring points can be obtained. In the following discussion, these features are derived, as is the f-sum rule which connects the effective mass, bandgaps, and momentum matrix elements.

3.5 Electron (or hole) velocity in a band and the f-sum rule

49

For simplicity, let us consider non-degenerate energy levels. We know the energy levels at a particular k-point; that is, we know En (k0 ) for all n. (The discussion may be generalized to degenerate states.) From this information, we can determine the energy at a neighboring k-point k , where k = k0 + k.

(3.77)

Consider the wave equation for the periodic part of the Bloch function at k : (p + hk ¯ )2 + V(r) unk (r) = En (k )unk (r), 2m

(3.78)

then

2 (p + hk hk ¯ 0 )2 ¯ · (p + h¯ k0 ) h¯ k2 + V(r) + + unk (r) = En (k )unk (r). 2m m 2m

(3.79)

The first two terms on the left-hand side give the energy levels at k0 , and the last term is a number that is second order in k. The third term, which we shall call H , can be used as a perturbation if k is small. When this term is used in this way, the method is called “k · p perturbation theory.” To second order in k, we have

| un k0 H unk0 |2 h¯ 2 k2 + En (k0 ) + unk0 H unk0 + , (3.80) En (k0 + k) = 2m En (k0 ) − En (k0 ) n=n

where the u’s are orthonormal since they are solutions to H(k0 ). Another way to obtain En (k ) to second order is to expand around k0 in a Taylor series, En (k0 + k) = En (k0 ) +

3 ∂En (k0 ) i=1

∂koi

3 1 ∂ 2 En (k0 ) ki + ki kj . 2 ∂koi ∂koj

(3.81)

i,j=1

By equating terms of the same order in Eqs. (3.80) and (3.81), we obtain the desired relations. The first-order terms yield

h¯ ∂En (k0 ) unk0 pi + h¯ koi unk0 = ∂koi m h¯ = nk0 | pi |nk0 , m where we have used the Dirac notation for the full Bloch state and the relation

nk0 | pi |nk0 = unk0 pi + hk ¯ oi unk0 .

(3.82)

(3.83)

This result allows a calculation of the velocity in the direction i for an electron in the state (n, k0 ), using vi,n,k0 =

1 ∂En (ko ) . h¯ ∂koi

(3.84)

3 Electronic energy bands

50

Equating second-order terms yields the f-sum rule ij m = δij + fnn , (mn )ij

(3.85)

n =n

where the effective mass is defined as 1 1 ∂ 2 En (k) ≡ 2 , (mn )ij h¯ ∂ki ∂kj

(3.86)

ij

and fnn is the oscillator strength which is related to matrix elements between Bloch states of the momentum operator

1 n k0 pi |nk0 nk0 | pj n k0 + n k0 pj |nk0 nk0 | pi n k0 ij . (3.87) fnn = m En (k0 ) − En (k0 ) We shall further discuss the meaning of the effective mass in Chapter 5. The main features of the f-sum rule can be illustrated by considering a model of a semiconductor with just two bands separated by a gap Eg . For simplicity, we assume constant momentum matrix elements |p| and spherical bands, and investigate how the effective mass of each band depends on the gap by considering Eq. (3.85), using these approximations to obtain 2 2 |p|2 m =1+ . m∗n m En − En

(3.88)

n =n

For band 2, which would be the conduction band of the semiconductor (as seen in Fig. 3.9), m 2 |p|2 2 |p|2 =1+ =1+ . ∗ m2 m E2 − E1 m Eg

(3.89)

Hence, m∗2 > 0 and, if Eg is small, m∗2 m. For band 1, the valence band, 2 |p|2 2 |p|2 m = 1 + = 1 − , m∗1 m E1 − E2 m Eg

(3.90)

and m∗1 < 0, since the absolute value of the second term is usually greater than unity. If Eg is very small, such that the second term on the right sides of Eqs. (3.89) and (3.90) dominates, then |m∗1 | = |m∗2 |. This model gives the main dependence of the effective masses on bandgaps, i.e. small gaps imply small masses. There are applications of the f-sum rule to interpret optical properties, since the momentum matrix elements can be related to optical transition probabilities. Next, we return to the example of the Kronig–Penney model and examine the velocities and effective masses. Consider the repulsive potential case and the calculations of the electron effective mass and velocity near k = 0 and k = π/a. For the first band (Fig. 3.4), E(k = 0) ≡ E0 , which is a constant depending on the potential. At k = πa ,

3.5 Electron (or hole) velocity in a band and the f-sum rule

51

E

2

Eg k

1

Figure 3.9

Two bands separated by a gap Eg (the two-band model). E1 = π 2 h¯ 2 /2ma2 , which is independent of the potential. Let us begin with k = 0, and letting α0 ≡ α(k = 0), we expand Eq. (3.31) about this point in a Taylor series 1 1 − K2 = f(α0 ) + f (α0 )(α − α0 ). 2

(3.91)

Since f(α0 ) = 1, this gives α = α0 −

1 K2 . 2 f (α0 )

(3.92)

The energy E can now be expressed in terms of α: h¯ 2 α 2 h¯ 2 1 K2 2 E= α0 − = 2ma2 2ma2 2 f (α0 ) =

h¯ 2 α02 h¯ 2 α0 2 k . − 2ma2 2mf (α0 )

(3.93)

If we now express E using an effective mass, we have E = E0 +

h¯ 2 2 k 2m∗

(3.94)

and

m∗

f (α0 ) =− .

m k→0 α0

(3.95)

As shown in Fig. 3.3, the slope of f(α0 ), f (α0 ) is negative. This means that m∗ > 0. As P increases, f(0) = 1 + P gets larger, and the slope at f(α0 ) is larger. Hence, large P means that m∗ is large, i.e. when the potential is stronger, the band is flatter.

3 Electronic energy bands

52

We can also compute v(k = 0) using v=

1 ∂E ∂α ∂K . h¯ ∂α ∂K ∂k

(3.96)

Now,

for small K. Since E =

∂α

−K sin K = =− ∂K α→α0 f (α0 ) f (α0 )

(3.97)

−hα ¯ 0 k

v= . mf (α0 ) k→0

(3.98)

h¯ 2 α 2 , 2ma2

We obtain this same result if we use Eq. (3.95) and the expression for the velocity v = ∗ . Similarly, for the top of the first band, hk/m ¯

m∗

f (π ) −P = (3.99) = 2.

m k→π/a π π Since f (π ) is negative, m∗ is negative. If P is large, again f (π ) is large and m∗ is large. If P is small, the gap to the next band is small, and f(α) must have a smaller slope; that is, the turning point of f(α) is closer to the −1 line. This is consistent with the statement that near a small bandgap the masses are small. The velocity at k = π/a can also be computed. Near K = π −K, f(α) = cos(π −K), where K → 0 and K ∂α = , ∂K f (π )

(3.100)

h¯ π 2 K

. v= mPa k=π/a−K/a

(3.101)

yielding

3.6 Periodic boundary conditions and summing over band states In the previous sections, En (k) was examined in general and for specific models in various limits. At this point, we assume that En (k) is known and explore the problem of using this function in evaluating properties such as response functions, densities of states, etc. Calculations of this type can involve sums or integrals over states. Because crystals have a finite size, the states associated with the electronic or vibrational properties (to be discussed in the next chapter) do not have a continuous range but are characterized by discrete wavevectors. As discussed in Chapter 2, periodic boundary conditions (PBCs) can be imposed as

3.6 Periodic boundary conditions and summing over band states

53

(a)

Real space

(b) –

a

Reciprocal space

π a

2π Na

0

π a

Na

Figure 3.10

(a) One-dimensional crystal of length Na. (b) Representative cell in k-space arising from ﬁnite sample size through PBCs.

a convenient method to account for finite crystal size. This approach leads to a straightforward method for counting states and for doing sums and integrals over k-states in the Brillouin zone. In one dimension, PBCs imply that for a crystal of N cells of lattice constant a, (x + Na) = (x).

(3.102)

It is as if the one-dimensional line were joined into a circle. If we next use the Bloch condition, then (x + Na) = eikNa (x), and therefore, eikNa = 1.

(3.103)

This gives the following condition for the allowed k-states: k=

2π n Na

(n = 0, ±1, ±2, . . . ).

(3.104)

For one dimension, the Brillouin zone is defined by −

G G 0.

(4.6)

4 Lattice vibrations and phonons

64

Using a Taylor series expansion about the equilibrium positions, U = U0 +

1 ∂ 2U α α ξn ξn + · · · , α α 2 n,α ∂ξn ∂ξn

(4.7)

n ,α

where α, α = x, y, z, and n, n = (, j) is the site index. If we let U0 = 0 and truncate the series after second order in the so-called harmonic approximation, then U=

1 αα α α A ξ ξ . 2 n,α nn n n

(4.8)

n ,α

From the equation of motion, P˙ n = −∇ ξ n U,

(4.9)

we have Mn ξ¨nα = −

n α

α Aαα nn ξn .

(4.10)

Hence, Aαα nn is the atomic force constant in the α direction on the nth atom when the n th atom is displaced in the α direction. In the harmonic approximation (i.e. terminating Eq. (4.7) in second order of the displacements), we may think of the crystal as a collection of atoms connected by springs and the A’s as the spring constants. The atomic force constant matrix A has some useful symmetry properties. It can be shown that A is a symmetric matrix, it depends only on R − R owing to crystalline periodicity, and it also has the group symmetry properties of the crystal. We can now explore the normal modes of vibration. In a mechanical system, the number of degrees of freedom = d×r×N, where d is the number of dimensions, r is the number of basis atoms, and N is the number of unit cells. To solve for the normal modes, we look for solutions in which each atom of mass Mj is moving periodically with the same frequency ω,

1 ξjα (t) = Cαj e−iωt , Mj

(4.11)

where C is the amplitude of vibration. Using the equation of motion (Eq. (4.10)), we obtain α ω2 Cαj = Dαα (4.12) jj (R − R )C j , j α

where

Dαα jj (R

Aαα jj (R − R ) − R ) = Mj Mj

(4.13)

4.1 Lattice vibrations

65

is a real drN×drN symmetric matrix. Thus, there exist drN real eigenvalues ωi2 . Physically, ω2 should be positive. However, if for some reason a particular mode has ωi → 0, it would suggest a possible structural phase transition, since this indicates a vanishing restoring face for distortions given by this mode. Analogous to the electron case, using periodic translation symmetry, we seek solutions in Bloch form. For a given q, Cαj = Cαj eiq·(R +τ j ) . 0

(4.14)

Equation (4.12) becomes ω2 Cαj

=

j α

−iq·(τ j −τ j )

e

Dαα jj (R

−iq·(R0 −R0 )

Cαj .

− R )e

!

(4.15)

"

Dαα (q) jj

Equation (4.15) is a set of d × r coupled equations. The matrix Dαα jj (q) is called the dynamical matrix. We arrive at ω2 Cαj =

j α

α Dαα jj (q)Cj .

(4.16)

This is an rd × rd matrix eigenvalue problem. Hence, lattice periodicity reduces our initial system of drN equations to a system of rd equations. We arrive at the solutions ωλ (q), where λ = 1, . . . , rd (the number of phonon branches) with q in the first Brillouin zone, where there are N q-points allowed, as discussed in the previous chapter. As an example, let us reexamine the familiar model of a one-dimensional chain of atoms with a one-atom basis (Fig. 4.1) and nearest-neighbor connecting springs with force constant γ . The solution to this model1 for a simple spring model derivation is ω2 (q) =

qa 2γ 4γ sin2 = (1 − cos qa), M 2 M

1 C. Kittel, Introduction to Solid State Physics, 8th ed. (New York: Wiley, 2005).

M

a (艎–1)th unit cell

Figure 4.1

Monatomic chain of atoms connected by springs.

艎th unit cell

(艎+1)th unit cell

(4.17)

4 Lattice vibrations and phonons

66

ω

ωmax

ω ∝ vsq π a

Figure 4.2

q

Acoustic phonon band structure for a monatomic chain of atoms. which is shown in Fig. 4.2. We can explore this example using the dynamical matrix D =

$ γ # A = −δ −,−1 − δ −,1 + 2δ− ,0 , M M

(4.18)

where δ’s are Kronecker delta functions and, as in Eq. (4.13), D = D( − ).

(4.19)

The Fourier transform of Eq. (4.18) gives D(q) = D( − )e−iq·(R −R )

& % γ − (δ −,−1 + δ −,1 − 2δ− ,0 ) × e−iqa(− ) = M

(4.20)

=−

γ −iqa 2γ (e (1 − cos qa). + eiqa − 2) = M M

Then, from Eq. (4.16), ω2 C = D(q)C,

(4.21)

which yields ω2 =

2γ (1 − cos qa). M

(4.22)

Hence, we obtain the same result as is found for the simple solution to the spring model using Newton’s law.

4.1 Lattice vibrations

67

M1

M2 a b = 2a 艎th unit cell

(艎–1)th unit cell

Figure 4.3

(艎+1)th unit cell

Diatomic chain of atoms connected by springs.

We note that ω = ωmax when qa = π , i.e. q = π/a, which is the Brillouin zone √ boundary, and therefore ωmax = 2 γ /M. The saturation of the dispersion curve results from the discreteness of the atomic arrangement in the solid, and q is only meaningful inside the first Brillouin zone. If we examine the long wavelength limit, then lim ω2 =

q→0

2γ 1 (qa)2 . M 2

(4.23)

Therefore, ' ω(q → 0) =

γ aq = vs q, M

(4.24)

γ a M

(4.25)

where ' vs =

represents the sound velocity. Another example that is useful to explore is a one-dimensional diatomic chain (Fig. 4.3). The dynamical matrix Djj (q) is a 2 × 2 matrix in this case. From Eq. (4.13), we find that 2γ δ −,0 , M1 2γ δ −,0 , D22 ( − ) = M2 D11 ( − ) =

(4.26) (4.27)

and −γ (δ −,0 + δ −,−1 ). D12 ( − ) = √ M1 M2

(4.28)

Thus, the symmetric dynamical matrix is ⎛

2γ ⎜ M1 D(q) = ⎜ ⎝ 2γ −√ cos qa M1 M2

−√

⎞ 2γ cos qa ⎟ M1 M2 ⎟, ⎠ 2γ M2

(4.29)

4 Lattice vibrations and phonons

68

and solving the eigenvalue problem ω2 C = DC yields ( 1 1 1 1 2 −4 sin2 (qa) 2 ω =γ ±γ + + + . M1 M2 M1 M2 M1 M2

(4.30)

As expected, there are two solutions, and thus two vibrational branches (one is called acoustic and the other optical). This result can also be found using elementary methods. If we again examine the limiting cases, as q → 0, 1 1 2 , (4.31) + ω+ → 2γ M1 M2 2 ω− →

2γ (qa)2 . M1 + M2

(4.32)

If M1 = M2 , '

γ qa, M ' γ , ω+ → 2 M

ω− →

(4.33) (4.34)

and the ω− branch becomes that of the monatomic chain result (see Fig. 4.4). At the zone boundary where q = G/2 = π/b = π/2a (see Fig. 4.4), we find a gap. If we assume M2 > M1 , then 2 = ω+

2γ M1

(4.35)

2 ω− =

2γ . M2

(4.36)

and

ω Optical branch

1 1 2γ M 1 + M2

1/2

2γ /M1

1/2

2γ /M2

1/2

Acoustic branch qBZ

Figure 4.4

Lattice vibration dispersion curves for a diatomic chain of atoms with M2 > M1 .

q

4.1 Lattice vibrations

69

ω

π b

Figure 4.5

π a

q

Mapping of the lattice vibration dispersion curves for a diatomic chain of equal masses from that of a monatomic chain. However, if we set M1 = M2 , then at the zone boundary the gap goes to zero. When the two masses are equal, the periodicity of the system is half of the initial unit cell. So, if we consider a unit cell with half the initial periodicity, we would obtain a G that is twice the initial G. However, the dispersion curve will have only one acoustic branch. This leads to a dispersion curve where the upper half of the acoustic mode is folded back into an optical mode in the smaller Brillouin zone (Fig. 4.5). We now examine the motion of the atoms of a one-dimensional diatomic chain. The normal mode equation has the form C1 D11 = ω C2 D21 2

D12 D22

C1 . C2

(4.37)

By solving the above eigenvalue problem, we obtain C1 D12 (q) = 2 . C2 ω − D11 (q)

(4.38)

The displacement of the atoms in terms of Cj is Cj ξj = eiq·(R +τj )−iωt . Mj

(4.39)

Therefore, after using Eq. (4.38), the ratio of the displacement of the atoms is ξ1 (q) cos qa = . 2 ξ2 (q) 1 − ω2γ(q) M1

(4.40)

4 Lattice vibrations and phonons

Displacement ξ

70

Atomic displacement versus distance x for an acoustic mode for a diatomic chain.

Figure 4.7

Atomic displacement versus distance x for an optical mode for a diatomic chain.

Displacement

Figure 4.6

x

For the acoustic mode, as q → 0, ω → 0, and thus ξ1 /ξ2 → 1. Hence, the displacements of the atoms in one unit cell are in phase and of similar magnitude as expected for the acoustic mode, as shown in Fig. 4.6. 2 → 2γ (1/M +1/M ), and thus ξ /ξ → −M /M . For the optical mode, as q → 0, ω+ 2 1 1 2 2 1 Hence, the oscillations are out of phase, and the lighter mass has a larger amplitude, as expected of two oppositely charged atoms in an EM wave where the two atoms move in opposite directions; hence the name optical mode (Fig. 4.7). If we extend our study of the one-dimensional chain to higher dimensions, we can illustrate the procedure for counting branches. For a crystal of d dimensions with r atoms per unit cell, the total number of branches in the phonon dispersion curve is r × d. Of these r × d branches, there are d acoustic modes and d × (r − 1) optical modes. For example, consider KBr in the rock salt structure. Since KBr has two atoms per unit cell, there are six branches in the KBr phonon band structure, three of which are acoustic and three of which are optical (Fig. 4.8). The physical origin of having d acoustic modes arises from translational invariance of space, i.e. displacing all atoms by the same amount along any direction in d-space results in no restore force and hence there are d branches with ω(q → 0) = 0.

4.2 Second quantization and phonons

71

ω

LO TO × 2

LA TA × 2

qBZ

Figure 4.8

q

Lattice vibration dispersion curve for KBr. The transverse branches are doubly degenerate.

4.2 Second quantization and phonons We now turn to an elementary excitation view of lattice vibrational properties by associating phonons with the vibrational modes. Phonons are viewed as being particle-like and wave-like in analogy with electromagnetic radiation. We begin by considering a simple one-dimensional harmonic oscillator, satisfying the equation m¨x = −γ x.

(4.41)

√ The solution is x(t) = x0 e−iωt , where ω = γ /m for spring constant γ and mass m. If we take a quantum view starting with the Hamiltonian H=

1 p2 + γ x2 , 2m 2

(4.42)

then the energy levels are 1 En = hω n+ ¯ 2

(n = 0, 1, 2, . . . ).

(4.43)

It is convenient to take a second quantized view of this problem using creation and annihilation operators. The standard approach is to form a linear combination of the coordinate and momentum variables, x and p, and form new variables, a and a† , such that these variables satisfy the commutation relation

[a, a† ] = 1.

(4.44)

4 Lattice vibrations and phonons

72

The combinations of x and p for a and a† are 1 (p − imωx) a= √ 2hωm ¯

(4.45)

and a† = √

1 (p + imωx). 2hωm ¯

(4.46)

This choice satisfies Eq. (4.44) since [x, p] = ih¯ . Replacing x and p in Eq. (4.42) by expressing them in terms of a and a† , using Eqs. (4.45) and (4.46), yields H=

1 † hω(aa + a† a). ¯ 2

(4.47)

A matrix representation for a and a† can be introduced based on labeling states by the index n. We have the following eigenvalue equations for the harmonic oscillator √ (4.48) a |n = n |n − 1 and a† |n =

√

n + 1 |n + 1,

(4.49)

which are consistent with Eq. (4.44). In addition, Eqs. (4.48) and (4.49) give a† a |n = n |n,

(4.50)

1 hω H |n = n + ¯ |n = En |n. 2

(4.51)

and then, using Eq. (4.47), we have

From these essential features of the simple one-dimensional harmonic oscillator, we can propose a picture of excitations involving the creation and destruction of quanta in various states and the view of representing a state using the occupation number corresponding to specific quanta. This concept involves the setting up of a many-body state by operating on a vacuum state with creation and destruction operators to increase or decrease the number of particles in a given state. The state vector n1 ,n2 ,...,ni ... represents a state with n1 particles in state 1, n2 particles in state 2, and so on. The creation operators a†i repeatedly acting on the vacuum state |0 can produce this state vector. Also, when the destruction operator ai operates on the state vector, it destroys a particle in the ith state. There is an overall factor such that √ ni n1 ,n2 ,...,ni −1... , = ni + 1 n1 ,n2 ,...,ni +1... ,

ai n1 ,n2 ,...,ni ... =

(4.52)

a†i n1 ,n2 ,...,ni ...

(4.53)

a†i ai n1 ,n2 ,...,ni ... = ni n1 ,n2 ,...,ni ... .

(4.54)

4.2 Second quantization and phonons

73

Na γ M

γ M

γ M

γ

M

γ M

M

a

Figure 4.9

Finite linear chain with nearest-neighbor interactions. Therefore, the operator nˆ i = a†i ai measures the number of particles in the ith state, and it is called the number operator. Using this short description of second quantization and the occupation number representation for the state of a system, we can go beyond the simple harmonic oscillator and treat the model of interacting atoms, which we considered before, to represent lattice vibrations in a one-dimensional solid. This model uses a linear chain of N atoms of length L = Na with nearest-neighbor interactions (Fig. 4.9). Unlike the harmonic oscillator case, the “extension of the springs” depends on the relative displacements of the atoms. Hence, a simple real-space Hamiltonian composed of a combination of the squares of position and momentum is not possible. However, a decoupling occurs if we use a Fourier transformation of the original Hamiltonian, and this will lead us to the form we need. We begin with the Hamiltonian containing the kinetic and potential energies expressed in terms of real-space momenta pn and coordinates ξn , H=

1 2 1 p + γ (ξn+1 − ξn )2 , 2M n n 2 n

(4.55)

where ) * ξn , pn = ihδ ¯ n,n . As stated above, the desired form for the Hamiltonian is H = To accomplish this, we Fourier-transform the coordinate

(4.56)

k Hk .

1 ikna ξk e , ξn = √ N k

(4.57)

1 −ikna ξn e . ξk = √ N n

(4.58)

and

Using PBCs, k= with − N2 < ≤

N 2.

2π 2π = , Na L

(4.59)

Since ξn is Hermitian, † ξk = ξ−k .

(4.60)

4 Lattice vibrations and phonons

74

The momentum pk that is canonically conjugate to ξk is not obvious. To find it, we use the Lagrangian formalism. For the Lagrangian L({ξk , ξ˙k }), the canonically conjugate momentum becomes pk =

∂L . ∂ ξ˙k

Using

ei(k+k )na = Nδk+k ,0 ,

(4.61)

n

then the kinetic energy is T, with T= =

M (ξ˙n )2 2 n

M1 ξ˙k ξ˙k ei(k+k )na 2 N

(4.62)

k,k ,n

M ξ˙k ξ˙−k . = 2 k

Similarly, the potential energy (PE) becomes PE =

1 γ (ξn+1 − ξn )2 = γ ξk ξ−k (1 − cos ka), 2 n

(4.63)

k

and the Lagrangian has the form L=

M ξ˙k ξ˙−k − γ ξk ξ−k (1 − cos ka). 2 k

(4.64)

k

Hence, the conjugate momentum is pk =

∂L = Mξ˙−k . ∂ ξ˙k

(4.65)

Using Eq. (4.58), 1 −i(−k)na ξ−k = √ ξn e , N n and we have 1 pk = √ pn eikna , N n

(4.66)

4.2 Second quantization and phonons

75

thus p†k = p−k .

(4.67)

Finally, the Hamiltonian (using the results for the vibration frequency obtained in the last section) is ⎡ ⎤ H=

⎥ 1 ⎢ ⎢ pk p−k + 2γ (1 − cos ka) ξk ξ−k ⎥ ⎣ ⎦ ! " 2 M k

=

k

(4.68)

Mωk2

Mωk2 † 1 † p pk + ξ ξk , 2M k 2 k

and H=

(4.69)

Hk ,

k

which was our objective. Using the relations above, we can show that [ξk , pk ] = ihδ ¯ k,k .

(4.70)

If we now define 1 (Mωk ξk† − ipk ) 2hMω ¯ k

(4.71)

1 (Mωk ξk + ip†k ), 2hMω ¯ k

(4.72)

[ak , a†k ] = δk,k

(4.73)

[ak , ak ] = [a†k , a†k ] = 0.

(4.74)

a†k = √ and ak = √ then

and

Following our earlier description for the simple harmonic oscillator, we now have 1 † h¯ ωk ak ak + H= 2 k

and ' ωk =

2γ (1 − cos ka). M

(4.75)

76

4 Lattice vibrations and phonons

We can now make the comparison with the previous description for the simple harmonic oscillator. The operators a†k and ak create and destroy quanta (phonons) in the state k. The number operator nˆ k = a†k ak measures the number of phonons nk in the state k. The energy 1 Ek = nk + h¯ ωk 2 is viewed as the excitation energy of nk phonons of energy h¯ ωk plus the ground-state energy (zero-point motion 12 hω ¯ k ). The total energy of the vibrating system of cores is the groundstate energy plus the energy of a group of independent phonons excited above the ground state. For a given k, there is a quantized vibrational or sound wave mode of wavevector k and energy hω ¯ k . A sound wave with wavevector k is described by nk phonons excited above the ground state. Therefore, a statement in common use that a phonon is a quantized sound wave is incorrect. It takes nk phonons to describe a sound wave. The many-body state

nk , nk , . . . for phonons in different k-states can be constructed using creation operators 1 2 acting on the vacuum |0,

nk , nk , . . . = (a† )nk1 (a† )nk2 . . . |0 . (4.76) 1 2 k1 k2 The generalization of the one-dimensional case with vibrating cores (in the harmonic approximation) with r atoms per cell in d dimensions leads to the Hamiltonian H=

λk

1 † , hω ¯ λk aλk aλk + 2

(4.77)

where λ is the phonon branch index (λ = 1, 2, . . . , d × r) and ωλk are the frequencies from diagonalizing the dynamical matrix. To generalize, what we have done is to consider the Hamiltonian Hi (ri , pi ) + V(ri , rj , pi , pj ), (4.78) H= i

i,j

which we then transform into the following: Ek c†k ck + E. H = E0 +

(4.79)

k

The first term, E0 , in Eq. (4.79) is the ground-state energy, the second term represents the energy of the elementary excitations, and the third term, E, is the residual energy representing the interactions between the elementary excitations with terms involving more creation and destruction operators. This term can be expressed in terms of lifetimes for individual states k, τk ∼ h¯ /Ek . Hence τk measures the decay time of an excitation. For this picture of viewing a system in terms of elementary excitations (quasiparticles and collective excitations) to be useful, we require that Ek < Ek .

(4.80)

4.3 Response functions: heat capacity

77

When Eq. (4.80) is satisfied, then we can view our system as a collection of nearly independent excitations, and the properties of a solid can be viewed by considering the properties of a gas of these elementary excitations responding to a probe. In the example of phonons discussed above, E = 0 because we have made the harmonic approximation. Any anharmonic terms in Eq. (4.7) would lead to interactions between phonons.

4.3 Response functions: heat capacity In many respects, the response functions corresponding to different probes have similar features. The probe could be temperature or EM radiation, for example. The probes excite elementary excitations which then give rise to the response based on the properties of the system. The heat capacity at constant volume CV (T) is a response function, giving the responses to a temperature probe by describing the T dependence of the energy U of the system when elementary excitations are created. CV (T) =

∂U ∂T

.

(4.81)

V

For a gas of phonons, we compute the thermodynamic average energy U using Bose statistics for phonons (since they satisfy the boson commutator relations given in Eqs. (4.73) and (4.74)) with branch index λ, wavevector q, and energy hω ¯ λ,q : U(T) =

λ,q

1 , h¯ ωλ,q nλ,q (T) + 2

(4.82)

where the phonon occupation is given by 1

nλ,q (T) = e

h¯ ωλ,q kB T

.

(4.83)

−1

Then hω ¯ λ,q hω e kB T ¯k Tλ,q2 ∂U B = CV (T) = hω ¯ λ,q h¯ ω 2 , ∂T λ,q λ,q e kB T − 1

(4.84)

where kB is the Boltzmann’s constant. For a sample of volume V, q

V → (2π )3

d3 q BZ

(4.85)

4 Lattice vibrations and phonons

78

and 2 hω ¯ λ,q e kB T kB h¯ ωλ,q kB T V 3 CV (T) = h¯ ωλ,q 2 d q. (2π )3 BZ λ e kB T − 1

(4.86)

In the limit kB T hω, ¯

hω ¯ λ,q exp kB T

∼1+

hω ¯ λ,q . kB T

(4.87)

If we consider this limit for three dimensions, λ = 1, 2, . . . , 3r, and we arrive at the Dulong–Petit law, which is appropriate for high T, CV (T) =

V kB (3r) (2π )3

d3 q = kB (3r)N = 3R,

(4.88)

where R is the gas constant, r is the number of atoms in a cell, and we have used the fact that d3 q gives the volume of the Brillouin zone, which is d3 q =

(2π )3 × N, V

(4.89)

where N is the number of cells in the crystal. A typical CV (T) is shown in Fig. 4.10 along with the high T limit of 3R. The low-temperature T3 behavior will be discussed in Section 4.4.1, where we discuss the Debye model for phonons.

CV

T TD

Figure 4.10

Heat capacity of a solid as a function of temperature arising from lattice vibrations with TD ≈ 300 K (room temperature).

4.4 Density of states

79

4.4 Density of states Often in calculations of response functions such as CV (T), sums over q states are converted to integrals over q, as shown in Eqs. (4.85) and (4.86). A further transformation, which is often simplifying and gives more physical insight if the integrand depends only on the frequency explicitly, is to transform the q integral to an integral over ω or energy. This transformation involves the introduction of the density of states D(ω). The quantity D(ω)dω gives the number of states with frequencies between ω and ω + dω. Hence, for a function f(ω(q)), V 3 f(ω(q)) → f (ω (q)) d q → f(ω)D(ω)dω. (4.90) (2π )3 BZ q For the phonon case, each branch λ can contribute Dλ (ω) to the total density of states D(ω), so δ(ω − ωλ,q ) = Dλ (ω). (4.91) D(ω) ≡ λ,q

λ

In one dimension, the number of q states dN(q) within q and q + dq in the Brillouin zone for a line of length L is dN(q) = 2

L dq, 2π

where a factor of 2 is inserted to limit q to be positive. Hence, the density of q states W(q) becomes W(q) =

L dN = , dq π

(4.92)

and the density of states in the frequency domain D(ω) is D(ω) = W(q)

dq W(q) = , dω dω/dq

(4.93)

where dω/dq can be identified with the group velocity of the branch of interest. The generalization to d dimensions is, for each phonon branch λ, ds Ld , Dλ (ω) = d (2π ) s |∇q ωλ |

(4.94)

where s is a surface of equal ω in q-space and the integral is over the Brillouin zone. The one-dimensional chain is an instructive example to consider (Figs. 4.1 and 4.2). Rewriting Eq. (4.22), ω=

4γ M

1 2

sin

qa 2

= ωmax sin

qa 2

,

(4.95)

4 Lattice vibrations and phonons

80

hence dq = dω

2 a 1ω2

1

max

− ω2

21 ,

(4.96)

2

and D(ω) =

2L

π aωmax 1 −

ω ωmax

2 12

.

(4.97)

For ω = 0, we find a constant value for D(ω), D(0) =

2L , π aωmax

(4.98)

and there is a singularity at ω = ωmax , where the group velocity is zero. The diatomic one-dimensional chain (Figs. 4.3 and 4.4) is another instructive example. For the acoustic branch (Fig. 4.4), the situation is the same as in Fig. 4.2 for the monatomic lattice, and for M2 > M1 ,

DA (ω) ∝ 1 − where

ω ω1

2 − 12 ,

(4.99)

( 2γ , M2

ω1 =

and there is a singularity at ω1 . For the optical branch, the group velocity becomes zero at ( ω2 =

2γ M1

and at the maximum frequency ( ωm =

2γ

1 1 . + M1 M2

These give rise to singularities in D(ω), as shown in Fig. 4.11.

4.4.1 The Debye approximation The continuum approximation in three dimensions assumes a constant sound velocity vs ; that is, ω = vs q for q ≤ qD and for each polarization and for all directions (Fig. 4.12). The cutoff qD is defined by demanding that the volume of q space considered is the same as

4.4 Density of states

Density of states D(ω)

81

Acoustic

Optical

ω1

Figure 4.11

ωmax

ω2

ω

Density of phonon states for a diatomic chain. ω ωD

qD

Figure 4.12

q

The Debye dispersion curve.

the Brillouin zone. This is the Debye2 approximation. For this case, the density of states is given by Dλ (ω) =

V 4π q2 V ω2 = , (2π )3 vs 2π 2 vs3

(4.100)

with ω ≤ ωD , as shown in Fig. 4.13. In d dimensions, the Debye approximation yields Debye

Dλ

(ω) ∼ ωd−1 .

2 P. Debye, “Zur Theorie der spezifischen Waerme,” Ann. Physik. 39(1912), 789.

(4.101)

4 Lattice vibrations and phonons

Density of states D(ω)

82

~ ω2

ωD

Figure 4.13

ω

Density of states in the Debye approximation for three dimensions. Since each polarization has N states, if we define ωD as the frequency of qD , we have, in three dimensions,

ωD

N= 0

Dλ (ω)dω =

3V ωD 6π 2 vs3

(4.102)

and ωD =

N 2 6π V

1 3

vs .

(4.103)

Returning to the calculation of CV (T) for a three-dimensional system with one atom in a unit cell, we have 3 4 ω2 Debye (ω) = 3N . (4.104) Dλ 3 ωD Defining x≡

TD hω ¯ D ≡ , kB T T

(4.105)

where TD = kωD /kB is called the Debye temperate, Eq. (4.86) gives CV (T) = kB

ωD

ωD

0

λ

x2 ex Debye D (ω)dω (ex − 1)2 λ

x2 ex ω2 dω x − 1)2 (e 0 3 xD T x4 ex = 9NkB dx. TD (ex − 1)2 0 =

9NkB 3 ωD

(4.106)

4.4 Density of states

83

In the high-temperature limit T TD , x 1, CV (T) = 9NkB

T TD

3

xD 0

x4 dx = 3NkB , x2

(4.107)

which is the Dulong–Petit law we obtained previously for r = 1. In the low-temperature limit, T TD , x 1, TD /T → ∞, xD → ∞, and Eq. (4.107) becomes CV (T) =

12π 4 5

NkB

T TD

3 ,

(4.108)

which is the Debye T 3 law, which correctly fits the experimental CV (T) curve of insulators and is the calculated curve shown in Fig. 4.10. The Debye model works well at low T because in this regime only long-wavelength acoustic modes are excited. The ω(q) for these modes can be approximated by the continuum model or the Debye model.

4.4.2 The Einstein spectrum To explain the vanishing heat capacity of solids at low T, Einstein3 assumed that each mode had the same ω = ω0 and viewed a solid as a collection of atoms, with each vibrating at the same frequency ωλq = ω0 .

(4.109)

(ω) = Nδ(ω − ω0 ), DEinstein λ

(4.110)

The corresponding density of states is

where N is the number of cells. Letting kB TE ≡ hω ¯ 0, CV (T) = 3kB N

x2 ex δ(ω − ω0 ) dω (ex − 1)2

(4.111)

and 3NkB CEinstein (T) = V

TE T

2 e

TE 2 e T −1

TE T

.

(4.112)

So, at low temperature, a comparison of the models yields CEinstein ∼ e− V

TE T

(4.113)

3 A. Einstein, “Die Plancksche Theorie der Strahlung und die Theorie der spezifischen W¨arme,” Ann. Physik.

22(1907), 180.

4 Lattice vibrations and phonons

84

and Debye CV

∼

T TD

3 .

(4.114)

As mentioned previously, since acoustic modes are modeled more accurately in the Debye approximation, the heat capacity generally obeys Eq. (4.114); however, Eq. (4.113) does show a vanishing Cv (T), and it has applicability to other situations where the excitations have little wavevector dispersion.

4.5 Critical points and van Hove singularities In general, densities of states can exhibit sharp structures. This arises because, in the expression for the density of states, e.g. in three dimensions, V ds Dλ (ω) = , (4.115) (2π )3 |∇q ωλ | there are q-points in the Brillouin zone, where ∇q ωλ = 0. These points, where the group velocities are zero, are called critical points,4 and the resulting structures in the density of states are called van Hove singularities.5 As an example, Fig. 4.14 displays the dispersion curve for an optical phonon branch in one dimension, which resembles the optical mode of the diatomic lattice (Fig. 4.4). Because of the zero group velocity at ω = ω1 and ω = ω2 , the density of states exhibits singularities at these frequencies (Fig. 4.11), which correspond to the minimum and maximum frequencies in the optical branch. For three dimensions, D(ω) exhibits structures that can be characterized in terms of the van Hove singularities. To explore the influence of critical points on D(ω) in three dimensions, we examine the topology of the ω(q) curve near a critical point q = qcp , where ∇q ωλ = 0. To lowest order, with i = 1, 2, 3, we have (assuming the function is analytic and is expanded along principal axes) αi (q − qcp )2i . (4.116) ω(q) = ω(qcp ) + i

If α1 , α2 , α3 > 0, then we have a minimum. If α1 , α2 , α3 < 0, then we have a maximum. If some are positive and some are negative, we have a saddle point. These singularities are classified according to the number of negative α’s, as listed in Table 4.1. There exists a theorem concerning the minimum number of critical points in a branch or band of a dispersion and periodic curve.6 An analytic function with N variables, which is 4 J. C. Phillips, “Critical points and lattice vibration spectra,” Phys. Rev. B 104(1956), 1263. 5 L. Van Hove, “The occurrence of singularities in the elastic frequency distribution of a crystal,” Phys. Rev.

89(1953), 1189. 6 L. Van Hove, “The occurrence of singularities in the elastic frequency distribution of a crystal,” Phys. Rev.

89(1953), 1189.

4.5 Critical points and van Hove singularities

85

Table 4.1 Classiﬁcation of critical points in three dimensions. Class

Name

0 1 2 3

M0 M1 M2 M3

Called parabolic point (minimum) saddle point saddle point parabolic point (maximum)

ω

ω2

ω1

qBZ

Figure 4.14

q

There are at least two critical points in one dimension for an analytical periodic function, a maximum at ω2 and a minimum at ω1 . periodic in all of them, must have at least CN n critical points of type n, where

CN n =

N! n!(N − n)!

(4.117)

with n ≤ N. Therefore, in one dimension, N = 1 and n = 0 or 1. We have C10 = 1 (minimum) and C11 = 1 (maximum). These are the critical points which we associated with Fig. 4.14. For two dimensions, N = 2 and n = 0, 1, or 2, and we have C20 = 1 (minimum), C21 = 2 (two saddle points), and C22 = 1 (maximum). Hence in two dimensions, we must have at least a maximum, a minimum, and two saddle points. For three dimensions, C30 = 1 (one minimum M0 ), C31 = 3 (three saddle points of type M1 ), C32 = 3 (three saddle points of type M2 ), and C33 = 1 (one maximum M3 ). Hence, there are at least eight critical points in a three-dimensional spectrum. Most density-of-states functions in three dimensions have more than the minimum number of critical points. Another theorem associated with the critical points is that ω0 < ω1 < ω2 < ω3 , where ω0 is the frequency at which the M0 critical point exists, etc. Different M1 ’s can be at the same energy, and similarly for the M2 ’s, so that a three-dimensional D(ω) can look like it has only four van Hove singularities, as will be discussed later.

4 Lattice vibrations and phonons

86

The structure in D(ω) near a critical point can be explored by examining the integral in Eq. (4.115). The topology of the energy surface leads to specific forms for the frequency dependence of D(w) near the critical point, and they will depend on the number of dimensions of space. In three dimensions, to explore the structure near a critical point, it is convenient to write Eq. (4.116) in cylindrical coordinates, with the assumption that α1 = α2 with no loss of generality if we are close to the critical point. If we now choose (q, θ , qz ) as our coordinates, where q2 = q21 + q22

(4.118)

and q2 , q1

(4.119)

qz = q3 ,

(4.120)

tan θ =

then Eq. (4.116) becomes ω − ωc = α1 q2 + α3 q2z .

(4.121)

Near an M0 singularity, ωc = ω0 , α1 > 0, and α3 > 0, and the surface in q-space for ω near ω0 is an ellipsoid if ω > ω0 , and there is no solution of Eq. (4.121) if ω < ω0 . For an M1 singularity, ωc = ω1 , α1 > 0, and α3 < 0, and Eq. (4.121) yields a q-space surface which is a hyperboloid of two sheets if ω < ω1 . If ω > ω1 , we have a hyperboloid of one sheet. For an M2 singularity, ωc = ω2 , α1 < 0, and α3 > 0, and, for ω < ω2 , one has a hyperboloid of one sheet, while for ω > ω2 , one has a hyperboloid of two sheets. Finally, for an M3 singularity, ωc = ω3 , α1 < 0, and α3 < 0, and the q-space surface is an ellipsoid for ω < ω3 , and no solution of Eq. (4.121) is possible for ω > ω3 . If we choose qz to be along the principal axis of the structures above, which can all be chosen to be symmetric about the qz axis, it can be shown that D(ω) is proportional to the extent of the surface in the qz direction in the vicinity of the critical point. Hence for an M0 critical point, using Eq. (4.121) and ignoring the q variable, the qz range is

ω − ω0 − α3

1 2

≤ qz ≤

ω − ω0 α3

1 2

.

(4.122)

The integral in Eq. (4.115) over the qz variable therefore gives a D(ω) dependence near M0 of the form 1

D(ω) ∝ (ω − ω0 ) 2 . A schematic drawing is given in Fig. 4.15.

(4.123)

4.5 Critical points and van Hove singularities

87

Density of states D(ω)

M0

Infinite slope

ω

ω0

Figure 4.15

Density of states in three dimensions near an M0 van Hove singularity.

Density of states D(ω)

M1 Infinite slope

ω ω1

Figure 4.16

Density of states in three dimensions near an M1 van Hove singularity.

For an M1 singularity, following the approach above, for ω > ω1 (α3 < 0), the surface extends from qz = −∞ to qz = ∞, except for a gap from qz = −

ω1 − ω α3

1 2

to qz =

ω1 − ω α3

1 2

(4.124)

(for a hyperboloid of two sheets) and no gap for ω > ω1 (a hyperboloid of one sheet). The infinite extent is not relevant since this approximation is appropriate only near the critical point. The outer portions of the surface are finite and smoothly varying. As a result of Eq. (4.124) and this analysis, D(ω) approaches ω1 from below with infinite slope and leaves (ω > ω1 ) with finite slope as shown in Fig. 4.16. Since an M2 singularity has the opposite ω behavior relative to an M1 singularity, the D(ω) approaches ω2 with finite slope and then drops with infinite slope, as shown in Fig. 4.17. A similar argument can be made when comparing an M3 maximum with an M0 minimum. This gives rise to D(ω) ∝ (ω3 − ω)1/2 below ω3 and zero above, as shown in Fig. 4.18. Figure 4.19 shows the simplest spectrum in three dimensions for a periodic branch. It contains an M0 at the minimum frequency ω0 , three degenerate M1 saddle points at ω1 , three degenerate M2 saddle points at ω2 , and an M3 maximum at ω3 . Although the eight critical points required for three dimensions are displayed in Fig. 4.19, the degeneracies at ω1 and ω2 are not required.

4 Lattice vibrations and phonons

88

Density of states D(ω)

M2 Infinite slope

ω

ω2

Figure 4.17

Density of states in three dimensions near an M2 van Hove singularity.

Density of states D(ω)

M3

Infinite slope ω ω3

Density of states in three dimensions near an M3 van Hove singularity.

Density of Status D(ω)

Figure 4.18

ω0

Figure 4.19

ω1

ω2

ω3

ω

The total density of states obtained by including one of each of the critical points. This can be viewed as the simplest D(ω) for N = 3 if the M1 and M2 singularities are each taken to be threefold degenerate.

For the Debye spectrum with a minimum in the acoustic branch consistent with lim ω(q) = 0,

q→0

(4.125)

the dispersion curve ω(q) is not analytic in q. In fact, ω(q) = vs q,

(4.126)

where the velocity of sound vs can be different in different directions. Hence the rules above do not apply in this case. Therefore, for the low-frequency acoustic modes, our earlier result D(ω) ∝ ω2 applies.

4.5 Critical points and van Hove singularities

89

ω

LA

TA2

TA1

q

qBZ

Figure 4.20

The phonon dispersion curve for Al in the (1,1,0) direction (TA1 and TA2 are the transverse acoustic modes, and LA is the longitudinal acoustic mode).

D(ω)

TA1 ω

TA2

ω

LA

ω LA Total

TA1

TA2

ω

Figure 4.21

Sketch of the density of states for the three diﬀerent phonon branches of Al and the total density of states.

90

4 Lattice vibrations and phonons

For a real crystal example, we can consider Al, which is an fcc crystal with one atom per unit cell. Therefore, there are three phonon branches, as shown schematically in Fig. 4.20. The corresponding D(ω) appears in Fig. 4.21, with van Hove singularities easily recognizable in the spectrum.

Part I Problems

I.1. Crystal structure of MgB2 . MgB2 is a superconductor with a high transition temperature of 39K and has multiple values for the superconducting energy gap. The material has a rather simple structure as given by the model below in Fig. I.1 – the boron atoms (dark balls) form graphitic honeycomb layers (stacked identically on top of each other) and the magnesium atoms (light balls) are located above the center of the B hexagons exactly in between the layers. Let a be the B–B distance in the layer and c be the distance between the boron layers. (a) Construct the primitive lattice vectors, the reciprocal lattice, the Wigner–Seitz cell, and the Brillouin zone for MgB2 . (b) What is the volume of the primitive unit cell? What is the volume of the Brillouin zone? Give the locations of the basis atoms in terms of the primitive lattice vectors. (c) In general, crystal structures have many symmetry operations; those operations can be one of four types: rotation, inversion, reflection, or translation (to find out more about them, read Tinkham’s Group Theory and Quantum Mechanics). Find, for MgB2 , all symmetry operations which leave the crystalline Hamiltonian invariant. (You may neglect spin–orbit interaction and other relativistic effects.) (d) Draw the irreducible part of the Brillouin zone. I.2. The GaN Crystal. The 2014 Nobel Prize in Physics was given for work on the GaN crystal, specifically for using it in blue light-emitting diodes (LEDs). A model of its crystal structure is given in Fig. I.2, where the Ga atoms are denoted by the light balls and the nitrogen atoms by the dark balls. It has a hexagonal lattice, with a1 = a2 = a, a3 = c, and the angle between the vectors a1 and a2 is 120◦ .

Figure I.1 91

Crystal structure of MgB2 .

Part I Problems

92

a3

a1

Figure I.2

a2

Crystal structure of GaN.

(a) Write down the explicit expressions of a set of primitive reciprocal lattice vectors b1 , b2 , and b3 in Cartesian coordinates (in terms of the values a and c). Sketch the first Brillouin zone. What is the volume of the first Brillouin zone in terms of a and c? (b) How many atoms of each kind are there in the basis of this crystal structure? (c) In addition to translations, there are many symmetry operations under which the above structure remains invariant. Name any six specific operations among them. (d) GaN is used in blue LEDs as it is a wide-bandgap semiconductor. Why is it not surprising that this material is an insulator? Explain your answer in terms of the band theory. I.3. Born–Oppenheimer approximation for a molecule. Consider a diatomic molecule with linear dimension a and reduced mass M. Show that the electronic, vibrational, and rotational energy levels can be estimated as terms which are proportional to successively higher orders in the small ratio m/M (m is the electron mass). How is this related to the Born–Oppenheimer approximation discussed in the text? I.4. Hartree–Fock approximation. The Hartree–Fock approximation is a simple yet important model for understanding electron–electron interaction in crystals. (a) Derive the Hartree–Fock self-consistent field equations from the variational principle using a Slater determinant of single-particle orbitals as a trial many-electron wavefunction. (b) Consider the total electronic energy of a system (e.g. a molecule) in the Hartree– Fock approximation. Calculate the change in the energy of the system if an electron is promoted from an occupied ith orbital to an unoccupied jth orbital, assuming that the orbitals are unchanged after the excitation. How is this excitation energy related to the eigenvalues of the Hartree–Fock equations? This kind of excitation is called a neutral excitation, which occurs for example in a photoexcitation process, since no electrons are added or removed from the system. The result is known as Koopmans’ theorem. I.5. Born–von Karman boundary condition. The use of the Born–von Karman boundary condition makes possible a simple and effective description of infinitely extended

Part I Problems

93

crystals. With this boundary condition, the number of k-states is finite and equivalent in the successively higher Brillouin zone. This leads to different choices of representation for the electron band structure. (a) Describe and justify the three possible representations of the band structure (that is, the electron energy vs. wavevector) for a crystal: reduced zone scheme, repeated zone scheme, and extended zone scheme. (b) Show that there are exactly the same number of allowed wavevectors in the first Brillouin zone as there are unit cells in the crystal. I.6. Energy bands of elemental solids. Name three elements in each category which are: (a) semiconductors (and give their crystal structure); (b) semimetals (and give their crystal structure); (c) metals in the fcc structure; (d) metals in the bcc structure; (e) metals in the hcp structure. Consider only elements lighter than Rn. Distinguish metals which are transition metals in (c), (d), and (e). I.7. Point group. Prove the general theorem that only rotations that are multiples of 60◦ , 90◦ , 120◦ , and 180◦ can be symmetry elements of a crystal. (Hint: consider rotation by θ . By writing it as a matrix, show that 1 + 2 cos θ = integer.) I.8. Lattice sums. It is often necessary to do “lattice sums” and sums over “q-space.” For lattice vectors Rn , find the results for the following sums: iq·R e n, (a)

n

iq·R 2

, n (b) e

n iq·R n e . (c) q

I.9. Free electron gas. Treat a metal as a free-electron gas and calculate: (a) the density of states as a function of energy, (b) the density of states at the Fermi level in terms of n and EF , (c) the electronic heat capacity. I.10. Heat capacity from electrons in a semimetal. Find an expression for the electronic contribution to the heat capacity of a semimetal at very low temperatures for electrons of mass me and holes of mass mh . Let Ee be the energy of the bottom of the electron band and let Eh be the energy of the top of the hole band. I.11. Another form of the Kronig–Penney model. Consider an electron in one dimension in the presence of the potential U0 (x − ma)(ma + b − x), (I.1) U(x) = m

where (x) is a step function (= 0 if x < 0, = 1 if x > 0), a is the lattice constant, b is the width of the potential well, and U0 is the potential height/depth. (a) Focus on a single unit cell and write down the boundary condition on the Schr¨odinger equation that leads to Bloch states in this unit cell.

Part I Problems

94

(b) Solve the Schr¨odinger equation in this cell by taking summation of planewaves and imposing suitable boundary conditions at the positions 0, b, and a. The result is a condition on the Bloch index k. 2 a−2 . The condition on the (c) Take the limit b → 0, U0 → ∞, and U0 b → W0 a h¯ m Bloch index should become cos ka =

W0 sin Ka + cos Ka, Ka

(I.2)

where K = 2mε/h¯ 2 , with ε the energy of the state. (d) Produce plots of the two lowest-energy bands following from Eq. (I.2) for a = 1, m = 1, and W0 = 1. Display the bands in the reduced zone scheme and the extended zone scheme. I.12. Structure factor. An energy gap is not necessarily opened up at the Brillouin zone (BZ) edges, due to the vanishing Fourier components of the crystal potential. One example is nearly-free electrons in a hexagonal lattice. The empirical pseudopotential method introduced in the text is closely related to the Fourier components of the crystal field. (a) Define the term “structure factor” and evaluate it for an hcp lattice. Show that its value leads to a vanishing energy gap for states on the hexagonal face of the Brillouin zone for this structure in the nearly-free electron model (NFEM). (b) Show explicitly that the first three pseudopotential form factors needed for a band calculation for Si are V(G2 ) for G2 = 3, 8, 11 (in units of (2π/a)2 ). What are the values of the G2 ’s for the next five relevant form factors? I.13. Tight-binding model. Using the tight-binding method, and assuming one spherically symmetric atomic orbital/atom and only nearest-neighbor interactions, (a) find E(k) for the simple cubic, bcc, and fcc crystal structures, (b) find E(k) for a two-dimensional (2D) square lattice, (c) plot E(k) = constant in the first BZ in part (b). In (a), (b), and (c), treat the hopping integral as a parameter and the overlap integrals equal to zero for neighboring orbitals. I.14. Diatomic chain. Calculate the band structure of a diatomic chain with the Hamiltonian H=

† † 1 c2i c2i + 2 c†2i+1 c2i+1 + (−t) c2i c2i+1 + h.c. , i

(I.3)

i

where 1 > 2 , and c†i and ci are the creation and destruction operators of electronic orbitals at the ith site, respectively. Suppose t (1 − 2 ) and expand (k) in t/(1 − 2 ). I.15. Tight-binding calculation in 2D. In high Tc cuprate superconductors, there are layers of Cu–O planes, as shown in Figure I.3. Consider the above 2D square Cu–O crystal with the distance between copper atoms given by a, and the oxygen atoms

Part I Problems

95

Cu

O

O

Cu

Figure I.3

O

O

O

O

Cu

Cu

Cu

O

O

O

O

Cu

Cu

Cu

O

O

Cu

Cu–O plane in high-temperature cuprate superconductors.

I.16. I.17.

I.18. I.19.

I.20.

I.21.

located midway between the copper atoms. Using the tight-binding method and considering only nearest-neighbor interactions (assuming orthogonal orbitals), do the following calculations. (a) Find E(k), assuming that there is one d-orbital of (x2 − y2 ) symmetry on each copper atom and one p-orbital on each oxygen atom that is pointing along the nearest-neighbor direction. How many electronic bands are there for this model Hamiltonian? (b) Sketch the energy bands along the [10] and [11] directions. Schr¨odinger equation of crystal electron. Find the Schr¨odinger equation for the periodic part of the Bloch function (i.e. uk (r)). Dirac equation and spin–orbit interaction. Derive the spin–orbit contribution to the one-electron Hamiltonian starting with the Dirac equation. How does this affect Bloch’s theorem? Discuss translational invariance, rotational invariance, inversion symmetry, and time-reversal invariance for this Hamiltonian. Orthogonality of Bloch functions. Show that two Bloch functions eik·r uk (r) and eik ·r uk (r) are orthogonal if k − k is not a reciprocal lattice vector. Parity of Bloch waves. Consider a crystal potential with inversion symmetry. (a) Show that for most wavevectors in the first Brillouin zone, the Bloch functions cannot have a definite parity in spite of the crystal inversion symmetry. (b) There are specific wavevectors for which the Bloch functions can have definite parity. Find the wavefunctions and describe their locations in the first Brillouin zone. f -sum rule. Examine the problem of deriving the f-sum rule for the case of degenerate bands. Assume E(k0 ) is s-fold degenerate. Show that for a crystal with inversion symmetry, the first-order contributions of perturbation theory are zero and one must consider second-order effects (Van Vleck perturbation theory). Discuss the analytic properties of the bands for the s = 2 case and define an effective mass tensor (if possible) for this case. Delta function potential. Solve the Schr¨odinger equation for a single onedimensional delta function potential. Under what conditions does a bound state

Part I Problems

96

I.22.

I.23.

I.24.

I.25.

exist? What is the energy of the bound state? Do the same calculation for two onedimensional delta function potentials separated by a distance a. Describe (without repeating the previous Kronig–Penney calculations) what happens as one goes to the many delta function problems. High symmetry points. Look up the names (given in Greek letters) of the high symmetry points in the first Brillouin zone for the common lattices given below. Compute and plot E(k) for the free-electron model (FEM) in the following symmetry directions in the first Brillouin zone: (a) simple cubic, to R; (b) bcc, to N; (c) fcc, to X; (d) hcp, to A. Deep core levels. Estimate the effect of other atoms on the deep core levels of an atom in a crystal in the following way. Consider a model simple cubic crystal with ˚ and one atom per unit cell of atomic number z = 6. Calculate roughly the a = 5A width of the “energy band” formed by the lowest-lying s electrons, and calculate numerically the ratio between this bandwidth and the energy of the atomic s states. Make appropriate approximations in evaluating any integrals that may appear in your answer. Buckyballs. Buckyballs are molecules with 60 carbon atoms. They crystallize in an fcc lattice. (Assume no band overlap.) (a) How many filled electron bands are there? (b) How many partially filled electron bands do you expect? When this system is doped with potassium, one can form K3 C60 in an fcc lattice with the three potassium atoms inserted in the primitive cell. (c) How many filled electron bands are there for K3 C60 ? (d) How many partially filled electron bands do you expect in K3 C60 ? Density of states. (a) Show explicitly that the density of states in three dimensions has the form ds . (I.4) D(ω) = 3 (2π ) |∇ q ω|

(b) For a 2D lattice, derive the expression for the behavior of the density of states near critical points giving: (i) a minimum, (ii) a maximum, (iii) a saddle point. √ I.26. Velocity of sound. The classical formula for the velocity of sound is vs = R/ρ, where R is the bulk modulus and ρ is the atomic mass density. (a) Evaluate vs for a free electron gas using the electron bulk modulus and density. (b) Are the sound waves the same as ordinary sound waves? (c) Evaluate this vs for a gas of He-3 atoms, neutrons, muons, positrons, and protons, assuming in each case a concentration of n fermions/cm3 . (d) What is kF for each group of fermions in (c)?

Part I Problems

97

α

m

M

m

a

Figure I.4

α

β

M

b

Spring model of a diatomic chain.

I.27. Vibrational modes in graphene. Consider a graphene crystal and let us ignore the degree of freedom along the direction that is perpendicular to the carbon atomic plane, i.e. viewing this system as a strictly 2D system. (a) How many acoustic phonon branches and optical phonon branches are there for this 2D crystal? Why? (b) Using a Debye model for the phonon density of states, obtain the temperature dependence of its phonon-heat capacity at low temperature. (c) What is the minimum number of van Hove singularities for each optical phonon branch of such a 2D crystal? Sketch the functional form of an M0 van Hove singularity in the density of states for an optical branch of this system. I.28. Debye model. Consider a three-dimensional crystal with one atom per unit cell in the Debye approximation. (a) Find the mean square displacement of an atom at absolute zero temperature. (b) Derive a formula for the contribution of the zero-point motion to the total energy of the crystal. (c) Determine an expression for the phonon entropy. (d) Evaluate (a), (b), and (c) numerically for the case of solid aluminum. I.29. Lattice dynamics of a molecular chain. Consider the following model (see Fig. I.4) for a chain of diatomic molecules, where a = 2b, M and m are masses of the atoms, and α and β are harmonic force constants. In this problem, consider the longitudinal phonons only. (a) Construct the dynamical matrix and calculate the phonon frequencies, ωλ (k). (b) Sketch the phonon dispersion relation and the phonon density of states. (c) Apply the procedure discussed in the text on second quantization to the system and show that with a suitable choice of a and a† the Hamiltonian becomes ˆ = H

λk

1 nˆ λk + hω ¯ λk , 2

(I.5)

where nˆ λk = a†λk aλk . I.30. One-dimensional Debye model. Find the low-temperature heat capacity (within a dimensionless multiplying factor) for a monatomic lattice in one dimension in the Debye approximation. Express your answer in terms of T/TD , where T is the temperature and TD is the Debye temperature.

Part I Problems

98

I.31. Phonons in 2D. Consider a 2D square lattice with lattice constant a and a basis of three atoms per primitive cell. (a) What are the total number of phonon branches for each of the following: longitudinal acoustic, transverse acoustic, longitudinal optic, and transverse optic? (b) Assume that the acoustic modes are represented by the Debye model. What is the maximum acoustic phonon frequency in terms of the lattice constant a and the velocity of sound vs ? (c) Find the contribution to the low-temperature heat capacity (within a dimensionless coupling constant) from the longitudinal acoustic phonon branch. Express your answer in terms of T, TD , and N, where T is the temperature, TD is the Debye temperature, and N is the number of cells in the crystal. I.32. Zero-point energy correction. Find a simple expression for the zero-point energy correction to the total energy of a solid in the following two cases. (a) Assume a three-dimensional Debye model with one atom per cell where all acoustic modes are degenerate. (b) Assume a three-dimensional Einstein model with one atom per cell and all three modes degenerate. I.33. Charged harmonic oscillator. Consider a charged harmonic oscillator in a constant electric field F = (−e)E. The Hamiltonian is H=

γ p2 + x2 + eFx. 2m 2

(I.6)

(a) Show that the Hamiltonian can be written as (h¯ = 1) λ2 1 H = ω(A† A + ) − , 2 ω

(I.7)

√ where) ω = * γ /m, and give the expressions for λ and A. (b) Find A, A† . (c) Give an expression for the position operator X(t) and give a physical explanation for its form. I.34. Mean position of particles in a one-dimensional potential. A particle is bound in a one-dimensional potential, V(x) = 12 mω2 x2 − Cx3 (for small x). Describe how the mean position of the particle changes for the different eigenstates when C is small. (Hint: use perturbation theory and show that anharmonic terms will cause expansion.)

PART II

ELECTRON INTERACTIONS, DYNAMICS, AND RESPONSES

5

Electron dynamics in crystals

In the preceding chapters, we discussed the electron states within a single-particle picture in a perfect crystal. This is in some sense equivalent to considering electrons in free space in quantum mechanics; the interaction of the electron with the crystalline potential renormalizes the dispersion relation of the electrons. To understand many phenomena, such as electrical transport in a solid, we would need to describe the behavior of electrons in crystals when some non-periodic perturbation, either from an external applied field or a defect structure, is added to the crystalline periodic field. In this chapter, we introduce in a more rigorous fashion the concepts of group velocity v, effective mass m∗ , and the equation of motion for the dynamics of the electron. Denoting H0 as the perfect crystal Hamiltonian, the motion of an electron in an additional potential U(r) within a one-electron picture is given by the usual time-dependent Schr¨odinger equation ∂ψ(r, t) [H0 + U(r)] ψ(r, t) = ih¯ . (5.1) ∂t The static perturbation U(r) may arise from external applied electric or magnetic fields, or come from imperfections in the crystal, such as structural defects and impurities. In many important and common situations, U(r) is slowly varying in space (compared to the atomic separation) but becomes very large as r → ∞. For example, a uniform applied electric field E gives rise to U(r) = −eE · r, and a uniform magnetic field B produces a vector potential A = 12 B × r in the symmetric gauge. Potential perturbations caused by charge impurities, dislocations, surfaces, etc. are also often static and slowly varying compared to the interatomic distance, but they can be very large. These common situations cannot be treated straightforwardly by standard perturbation methods since, particularly for uniform applied fields, the perturbing potential diverges at large distance r in an extended crystal.

5.1 Eﬀective Hamiltonian and Wannier functions We develop here a formulation that will allow us to determine the behavior of crystal electrons in an external potential, which is slowly varying in both space and time. The framework is to consider that the problem of an electron in a perfect crystal is solved, and that we transform the dynamics of an electron under the influence of an external potential to an electron in free space with renormalized properties. The basic assumption or approximation is that the electron moves entirely within the states of a single band. This approach is named the effective Hamiltonian theory or approximation. This is a reasonable approximation for the case where a potential that is nearly 101

5 Electron dynamics in crystals

102

E

Wavevector k

Figure 5.1

Dynamics of a crystalline electron in a slowly varying ﬁeld. A slowly varying potential moves an electron in a state with wavevector k to nearby states in the same band. constant in space and smoothly varying in time moves the electron adiabatically between states of nearly the same energy without causing transitions to states in another band, as illustrated in Fig. 5.1. Electron dynamics is best discussed in terms of localized wavefunctions because we will be thinking in terms of wavepackets. One such set of functions is the so-called Wannier functions.1 Let φnk (r) be Bloch functions of wavevector k in the band n; the Wannier functions are, in the simplest form, defined by 1 −ik·Rj e φnk (r), wn (r − Rj ) ≡ √ N k

(5.2)

where N is the number of unit cells and Rj is a lattice vector. This expression is for a single non-degenerate band. It can be generalized to a band complex. Moreover, there is considerable freedom in defining Wannier functions. Other possible definitions of Wannier functions include adding a well-chosen phase factor eiθk in each term of the sum on the right-hand side of Eq. (5.2) to maximize its localization in real space.2 Wannier functions defined by Eq. (5.2) form a complete set and have the following useful properties: (i)

1 ik·Rj e wn (r − Rj ), φnk (r) = √ N j

(ii)

wn (Ri )|wn (Rj ) = δn n δij ,

(5.3)

(iii) wn (r − Rj ) is localized about Rj . 1 G. H. Wannier, “The structure of electronic excitation levels in insulating crystals,” Phys. Rev. 52(1937), 191. 2 N. Marzari and D. Vanderbilt, “Maximally localized Wannier functions for composite energy bands,” Phys.

Rev. B 56(1997), 12847.

103

5.2 Electron dynamics in the eﬀective Hamiltonian approach

n

(r – Rj)

r Rj

Figure 5.2

Schematic diagram of a Wannier function localized around the lattice site Rj . The Wannier functions are therefore an orthonormal set of localized functions in real space that span the same functional space as the Bloch states. We have used the Dirac bra– ket notation above. A real-space picture of a Wannier function, given by Eq. (5.2) and computed with planewave Bloch functions, is illustrated in Fig. 5.2.

5.2 Electron dynamics in the eﬀective Hamiltonian approach We now consider the motion of an electron described by Eq. (5.1) in the effective Hamiltonian approximation. It is most easily discussed in the notation of the state vector |ψ(t) for the electronic state. Mathematically, |ψ(t) is just a vector in Hilbert space. It can be expanded in any complete set of “basis” functions that spans the Hilbert space. In particular, the Bloch states |φnk , the position states |r, or the Wannier functions |wn (R) may all be used as separate sets of such basis functions. For the three sets of basis functions of interest here, completeness of each set of functions gives |φnk φnk | 1= nk

=

|r r|

(5.4)

r

=

wn (Rj ) wn (Rj ) . nRj

For example, we may express |ψ(t) =

r

|r r| ψ(t) =

r

ψ(r, t) |r

(5.5)

104

5 Electron dynamics in crystals

in expanding the state vector in the basis set of |r, called the r-representation. Here we have denoted the expansion coefficients ψ(r, t) ≡ r|ψ(t) |r. This is just the real-space wavefunction ψ(r, t) in elementary quantum mechanics as given in Eq. (5.1). The state vector can equivalently be expanded in the basis set of Bloch states |φnk , and in the Bloch representation we have |ψ(t) =

|φnk φnk |ψ(t)

nk

≡

ψn (k, t)|φnk ,

(5.6)

nk

where we have denoted the expansion coefficients φnk |ψ(t) |r as ψn (k, t). Similarly, in an expansion in Wannier functions, we have |ψ(t) =

|wn (Rj )wn (Rj )|ψ(t)

nRj

≡

ψn (Rj , t)|wn (Rj ),

(5.7)

nRj

with ψn (Rj , t) ≡ wn (Rj )|ψ(t) |r denoting the expansion coefficients in the Wannier representation. We would now like to derive a more simplified equation of motion for the state vector |ψ(t), starting with ∂|ψ , (5.8) H|ψ = ih¯ ∂t where H = H0 + U(r) is the Hamiltonian operator. Since U(r) is slowly varying in r and t, we assume that the motion of the electron is well approximated by the Bloch states within a single band. Let us call this the nth band. Then Eq. (5.7) in the effective Hamiltonian approach is taken to be well approximated by |ψ(t) =

ψn (Rj , t)|wn (Rj ).

(5.9)

j

The sum is now restricted to Wannier functions of a single band of index n. Combining Eqs. (5.5) and (5.9), we see that ψ(r, t) =

ψn (Rj , t)wn (r − Rj ).

(5.10)

j

The time evolution of the wavefunction ψ(r, t) is then equivalently given by the time evolution of ψn (Rj , t). In this form, we see that the electron wavepacket (as a solution to Eq. (5.1)) can be viewed as a set of Wannier functions convoluted by an envelope function that depends only on the lattice site index Rj . The electron function ψ(r, t) may have a lot of internal structure, but as far as the dynamics of the wavepacket are concerned, we

5.2 Electron dynamics in the eﬀective Hamiltonian approach

105

only need to know the dynamics of the envelope function (or the wavefunction in the Wannier representation), i.e. the time evolution of ψn (Rj , t) with respect to the crystal lattice positions. We therefore need to develop quantum operators in the Wannier representation. pop operators that have the properties We start with the usual position rop and ) momentum * rop |r = r |r , pop |p = p |p, and pop , rop = −ih, ¯ and define the operators Rop and kop using the relations kop |φn,k ≡ k|φn,k and Rop |wn (Rj ) ≡ Rj |wn (Rj ).

(5.11)

Then, it is straightforward to show that Rop and kop form a conjugate pair of dynamical variables with [kop , Rop ] = −i, Rop = i and kop = −i

(5.12)

∂ , ∂k

(5.13)

∂ . ∂Rj

(5.14)

We now consider the action of a slowly varying potential U(r) on a Wannier function. Since the potential is position dependent, it is well-defined as an operator acting on a function that is dependent on r. We may express the Wannier function in the r-representation and obtain Uop |w(Rj ) = Uop

|rr|w(Rj ) =

r

U(r)|rr|w(Rj ).

(5.15)

r

Since r|w(Rj ) is a very localized function around the point Rj , and U(r) is very slowly varying in the scale of the spacing of the R’s, we may write

Uop w(Rj ) ∼ |rr|w(Rj ) = U(Rj )|w(Rj ). = U(Rj )

(5.16)

r

Equation (5.16) gives a great simplification to Eq. (5.8). Using the single-band approximation, Eqs. (5.13) and (5.14), H0 |ψ ∼ =

k

En (k)φn,k |ψ|φn,k =

Rj

∂ En −i w(Rj )|ψ |w(Rj ). ∂Rj

(5.17)

Equation (5.8) can now be rewritten in the Wannier representation, within the slowly varying potential regime, as ∂ ∂ En −i ih¯ + U(R) ψ(R, t)|w(R) = ψ(R, t)|w(R), ∂R ∂t R

R

(5.18)

5 Electron dynamics in crystals

106

where, for simplicity, we have dropped the index j on the lattice positions. We then have an effective equation for the wavepacket envelope function ∂ ∂ + U(R) ψ(R, t) = ih¯ ψ(R, t). En −i ∂R ∂t

(5.19)

Effectively, we have the following Hamiltonian for considering the dynamics of the crystal electrons: ∂ + U(R) (R-representation) (5.20) Heff = En −i ∂R or

∂ Heff = En (k) + U i ∂k

(Bloch representation).

(5.21)

Within this formalism, by making use of the slowly varying potential approximation, we have eliminated the electron coordinates r from the problem, and hence all the details of the electron’s interactions with the crystal. The effects of the crystal on the behavior of the electron are incorporated completely in the band structure term in Eq. (5.20). The electron behaves as if it moves only in the potential U(R) but with a renormalized kinetic energy operator in Eq. (5.20) or Eq. (5.21). Making a connection to the usual electron wavefunction, we have ψ(R, t)wn (r − R) (5.22) ψ(r, t) = R

if Eq. (5.20) is used, and ψ(r, t) =

ψ(k, t)φnk (r)

(5.23)

k

if Eq. (5.21) is used. The two forms are completely equivalent; which one to use is a matter of computational or conceptual convenience. The effective Hamiltonian approach is expected to be a good approximation if the spatial and temporal variations of U are such that (a) (∇U) · d is much less than the bandwidth where d is an interatomic distance, and (b) hω ¯ is much less than the interband energies where ω is the time variation frequency of U. Under these conditions, a state initially composed of Bloch states within one band will not mix with states of other bands under the influence of the potential U. The robustness of the approach is illustrated schematically in Fig. 5.3 using a constant applied electric field as an example. The quality U(r) is the difference between the exact external potential and the piece-wise constant potential taken at the lattice sites where the Wannier functions are located. We see that U is small (∼eEd) and oscillatory. The largeness (diverging at large distances) of the perturbation is entirely captured in U(R). Moreover, since U is periodic, its effects may in fact be included by redefining the Bloch and Wannier functions as solutions to a new band structure problem, i.e. a periodic crystalline Hamiltonian with U included. Of course, the effects of U in the Wannier functions in Fig. 5.3 are real physical effects that were left out of the theory, e.g. those related to polarization.

5.3 Shallow impurity states in semiconductors

107

(a)

i (r) n

Wannier function

i–1 n

≡

– Ri)

n (r

r i n

r i+1 n

r Ri–1

External and cell average potentials

(b)

Ri

Ri+1

U (r) = –e ε · r Ũ (r) = –e ε · R(r) r Ri–1

Ri

Ri+1

Difference in potential

(c)

Figure 5.3

ΔU (r) = U (r) – Ũ (r) r Ri–1

Ri

Ri+1

Schematic of Wannier functions (a) at diﬀerent lattice sites Rj and (b) the potential due to a uniform electric ﬁeld and ˜ is a piece-wise constant function that takes the value of the ˜ (c) the diﬀerence between U(r) and U(r). Here R(r) closest value of Rj at a given position r.

5.3 Shallow impurity states in semiconductors A good example of an application of the effective Hamiltonian approach is its use in determining the shallow impurity states in semiconductors. Let us consider the simple case of a substitutional impurity (with an extra valence electron from the impurity atom) in a semiconductor that has an isotropic and parabolic conduction band. This would be, for example, the case of Si in GaAs replacing one of the Ga atoms. The extra electron would be attracted to the Si site and in a state that is expected to be comprised of states from the conduction band only (see Fig. 5.4). We use the single-band approximation and write the impurity wavefunction in terms of the conduction band states: ψ(k, t)φck (r) ψ(r, t) = k

=

R

ψ(R, t)wc (r − Rj ),

(5.24)

108

5 Electron dynamics in crystals

E Conduction band Donor state Eg

Valence band Wavevector k

Figure 5.4

Diagram of a shallow donor state in a direct gap semiconductor with a bandgap Eg separating the valence band from the conduction band. where φck (r) and wc (r − R) are the conduction band Bloch functions and Wannier functions, respectively. The conduction band dispersion relation measured from the top of the valence band, assuming an isotropic and parabolic form, is given by Ec (k) = Eg +

h¯ 2 k2 , 2m

(5.25)

where Eg is the bandgap and m∗ is a parameter describing the band curvature. Application of Eq. (5.20) leads to the following effective Schr¨odinger equation for the wavefunction in the Wannier or R-representation, assuming a Coulomb interaction (screened by the dielectric constant of the material) between the additional electron and the positively charged impurity core site, 2 e h¯ 2 2 (5.26) ψ(R) = (E − Eg )ψ(R). − ∇ + − 2m R This leads to the hydrogenic model for shallow impurity states in the bandgap near the conduction band of semiconductors given in elementary treatments. Table 5.1 compares the calculated results using the effective Hamiltonian (or effective mass) model with experimental impurity levels.

5.4 Motion in external ﬁelds We now proceed to analyze the motion of crystal electrons in an external field using the formalism developed in Section 5.2. The equation of motion for the operators Rop and kop may be obtained using the usual relation from quantum mechanics for operator A, ∂A 1 dA = + [A, H]. dt ∂t ih¯

(5.27)

5.4 Motion in external ﬁelds

109

Table 5.1 Binding energies Eb of the ground (1s) state of shallow donor impurities in some common semiconductors, comparing experimental data with results from the eﬀective Hamiltonian or eﬀective mass theory. The symbol XY denotes that the element Y in the host material is substitutionally replaced by an impurity atom X. (After Cardona and Yu, 2010.)3 Semiconductor

Theory Eb (meV)

GaAs

5.72

InSb CdTe

0.6 11.6

ZnSe

25.7

Experiment Eb (meV) SiGa : 5.84 GeGa : 5.88 SAs : 5.87 SeAs : 5.79 TeSb : 0.6 InCd : 14.0 AlCd : 14.0 AlZn : 26.3 GaZn :27.9 FSe : 29.3 ClSe : 26.9

Using the effective Hamiltonian in Eqs. (5.20) and (5.21), we obtain for the operator R the following equation of motion:

ih¯

dR = [R, Heff ] dt ∂ + U(R) = R, En −i ∂R ∂ = R, En −i ∂R ∂ = i , En (k) ∂k ∂ ∂ En (k) − En (k)i ∂k ∂k ∂ En (k) . =i ∂k =i

(5.28)

3 P. Y. Yu and M. Cardona, Fundamentals of Semiconductors: Physics and Materials Properties, 4th ed. (Berlin:

Springer, 2010).

5 Electron dynamics in crystals

110

Thus, the velocity operator v is given by v=

dR 1 ∇ k En (k) . = h¯ dt

(5.29)

Note that v does not depend on the form of the perturbation U. It is a general property of the electronic band structure. For k, again using Heff , we obtain the equation of motion ih¯

dk = [k, Heff ] dt ∂ = k, U i ∂k ∂ , U(R) = −i ∂R = −i (∇R U(R))

(5.30)

or

dk = −∇ R U(R). dt Since −∇U(R) is the force F on the electron, we have h¯

h¯

(5.31)

dk = F. dt

(5.32)

For the special case of a constant force F, Eq. (5.32) can be integrated immediately to t k(t) = k(t = 0) + F . h¯

(5.33)

With Eqs. (5.29) and (5.31), we can follow the motion of an electron starting at t = 0 in any individual Bloch state with wavevector k0 , or of a wavepacket centered about a given k0 . For example, consider a crystal with the band structure given in Fig. 5.5 in a uniform electric field E = εxˆ . The wavevector of a state with initial wavevector at k0 = 0 at t = 0 will change according to Eq. (5.33) to k(t) = − The group velocity is given by hv ¯ x= in the position of the particle as x(t) =

t

∂En ∂kx

1 = (−|e|ε)

(5.34)

(see Fig. 5.6), which leads to a time dependence

dt ∂En dkx 0 0 dkx ∂kx 1 2 [En kx (t)) − En (kx (t = 0) ].

vx (t)dt =

0

|e|εt xˆ . h¯

t

dt ∂En 1 = h¯ ∂kx h¯

t

(5.35)

5.4 Motion in external ﬁelds

111

E

C′

C

B′

B A

–G/2

G/2

0

G

Wavevector kx

Figure 5.5

Schematic of a band structure in a repeated zone scheme along the kx direction, where G is the smallest reciprocal lattice vector along this direction.

x

B′

A

B kx

–G/2

Figure 5.6

0

G/2

G

Group velocity vx as a function of kx for the lower band in Fig. 5.5.

x

0

Figure 5.7

t

Δ xmax =

W eε

Schematic of x(t) of a crystalline electron in a uniform ﬁeld which shows Bloch oscillation where W is the band width.

Physically, what these equations tell us is that the wavepacket’s center of mass wavevector in k-space and its center of mass in real space are changing (due to the interaction with the field) as a function of time. When the center of mass wavevector reaches the Brillouin zone boundary, the wavepacket is Bragg-reflected, leading to an oscillatory behavior in r(t) as illustrated in Fig. 5.7. As a consequence, in this idealized situation, there is no net current for a perfect crystal. However, for real materials, impurities and zero-point motions of various excitations will introduce scattering that would give rise to a net current even at temperature T = 0. The oscillations in the motion of the electrons given by Eq. (5.35) are called Bloch oscillations. Observation of these oscillations requires that the electron travel many periods

5 Electron dynamics in crystals

112

E

Band 2

eε

Eg Band 1

x

W

Δ xmax =

Figure 5.8

W eε

d=

Eg

eε

Semiclassical picture of Bloch oscillations with E an applied uniform electric ﬁeld and W the bandwidth.

without being scattered. The distance traveled in half of a period is given by

xmax =

W , |eε|

(5.36)

where W is the bandwidth. Under normal conditions, with an electric field of the order of V/mm and W ∼ few eV, xmax ≈ a few mm, making the Bloch oscillations unobservable for usual samples since the mean free path of the electrons is significantly shorter. Bloch oscillations, however, have been observed in man-made periodic systems, such as semiconductor superlattices and atoms in optical lattices, where the large unit cell dimensions reduce W to small values.4 The Bloch oscillation phenomenon may also be understood in a semiclassical picture as illustrated in Fig. 5.8. In a slowly varying potential, the electron in a state at the band extrema effectively runs into a triangular potential barrier with width d that is determined by the bandgap to the next band and by the electric field strength. The electron wave is reflected at the barriers, giving rise to the oscillations. There is, however, a finite probability for tunneling to the next band if |E| is large enough (i.e. if the barrier is thin enough), leading to phenomena such as Zener tunneling (see Fig. 5.9). Interband transitions are, however, not included in the present effective Hamiltonian formalism, since it is assumed that the wavefunction is always made up of states from a given band or band complexes.

4 See, for example, M. Raizen, C. Salomon, and Q. Niu, “New light on quantum transport,” Phys. Today

50(1997), 30.

5.5 Eﬀective mass tensor

Energy

113

Wavevector k

Figure 5.9

Schematic of Zener tunneling with an electron tunneling from the lower band to the upper band under the inﬂuence of a strong external ﬁeld.

5.5 Eﬀective mass tensor In the example in Figs. 5.5 and 5.6, under the influence of a force F, the wavevector k(t) of an electron changes as a function of time. The velocity of the electron v goes to zero and then changes sign as k crosses the Brillouin zone edge under a constant force. The electron appears as if it has a mass that is a function of k and becomes negative near the top of the band. This leads us to define the useful concept of the effective mass tensor in electron dynamics (discussed previously in Chapter 3). As in classical mechanics, mass is defined by F = ma or, more generally, 1 Fβ = aα . (5.37) m∗ αβ β

Since from Eq. (5.29), 1 d ∂E dvα 1 ∂ 2 E dkβ = , = dt ∂kα ∂kβ dt h¯ dt ∂kα h¯ β and from Eq. (5.32)

dk dt

(5.38)

= Fh¯ , we have aα =

1 β

∂ 2E Fβ . h¯ 2 ∂kα ∂kβ

The effective mass tensor is thus given by 1 1 ∂ 2E = 2 . ∗ m αβ h¯ ∂kα ∂kβ

(5.39)

(5.40)

The form and properties of the effective mass tensor play an important role in determining the transport properties of materials, especially those of carriers in semiconductors. In semiconductors, one is mainly dealing with carriers (either electrons or holes) near band extrema, which typically occur near a symmetry point k0 in the Brillouin zone, e.g.

5 Electron dynamics in crystals

114

at k0 equal to the point for GaAs. There is a way, as discussed in Chapter 3, that allows one to determine the nearby band structure and the effective mass tensor given that we know the energy states at a given point k0 . The method makes use of the knowledge of the electron band structure at a given point of k-space to find the states nearby, and the effective mass tensor, in the so-called k · p perturbation theory, resulting in, for the nth band,

1 m∗

n,αβ

pαn n pnn 1 ∂ 2 En 1 2 β δαβ + = 2 = m m En (k0 ) − En (k0 ) h¯ ∂kα ∂kβ n αβ 1 δαβ + fnn . = m

(5.41)

n

We have used the notation pαn n = n k0 |pα |nk0 and defined the quantity f through the second line of Eq. (5.41).

5.6 Equations of motion, Berry phase, and Berry curvature The equation of motion given in Eq. (5.29) is incomplete when we consider the effects of geometric or Berry phase5 on the motion of crystal electrons. In the effective Hamiltonian approximation, an electron in a Bloch state |nk with wavefunction r|nk = ψnk (r) = eik·r unk (r)

(5.42)

is constrained to move within a single band n. In the presence of a slowly varying static potential U(r), the electron will adiabatically drift in k-space along a path C (see Fig. 5.10). Denoting the electron to initially be in the state |ψ(t = 0) = |nk(0), then at some later time t, the state of the electron will evolve into the state |ψ(t), which within the effective Hamiltonian approximation is |nk(t) apart from a phase factor according to the adiabatic theorem of quantum mechanics.6 (Here |nk(t) is given by Eq. (5.42).) The phase factor that relates |ψ(t) to |nk(t) may be determined by the following analysis. The cell periodic part of a Bloch wavefunction |unk satisfies the equation

(p + hk) ¯ 2 + V(r) unk (r) = En (k)unk (r), 2m

(5.43)

or H(k) |unk = En (k) |unk .

(5.44)

5 M. V. Berry, “Quantal phase factors accompanying adiabatic changes,” Proc. R. Soc. Lond. A 392(1984), 45. 6 See, for example, Chapter 10 in D. J. Griffiths, Introduction to Quantum Mechanics, 2nd edn. (Upper Saddle

River, NJ: Prentice Hall, 2005).

5.6 Equations of motion, Berry phase, and Berry curvature

115

2π b

Ωn (k)

γn

ky

C 0

Figure 5.10

unk

kx

2π a

Berry curvature in k-space. Here |unk is the periodic part of a Bloch state and n (k) is the Berry curvature of band n. C denotes a closed loop over which an electron in the nth band picks up a Berry phase of γn .

We shall use the solutions |unk in Eq. (5.44) as an instantaneous orthonormal basis to expand |ψ(t). Equation (5.44) allows, however, an arbitrary k-dependent phase factor of |unk . To remove this arbitrariness, we make a phase choice, or a gauge, that requires the phase of |unk to be smooth and single-valued along the path C in the parameter or k-space. Treating k(t) as a parameter along the path C, the periodic part of the state of the electron (denoted by φ(r, t) ≡ e−ik·r ψ(r, t)) evolves according to the time-dependent Schr¨odinger equation d (5.45) H k(t) |φ(t) = ih¯ |φ(t) . dt Adiabatically, a system prepared in |nk(0) will evolve with H k(t) and therefore be in the state |nk(t) at t. So, |φ(t) can be expressed as |φ(t) = exp

−i h¯

t

1 2 dt En k(t ) exp iγn (t) |unk (t) .

(5.46)

0

The first exponential factor on the right-hand side of Eq. (5.46) is the familiar dynamical phase factor. The second exponential contains a phase which is in general non-integrable and cannot be written as a function of k. We determine γn (t) by requiring that |φ(t) in Eq. (5.46) satisfy the time-dependent Schr¨odinger equation. Substituting Eq. (5.46) into Eq. (5.45) leads to the following expression for the time rate of change in γn (t):

dk d γn (t) = i unk(t) ∇ k unk(t) · , dt dt where

un(k+dkkˆ i ) − |unk

∇ k unk(t) = kˆ i . dk i

(5.47)

(5.48)

116

5 Electron dynamics in crystals

Integrating Eq. (5.47) along the path C from some point k0 with respect to time gives γn (k) = i

k

unk | ∇ k unk · dk .

(5.49)

k0

The normalization of |unk dictates that unk | ∇ k unk = − ∇ k unk | unk , and therefore γn (k) is real. Let us define the Berry vector potential An (k) (or the Berry connection) as the quantity An (k) = i unk | ∇ k unk = −Im unk | ∇ k unk .

(5.50)

We note that A has dimensions of length and is always real, as argued above. The electron’s ket vector |φ(t), during its adiabatic evolution along the path C in parameter space, acquires an extra phase γn (k), in addition to the dynamical phase with

k

γn (k) =

dk · An (k ).

(5.51)

C

The form of Eq. (5.51) reveals that we may regard this phase as an Aharonov–Bohm phase caused by an effective “magnetic field” n (k) = ∇ k × An (k),

(5.52)

which lives in parameter space k. This field n (k) is called the Berry curvature. The Berry vector potential An (k) is gauge dependent. If we make a gauge transformation |unk → eiμ(k) |unk ,

(5.53)

where μ(k) is an arbitrary smooth function of k, then Eq. (5.50) yields An (k) → An (k) − ∇ k μ(k).

(5.54) 1 2 (k) in Eq. (5.51) is gauge dependent, changed by μ k(0) − As1 a consequence, the phase γ n 2 μ k(t) in its value after the gauge transformation. However, for a closed loop C in the parameter space, the extra phase acquired by the state vector |φ after it has traversed the loop back to the starting position 5 dk · An (k) (5.55) γn = C

is gauge invariant and is physically observable. The phase γn in Eq. (5.55) is known as the Berry phase or geometric phase. Although not gauge invariant, γn (k) in Eq. (5.51) is also often loosely referred to as the Berry phase. The1 Berry curvature n (k) defined in Eq. (5.52) is also a gauge-invariant quantity, since 2 ∇ k × ∇ k μ(k) = 0 for any smooth function μ(k). Using Stoke’s theorem, we may rewrite the Berry phase for a closed loop in the form 5 dk · An (k) = ds · n (k), (5.56) γn = C

S

5.6 Equations of motion, Berry phase, and Berry curvature

117

where S is any surface enclosed by the closed loop C. Unlike the Berry vector potential, since it is gauge invariant the Berry curvature is observable. The physical origin of the Berry curvature arises from the adiabatic approximation employed, which is equivalent to a projection operation restricting the dynamics of the system to the nth band. The Berry curvature can be viewed as arising from the residual interaction with states in the bands that are not considered in the effective Hamiltonian. The Berry curvature n (k), an intrinsic local property in k-space of the band structure of a crystal, modifies the motion of the electron. Let us consider the effective Hamiltonian with external potential U(r) in the Bloch representation H = En (k) + U(R),

(5.57)

where R = i∇ k is the Wannier coordinate indexing the lattice sites and En (k) is the unperturbed band structure. We may perform a gauge transformation to remove the effective Aharonov–Bohm phase or Berry phase in Eq. (5.46), at the expense of adding the Berry vector potential An (k) to i∇ k in the argument of U in Eq. (5.57). The transformed Hamiltonian H is then equal to 1 2 H = En (k) + U i∇ k + An (k) .

(5.58)

The position operator in this gauge-transformed system is now given by x = i∇ k + An (k)

(5.59)

and is no longer simply R. As an operator, the components of x do not commute with each other. Their commutation relations are given by ) xi , xj ] = i ijk nk (k),

(5.60)

where ijk is the Levi-Civita symbol in three dimensions. We may now derive the equations of motion with the transformed Hamiltonian H in Eq. (5.58). The equation for dk dt may be obtained using h¯

dk = −i[k, H ] = −∇ R U(R), dt

(5.61)

which is unchanged from Eq. (5.31). However, the equation for the velocity is now given by hv ¯ = −i[x, H ] = ∇ k En (k) + ∇ x U × n (k).

(5.62)

By comparison with Eq. (5.29), there is an extra term involving the Berry curvature. The new term is commonly known as the Luttinger anomalous velocity.7 For example, for a 7 M. C. Chang and Q. Niu, “Berry phase, hyperorbits, and the Hofstadter spectrum,” Phys. Rev. Lett. 75(1995),

1348.

5 Electron dynamics in crystals

118

1 2 crystal in a static electric field E with U(x) = −eE · x and a weak magnetic field B, the semiclassical equations of motion become h¯

e dk = eE + v × B dt c

(5.63)

and hv ¯ = ∇ k En (k) − eE × n (k).

(5.64)

The importance of the contribution of the Berry curvature term to the dynamics of crystal electrons depends on the systems of interest. In many cases, n (k) may be neglected. However, n (k) is nonzero in a wide range of materials, particularly those with broken time-reversal and inversion symmetries, and has given rise to insightful understanding of a number of interesting phenomena, including the anomalous Hall effect, the quantum Hall effect, electric polarization, orbital magnetization, topological insulators, etc. Let us analyze the general form of the Berry curvature n (k) by examining the velocity expression in Eq. (5.64). The velocity expression should be invariant under time-reversal or spatial inversion operations if the crystal has these symmetries. Under time reversal, v → −v, k → −k, and E → E; under spatial inversion, v → −v, k → −k, and E → −E. Thus, if the crystal has time-reversal symmetry, the invariance form shown in Eq. (5.64) dictates that (5.65) n (−k) = −n (k), and, if the crystal has spatial inversion symmetry, n (−k) = n (k).

(5.66)

This leads to the conclusion that, for crystals (such as Al) with both time-reversal and spatial inversion symmetry, the Berry curvature is identically zero throughout the Brillouin zone, with the possible exception of nonzero values at singular points in k-space due to band degeneracy. In such a case, one may use the simpler velocity expression given in Eq. (5.29). For systems with either broken time-reversal or broken spatial inversion symmetry, the proper equation for the velocity should include the Berry curvature term. In ferromagnetic materials, where time-reversal symmetry is broken, such as fcc Fe under a uniform Efield, the Berry curvature term in Eq. (5.64) gives rise to a current that is perpendicular to E and constitutes an intrinsic mechanism for the so-called anomalous Hall effect (in which a strong additional Hall resistivity results from the magnetization) in these materials. Presently, this research area is dynamic and evolving.8

8 See, for example, the review article by D. Xiao, M. C. Chang, and Q. Niu, “Berry phase effects on electronic

properties,” Rev. Mod. Phys. 82(2010), 1959.

6

Many-electron interactions: the homogeneous interacting electron gas and beyond Up until now, we have treated the electronic Hamiltonian of solids as an effective Hamiltonian of independent electrons moving in a mean (or average) field due to the ions and other electrons. This is a very useful conceptual approach and can be quantitative for certain physical properties if the appropriate field or self-consistent potential is used, as we shall see in the next chapter on density functional theory. The proper choice of the mean-field potential V(r) appearing in the one-electron Schr¨odinger equation 4 h¯ 2 2 − ∇ + V(r) ψ(r) = εψ(r) 2m

3

(6.1)

is a complex and subtle issue. Underlying this problem is the question of how best to approximate the effects of electron–electron interactions in the exact Hamiltonian H within the Born–Oppenheimer approximation for physical quantities of interest: H=

i

3

4 p2i 1 e2 + , Vion (ri − R) + 2m 2 |ri − rj |

(6.2)

i=j

R

where Vion (ri − R) is the ionic potential seen by the ith electron. Very often, an effective one-electron Schr¨odinger-like equation of the form Eq. (6.1) is obtained by seeking the ground-state energy and wavefunction of an interacting many-electron system using a variational principle approach. In the Hartree–Fock (HF) treatment, for example, we assume that the ground-state manyelectron wavefunction is of the form of a single Slater determinant: HF (r1 σ1 , r2 σ2 , ..., rN σN )

φ1 (r1 σ1 ) φ1 (r2 σ2 )

1

φ2 (r1 σ1 ) φ2 (r2 σ2 ) =√ .. .. N!

. .

φ (r σ ) φ (r σ ) N 1 1 N 2 2

φ1 (r3 σ3 ) φ2 (r3 σ3 ) .. .

... ...

φN (r3 σ3 ) ...

.

φN (rN σN ) φ1 (rN σN ) φ2 (rN σN ) .. .

(6.3)

Here N is the number of electrons in the system, and ri and σi denote the spatial and spin coordinates of the ith electron, respectively. φλ are single-particle orbitals to be determined in the calculation. Since an electron has spin 12 , σi may be up or down. Applying the variational principle, i.e. demanding the variation of the ground-state energy with respect 119

6 Many-electron interactions: the homogeneous interacting electron gas and beyond

120

to any of the single-particle orbitals φλ to be zero, δ HF |H| HF =0 δφλ

(6.4)

leads to the Hartree–Fock equations −

h¯ 2 2 ∇ φi (r, σ ) + Vion (r)φi (r, σ ) + VH (r)φi (r, σ ) 2m + Vx (r, r , σ , σ )φi (r , σ )dr = εi φi (r, σ ),

(6.5)

σ

where VH (r) =

e2

2 φ dr (r , σ ) , j |r − r | occ

σ

(6.6)

j

and Vx (r, r , σ , σ ) = −

occ j

e2 φ ∗ (r , σ )φj (r, σ ). |r − r | j

(6.7)

Equations (6.5)–(6.7) need to be solved self-consistently (i.e. iteratively). The Hartree– Fock equations differ from the Hartree equations by an additional term Vx on the left-hand side of Eq. (6.5), known as the exchange term. The exchange term arises from the antisymmetric form of the many-fermion wavefunction, which introduces an effective interaction between electrons owing to the Pauli exclusion principle. It is a nonlocal operator of the integral form when acting on a single-particle orbital φi (r, σ ), i.e. (6.8) Vx (r, r , σ , σ )φi (r , σ )dr , σ

which, in general, is rather difficult to treat quantitatively. The eigenvalue εi in the Hartree–Fock equation (Eq. (6.5)) is a Lagrange multiplier in the variational procedure, constraining the normalization of the single-particle orbitals. Thus, rigorously speaking, they are not electron excitation energies of the system. However, through the use of Koopmans’ theorem, these eigenvalues may be roughly interpreted as electron excitation energies to lowest order in the Coulomb interaction. (We will leave the proof of Koopmans’ theorem as a homework exercise for the interested reader.) The Hartree–Fock method, being a ground-state theory, provides an important first step in treating the effect of electron–electron interactions on the ground-state properties of condensed matter, such as the total energy, and structural and vibrational properties. In particular, the Hartree–Fock equations may be solved exactly for the case of the homogeneous interacting electron gas. In the remainder of this chapter, we shall examine the effects of many-electron interactions on the electronic properties of the electron gas as well as simple metals within the Hartree–Fock approximation and beyond.

6.1 The homogeneous interacting electron gas or jellium model

121

6.1 The homogeneous interacting electron gas or jellium model An important model system that illustrates the role of many-electron interactions in solids without having to deal with the complexity of the atomic structure is that of the uniform interacting electron gas or the jellium model. In this model, we consider a system of interacting electrons in a uniform positive-charged background so that the total system is neutral. The jellium model is then an idealized metal for which we can study the effects of electron interactions on the total energy, electron (or quasiparticle) excitations, and other properties as a function of electron density. In the zero-order approximation, we neglect electron–electron interactions; the jellium model reduces to that of a non-interacting charged Fermi gas, i.e. the Sommerfeld model. In the non-interacting limit, the Hamiltonian can be written as H0 =

p2 i + VPB = Hi0 , 2m i

(6.9)

i

where VPB is the potential due to the positive background. For an N electron paramagnetic system, we may take the ground-state wavefunction to be in the form 0 =

N 6

φi (ri , σi ),

(6.10)

i=1

with 1 0 (r) = √ eik·r χλ , φi (r, σ ) = φkλ

(6.11)

where is the volume of the sample and χλ is a spin function with λ = ↑ or ↓. The value of k is within the Fermi sphere, i.e. k ≤ kF , with kF the Fermi wavevector defined through N=2

1,

(6.12)

k≤kF

where the factor 2 is due to spin, and the orbital energy is independent of λ given by ε0 (k) =

h¯ 2 k2 . 2m

The total energy of the system is E0 = 2

ε0 (k).

(6.13)

k≤kF

The jellium model has only one variable physical parameter, the density of the electrons N n= or kF = (3π 2 n)1/3 in the paramagnetic phase. In the study of the interacting electron

122

6 Many-electron interactions: the homogeneous interacting electron gas and beyond

gas, it is often useful to express physical quantities in terms of another related parameter rs (the typical interelectron distance in units of the Bohr radius a0 ): rs =

3 4π

1 1 3 1 3 −1 a0 . n

(6.14)

The dimensionless parameter rs is known as the electron gas parameter and may be viewed as the effective radius of the volume occupied by the electron in units of the Bohr radius. In the literature, the density dependence of physical quantitites is traditionally expressed in terms of rs . For example, the Fermi wavevector kF = 1.92/rs (a−1 0 ), the Fermi energy 3/2 2 2 0 2 EF = h¯ kF /2m = 3.68/rs (Ry), and the plasma frequency hω ¯ p = 3.46/rs (Ry). Here Ry denotes the energy unit of one Rydberg. In the Sommerfeld model, the average kinetic energy per electron, EKE , is given by EKE =

2 0 3 2.21 εk = E0F = 2 (Ry). N 5 rs

(6.15)

k 1 corresponds to one with low density and dominant potential energy. Since rs is a measure of the ratio of the Coulomb energy to the kinetic energy of the electron gas, we may use it as a small parameter (if rs is small) to do perturbation theory to determine the effects of Coulomb interaction on the properties of the electron gas. However, real materials typically have values of rs between 1 and 5 so that EKE ∼ EPE , making the system strongly interacting, and making it difficult to apply traditional perturbation theory. Figure 6.1 illustrates the range of rs . The importance of treating many-electron effects going beyond Hartree–Fock will generally depend on rs and the dimensionality of the system under consideration. For example, in three dimensions and for rs > 100, electron correlation is so strong that the electrons crystallize into a crystalline arrangement forming an electronic lattice (the Wigner crystal).1 As we will see below, one can determine the exact correlation energy in the limit of extremely large rs .

1 E. Wigner, “On the interaction of electrons in metals,” Phys. Rev. 46(1934), 1002.

6.2 Hartree–Fock treatment of the interacting electron gas

123

KE

KE

PE

PE

10

1

100 rs

Real materials

Figure 6.1

3D Wigner e– crystal

Schematic of the range of the electron gas parameter rs on log scale showing the ranges where the kinetic energy (KE) dominates over the potential energy (PE) and vice versa. Typical metals in three dimensions have rs between 1 and 6. At extremely high rs , the electrons form a Wigner lattice.

6.2 Hartree–Fock treatment of the interacting electron gas To gain some insight into electron interaction effects, we solve the uniform interacting electron gas problem analytically within the Hartree–Fock approach. We shall assume that the single-particle orbitals in Eq. (6.3) are planewaves times a spin function, i.e. the orbitals are specified by the quantum numbers k and λ with 1 φiHF = φkλ = √ eik·r χλ ,

(6.17)

1 2 1 2 where χλ is the spin function 10 for λ = ↑ and 01 for λ = ↓, and show that φkλ are the solutions of the self-consistent Hartree–Fock equations (6.5)–(6.7). We note that planewave solutions result in a uniform electron charge density. This results in Vion (r) + VH = 0, since the electron charge density cancels the positively charged background density. Only the exchange term Vx given by Eq. (6.7) survives among the potential energy terms in Eq. (6.5). Equation (6.5) reduces to h¯ 2 − ∇ 2 φi (r, σ ) + 2m

Vx (r, r , σ , σ )φi (r , σ )dr = εi φi (r, σ ).

(6.18)

σ

Substituting in φi from Eq. (6.17), we have e2 1 h¯ 2 k2 dr φkλ (r) − 3/2 e−ik ·r eik ·r eik·r δλ λ χλ = ελ (k)φkλ (r). | 2m |r − r k ωp , the corresponding equations are 1 (ω) = 1 −

ωp2 τ 2 1 + ω2 τ 2

> 0,

(9.41)

with k(ω) → 0

(9.42)

and n(ω) =

√

1 → 1,

(9.43)

which implies that the metal is transparent. Figure 9.3 summarizes these results with a plot of 1 − R(ω) vs. ω. The abrupt increase in the transmission (since k(ω) = 0 in this high ω range) near ωp , as shown in Fig. 9.3, is an excellent experimental measure of the plasma frequency. For the Hagen–Rubens region, we can also estimate other relevant properties. The absorption coefficient η = 2ωk c becomes very large because ωp τ k(ω) = √ . 2ωτ 2 The relation was discovered by Ernst B. Hagen and Heinrich Rubens in 1903.

(9.44)

9 Electronic transitions and optical properties of solids

192

log10 (1 – R(ω))

0

–2

–4

I

II

III

ω

–6 ωp

1/τ

Incident light frequency ω

Figure 9.3

Frequency dependence of log10 (1 − R(ω)) within the Drude theory.

Also, the EM wave skin depth √ c c 2ωτ δ= = ωk ω ωp τ can be related to the dc conductivity σ1 (0) =

ne2 τ m ,

(9.45)

and we have

1 c ∼ ω− 2 . δ=√ 2π σ1 (0)ω

(9.46)

Hence, the simple Drude model, which is based on intraband transitions arising from scattering centers, gives the essential features of the optical properties of simple metals.

9.3 The transverse dielectric function As discussed in Section 9.1, when examining the physics of optical properties, the appropriate dielectric function to use for determining response functions for transverse EM probes is the “transverse dielectric function.” In our previous discussions, in Chapter 8 for example, we considered a longitudinal field with q E, because we assumed that ∇ 2 φ = −4π δρ ⇒ ∇ · E = −4π δρ.

(9.47)

As q → 0, this approximation is acceptable for transverse EM waves in a cubic or homogeneous system. However, more generally for an optical response, we need to consider a current–current response function derivation of the self-consistent field dielectric function.

9.3 The transverse dielectric function

193

For an EM field E(ω), the current density is given by ji = σij Ej ,

(9.48)

j

where the conductivity tensor can be shown from perturbation theory: σij = −i

e2 h¯ 2 f0 (Enk ) − f0 (En k ) n k |∇i |nknk|∇j |n k , m2 ω En k − Enk − hω ¯ − iη

(9.49)

nk n k

where η = 0+ . Using the relation (with η = 0+ ) 1 1 =P − iπ δ(x), x + iη x

(9.50)

we obtain Reσij =

π e2 h¯ 2 k ) n k ∇i |nk nk| ∇j n k δ(En k − Enk − hω). f (E ) − f (E ¯ 0 0 nk n 2 m ω nk n k

(9.51) This is the Kubo–Greenwood expression3 for the real part of the conductivity, which can be derived using different methods. Note that this formula is very general for quantum systems. For example, nk need not be band states. Using Eq. (9.14), the diagonal part of →

Eq. (9.51) yields (ˆe = unit vector E ) 4π ↔ Re eˆ · σ · eˆ ω

4π 2 e2 h¯ 2 k ) |n k |∇ · e f = (E ) − f (E ˆ |nk|2 δ(En k − Enk − h¯ ω). 0 0 nk n m2 ω2

2 (ω) =

nk n k

(9.52) Note that 2 (ω) now depends on eˆ . For a cubic system, we may write

| n k eˆ · ∇ |nk|2 = 13 | n k ∇ |nk|2 ,

(9.53)

which is independent of eˆ . Fermi’s golden-rule derivation of 2 (ω). We may arrive at the expression in Eq. (9.52) using perturbation theory. In a perturbing EM field, 1 1 |e|A(ri ) 2 pi + H= + eφ(ri ) + V(ri ) = H0 + H1 , (9.54) 2 m c i

i

i

3 R. Kubo, “Statistical-mechanical theory of irreversible processes I: General theory and simple applications

to magnetic and conduction problems,” J. Phys. Soc. Japan 12(1957); D. A. Greenwood, “The Boltzmann equation in the theory of electrical conduction in metals,” Proc. Phys. Soc. 71(1958), 585.

9 Electronic transitions and optical properties of solids

194

with H0 the unperturbed Hamiltonian, and H1 =

1 |e| 1 e2 2 A (ri ) + (pi · A(ri ) + A(ri ) · pi ) + 2 eφ(ri ). 2c m 2c m i

i

(9.55)

i

If we choose the Coulomb gauge ∇·A=0

(9.56)

φ = 0,

(9.57)

and

then we can write for the ith electron (in the limit of small A) |e|h¯ |e|h¯ e2 2 A (ri ) A(ri ) · ∇ i − i ∇ i · A(ri ) + 2mc 2mc 2mc2 |e|h¯ |e| A(ri ) · ∇ i = A(ri ) · pi . ≈ −i mc mc

˜ i1 = −i H

(9.58)

For an EM wave of the form A=

A0 i(q·r−ωt) [e − e−i(q·r−ωt) ], 2

(9.59)

we have E=−

1 ∂A c ∂t

(9.60)

or A=

c E. iω

˜ i = Hi + Hi∗ , with Therefore, H 1 1 1 Hi1 =

−|e|h¯ i(q·r−ωt) E 0 e · ∇. mω 2

(9.61)

We can now use Fermi’s golden rule to derive 2 (ω) for insulators. For absorption for insulators at T = 0, the absorption coefficient η is defined through

η≡

− dI energy absorbed/time–volume = 1 cdt2 , incident energy/area–time I n

(9.62)

where the incident energy is I ∼ e−2x/δ ,

(9.63)

9.3 The transverse dielectric function

195

(a)

(b) Conduction band t nk

ħω

nk

Figure 9.4

Photon

Valence band

Direct optical absorption process in an insulator. (a) Feynman diagram. (b) Band diagram. where δ is the distance over which E is reduced by 1e . Using dI −dI dx 2I c − = = , dt dx dt δ n

(9.64)

we obtain, using Eqs. (9.63), (9.16), and (9.18), − dI 2kω ω 2 η = 1 cdt2 = = = 2 . δ c nc I n

(9.65)

If we define Wtot (ω) ≡ number of photons absorbed/volume–time, then the energy absorbed/time–volume = Wtot (ω)hω. ¯ Hence, for an EM wave of the form in Eq. (9.59), 1 (nE0 )2 , which has energy density u = 8π c energy incident 1 = uv = (nE0 )2 area–time 8π n ncE20 = , 8π

(9.66)

and η=

8π hω ¯ Wtot (ω) ncE20

(9.67)

This gives 2 (ω) =

8π h¯ Wtot (ω). E20

(9.68)

We may now obtain 2 (ω) from Eq. (9.68) by considering the transition rate from (nk) → (n k ), 2π |n k |H1 |nk|2 δ(Enk − Enk − hω)(f ¯ nk − fn k ) h¯

2

π h¯ e2 E20

eˆ · Mnn (k, k )

δ(En k − Enk − hω)(f = ¯ nk − fn k ),

2 2 2m ω

w(nk → n k ) =

(9.69)

9 Electronic transitions and optical properties of solids

196

with M an interband transition matrix element from H1 . (See Section 9.4.) Wtot is the sum of all possible (nk → n k ), and we obtain Eq. (9.52) from Eq. (9.68).

9.4 Interband optical transitions in semiconductors and insulators For insulating crystals, the interband matrix element M in Eq. (9.69) may be evaluated using Eq. (9.61), H1 =

1 eh¯ E0 ei(q·r−ωt) eˆ · ∇, 2 mω

(9.70)

and we have

Mnn (k, k ) ≡ n k eiq·r ∇ |nk = u∗n k e−ik ·r eiq·r ∇(unk eik·r )d3 r = u∗n k (r)e−i(k −q−k)·r (∇ + ik)unk (r)d3 r.

(9.71)

Since u is a periodic function, Eq. (9.71) gives the result that M is zero unless k − q − k = G.

(9.72)

This is the origin of the selection rule of conservation of crystal momentum. For q ∼ 0, k ∼ k, we have 2 (ω) =

4π 2 e2 h¯ 2 |ˆe · Mvc (k)|2 δ(Ec − Ev − hω). ¯ m2 ω2 vc

(9.73)

k

Here v denotes the occupied valence bands and c the empty conduction bands. The real part of the dielectric function 1 (ω) can be obtained using the Kramers–Kronig relation. We now introduce the joint density of states J(E) in analogy with the usual density of states g(E) that is given for a paramagnetic system by ( is the sample volume) g(E) =

2 1 δ(E − Enk ) = (2π )3

d3 kδ(E − Enk ).

(9.74)

nk

The integral for 2 (ω) is over equal-energy-difference surfaces in k-space defined by Eck − Evk − hω ¯ = 0. In many cases, eˆ ·Mvc can be assumed to be a slowly varying function of k (except for the case M = 0 at some k-point, due to symmetry), and we can define the joint density of states as Jcv (ω) =

v ck

2 δ[Ec (k) − Ev (k) − hω] = ¯ (2π )3

ds s

1 , ∇k (Eck − Evk )

(9.75)

9.4 Interband optical transitions in semiconductors and insulators

197

6

Energy E (eV)

4 2

Approx. parallel bands

0

Approx. parallel bands

–2 –4 L

Γ

X

Γ

Wavevector k

Figure 9.5

An example of parallel bands leading to critical points and van Hove singularities in the joint density of states. where s = surface of constant h¯ ω = Eck − Evk , and within this simplification 2 (ω) ∼

1 |ˆe · Mvc |2 Jcv (ω), ω2 v c

(9.76)

where Mvc is a constant for a given (v, c) pair of bands. The joint density of states gives a measure of the density of full and empty states of equal energy difference. This quantity plays an important role in determining the interband contribution to 2 and the optical properties of solids for certain classes of materials for which Mvc ≈ constant. Similarly to the electron or phonon analysis of g(E), we define critical points in k-space by the condition ∇k (Eck − Evk ) = 0,

(9.77)

which associates a critical point with regions in k-space where the electronic energy bands are parallel, as shown in Fig. 9.5. Hence, near a critical point energy hω(k ¯ 0 ), we can expand the energy difference in principal axes to obtain in three dimensions hω(k) = h¯ ω0 (k0 ) + ¯

3 =1

α (k − k0 )2 .

(9.78)

Depending on the signs of the α , we obtain van Hove singularities of different types (as in the case of g(E)), M0 , M1 , M2 , and M3 in Jcv (E) for a three-dimensional crystal. In many applications involving the optical properties of semiconductors, the behavior of the absorption edge plays a very important role. The optical absorption edge of direct gap materials, where the valence band maximum and conduction band minimum lie at the same k, is quite different from those of the indirect gap materials. Direct transitions constitute the lowest-energy transitions of the absorption spectrum of direct gap materials and determine the shape of the absorption edge, as in the case of GaAs.

9 Electronic transitions and optical properties of solids

198

Energy E

Conduction band

Eg

Valence band

Wavevector k

Figure 9.6

A direct bandgap material with parabolic bands. For this case, near the band edges for parabolic bands (see Fig. 9.6), Eck − Evk = Eg +

h¯ 2 k2 h¯ 2 k2 h¯ 2 k2 − = Eg + , 2mc 2mv 2μ

(9.79)

where μ is the reduced mass of the electron (me = mc ) and hole (mh = −mv ). This yields Jcv (ω) =

3/2 2μ 1 1/2 (hω ¯ − Eg ) 3 (2π ) h¯ 2

(9.80)

and, near the edge, 2 (ω) ∼

1 1 (hω ¯ − Eg ) 2 2 ω

(9.81)

if one assumes that M is a constant. Dipole-allowed vs. dipole-forbidden transitions. We now consider dipole-allowed vs. dipole-forbidden transitions. In general, 2 (ω) (Eq. (9.73)) will depend on the matrix element |ˆ · M|2 , with (where the u functions are normalized in a unit cell) Mvc (k) = c, k + q| eiq·r ∇ |v, k = u∗c,k+q (∇ + ik)uv,k (r)d3 r = u∗c,k+q ∇uv,k d3 r + ik u∗c,k+q uvk d3 r

(9.82)

f

≡ Mdvc (k) + ikMvc (k). Usually, the second term of the sum can be neglected as compared with the first term because of the orthogonality of Bloch functions with the same k, since q ≈ 0. Mdvc gives

199

9.4 Interband optical transitions in semiconductors and insulators

h¯ω

nk t

mq

nk

Figure 9.7

Phonon-assisted transition caused by a photon of frequency ω through the absorption or emission of a phonon having wavevector q. the standard dipole selection rule: Mdvc = 0 between states of the same parity. For dipolef forbidden transitions, Mvc in the second term will determine the transition intensity. Hence, for dipole-allowed transitions (e.g. GaAs, in which the top of the valence band is p-like and the bottom of the conduction band is s-like), 2 ∼

1 d 2 hω |M | ¯ − Eg , ω2 v c

(9.83)

and, for dipole-forbidden transitions (e.g. NiO and the cuprates), owing to the extra k factor in the second term in Eq. (9.82), 2 ∼

1 f 3/2 |Mvc |2 (hω ¯ − Eg ) . ω2

(9.84)

We note also that if Mdcv (k), although zero at k0 , has a linear k-dependent term, it will contribute to give an effective total Mf in Eq. (9.84). Indirect optical transitions. Up to this point, we have only considered direct transitions. The wavevector or crystal momentum selection rule from the interaction H1 ∼ A · ∇ is kf = ki + qphoton + G.

(9.85)

However, if we have an indirect bandgap material, the absorption edge corresponding to the indirect gap energy range arises from transitions involving impurities (which remove the above selection rule) in the system or through the emission or absorption of phonons (or other elementary excitations). (See Fig. 9.7.) Therefore, we cannot consider only the term A · ∇. For phonon-assisted transitions, the k-selection rule is kf = k + qphoton ± qphonon + G.

(9.86)

The perturbation Hamiltonian becomes H1 = Helectron–photon + Helectron–phonon = Hrad + Hlat .

(9.87)

Since H1 involves terms separately with a photon and a phonon, we need to evaluate it to second order to obtain an indirect optical transition. The transition amplitude involves

9 Electronic transitions and optical properties of solids

200

summing up all virtual processes that lead to a final state of an electron in the conduction band and an electron missing (hole created) in the valence band. For the system in its ground state with Np photons and nq phonons, the initial state is

|i = electrons in their ground state, Np photons, and nq phonons ,

(9.88)

and the final state is

|f = excited electron–hole pair, Np − 1 photons, and nq ± 1 phonons .

(9.89)

Second-order perturbation theory gives the transition matrix element square for use in Fermi’s golden rule as

2

f | Hlat |m m| Hrad |i

, + (H ↔ H ) term rad lat

Em − Ei m

(9.90)

where |m is an intermediate state, and, as discussed in Chapter 10, 1 Hlat ∼ a†−q + aq )c†k+q ck ,

(9.91)

with

√ nq − 1 Hlat nq ∼ nq

(absorption)

(9.92)

and

nq + 1 Hlat nq ∼ nq + 1

(emission),

(9.93)

,

(9.94)

where the thermal averaged value nq is nq =

1 ¯ eβ hω(q)

−1

and β = kB1T . Owing to the difference in the energy denominator, typically only one of the two terms in Eq. (9.90) dominates. Since for absorption, nq =

1 ¯ eβ hω(q)

−1

,

(9.95)

and for emission, nq + 1 =

1 ¯ 1 − e−β hω(q)

,

(9.96)

9.5 Electron–hole interaction and exciton eﬀects

201

Square root of absorption coefficient η1/2

T>0

T=0

Emission

Absorption

Emission ω

2ħωq

Figure 9.8

Eg + ħωq

Phonon absorption and emission processes in optical absorption spectra. For T > 0, the emission onset is at lower energy because, in general, Eg decreases with T, and both emission and absorption processes can be appreciable.

we have, for a simple three-band model with a single intermediate band β and all bands parabolic, 1 ε2 (ω) ∼ 2 ω

ck | H |βk βk | H |vk 2 1 1 1

2 lat rad d3 k1 d3 k2

δ(Ec (k2 ) Eβ (k1 ) − Ev (k1 ) − hω ¯

− Ev (k1 ) − hω ¯ ± hω ¯ q) ∼

22 1 1 1 hω ¯ − Eg − h¯ ωq nq + 1) ω2

∼

22 1 1 hω ¯ − Eg + h¯ ωq (nq ) ω2

(for emission of phonon),

(9.97)

or (for absorption of phonon).

(9.98)

As seen in the above expressions and in Fig. 9.8, there are characteristic frequency and temperature dependences for phonon-assisted indirect transitions that are distinct from direct transitions.

9.5 Electron–hole interaction and exciton eﬀects Up to this point, we have not considered the Coulomb interaction between the excited electron and hole involved in an optical transition. If the electron and hole bind, this is analogous to the case of positronium, and the resulting excitation is called an exciton. Even without bound states, there are “exciton effects” owing to the correlations between the two quasiparticles created. Often excitons are broadly classified as Wannier excitons, when the

9 Electronic transitions and optical properties of solids

202

(b)

Energy E

Conduction band

Eex

Eg Valence band

1s

Absorption coefficient

(a)

n=1 l=0

2s Free 3s

Wavevector k

Figure 9.9

Eg

ω

Schematic of energy levels of excitons in a two-parabolic band model: (a) Quasiparticle band structure with bandgap Eg and an exciton state at energy Eex indicated. (b) Sketch of absorption spectrum of a dipole-allowed direct bandgap semiconductor with the lowest three excitonic transitions shown.

electron and hole are weakly bound, i.e. the electron and hole spatial correlation is large compared to the lattice constant and Frenkel excitons, when they are strongly bound. Wannier excitons can often be described approximately by an effective mass equation, which at the simplest level is given by

e2 p2 − F(r) = EF(r), 2μ r

(9.99)

where

E = Eex − Eg

(9.100)

is the exciton binding energy and F(r) is its wavefunction with r the electron–hole relative coordinates. Here Eex is the energy of the excitonic state and Eg is the bandgap (see Fig. 9.9), with 1 1 1 = + μ mh me and r = re − rh .

(9.101)

More rigorously, an exciton state is a coherent superposition of many free electron–hole excitation configurations given in the form |ψex =

i

αi |φi ,

(9.102)

9.5 Electron–hole interaction and exciton eﬀects

Energy E

203

Wavevector k

Figure 9.10

Schematic picture of an exciton state composed of many independent-particle transitions or electron–hole pairs represented by the arrows. where |φi = c†c,k+q cv,k |G,

(9.103)

and c† and c are the one-particle (or, more rigorously, quasiparticle) creation and annihilation operators, and |G represents the electronic ground state. This is depicted in Fig. 9.10. To determine the exciton energies and wavefunctions, we solve the many-body Schr¨odinger equation, H |ψex = Eex |ψex , where

H is the many-electron Hamiltonian. To solve this problem, we need to find φi | H φj . For example, the ground-state Slater determinant is described by G (1, . . . , N) = A{a1 (1)a2 (2) . . . aN (N)},

(9.104)

where A is the antisymmetry operator, ai are single-particle orbitals, and 1 denotes a composite index x1 = (r1 , σ1 ). In the occupation number formalism, this can be written as (where the orbitals are positioned in order of increasing energy) |G = |1111 . . . 0000.

(9.105)

It is convenient to separate the Hamiltonian into two parts (H = H1 +H2 ), the one-electron Hamiltonian H1 and the electron–electron interaction term H2 , where H1 =

N

h1 (ri ) =

i=1

N 2 p i

i=1

2m

+ V(ri )

(9.106)

and H2 =

1 1 e2 h2 (i, j) = . 2 2 rij i,j

i=j

(9.107)

9 Electronic transitions and optical properties of solids

Figure 9.11

Illustration of the diﬀerent types of Slater determinants required to create all the matrix elements needed to solve the exciton problem. The dots indicate occupied orbitals and arrows indicate a transition creating a free electron–hole pair.

Energy

204

To solve this problem, which we will do in the next section, we need to calculate the matrix elements between three types of Slater determinants, as shown in Fig. 9.11. These matrix elements can be worked out if |A is a given single Slater determinant, as ai | h1 |ai A| H1 |A = i

and A| H2 |A =

1 ij

where

ai aj h2 ai aj =

ai aj h2 ai aj − ai aj h2 aj ai ,

2

a∗i (x1 )a∗j (x2 )h2 (r2 , r1 )ai (x1 )aj (x2 )dx1 dx2 .

(9.108)

(9.109)

For |B = c†bk cak |A, as depicted in Fig. 9.11, A| H1 |B = ak | h1 |bk

(9.110)

and A| H2 |B =

ak aj h2 bk aj − ak aj h2 aj bk .

(9.111)

j

For |C = c†ck cak c†c ca |A, as depicted in Fig. 9.11, A| H1 |C = 0

(9.112)

A| H2 |C = ak a | h2 |ck c − ak a | h2 |c ck .

(9.113)

and

205

9.5 Electron–hole interaction and exciton eﬀects

9.5.1 Weak binding limit in the two-band model To illustrate the physical properties of excitons, we examine the weak binding limit in a two-band model. We also note that the basis states or determinants defined above can have finite center of mass momentum (see below). This is shown schematically in Fig. 9.12. For an insulating material with weak spin–orbit coupling (i.e. the spin is not coupled to the orbital motion), we may construct the ground state as & % |G = A φv,k1 (r1 )α(1)φv,k1 (r2 )β(2) . . . φv,k N (rN )β(N) , (9.114) 2

where v is the band index, and α = ↑, β = ↓ represent spin-up and -down spinor functions. Hence, the free electron–hole excited configurations take the form

φck

e se ,v kh sh

= c†cke se cvkh sh |G,

(9.115)

where, at this point, we are not limiting ourselves to optical excitations, so ke and kh do not need to be the same and the spin can flip. The wavevector kex = ke − kh characterizes the center of mass momentum of the free electron–hole (e–h) pair excitation. The exciton state can now be written as |ψex = (9.116) Ai |φi , i

where |φi is given by Eq. (9.115). We now need to solve for the coefficients Ai in Eq. (9.116) by solving the many-electron Schr¨odinger equation in order to obtain the exciton states by taking matrix elements of the Hamiltonian, H = H1 + H2 , given in Eqs. (9.106) and (9.107). This Hamiltonian is spin independent (since we neglect spin–orbit interaction, which can be important for heavier atoms). Therefore, we should have a well-defined spin configuration for the excited states. Combining two spin 12 particles (an electron and a hole) yields an S = 1 triplet state or E ke

kh Wavevector k

Figure 9.12

Schematic picture showing a nonzero center of mass momentum for a free electron–hole pair conﬁguration.

9 Electronic transitions and optical properties of solids

206

an S = 0 singlet state. We note here that the spin state of a hole is opposite to that of the electron state being emptied. For S = 1, we may have schematically (with the second spin being that of the hole) Sz = 1: |↑ |↑, Sz = 0: √1 |↑ |↓ − |↓ |↑ , 2

Sz = −1: |↓ |↓, and for S = 0, Sz = 0:

√1 2

|↑ |↓ + |↓ |↑ .

(9.117)

Letting M denote a specific spin state, we have within a two-band model (i.e. neglecting the sum over v and c)

M

M

ψ = (9.118) A ke ,kh φke ,kh , ex ke ,kh

where φ M is a composite Slater determinant of the form given by combining Eqs. (9.115) and (9.117). The Hamiltonian also has crystalline translational symmetry, and, therefore, the exciton has a well-defined center of mass wavevector kex · So kex is a good quantum number and each of the terms in Eq. (9.118) must have kex = ke − kh . This implies that ke − kh = ke − kh in Eq. (9.118). In other words, the exciton wavefunction is made up of transitions with the same change in k. Thus, we can write the exciton wavefunction as

M

M

ψ = φ . (9.119) A(k)

1 1 ex k+ k ,k− k 2 ex

k

2 ex

We define the following “envelope function” in real space: F(r) = A(k)eik·r .

(9.120)

k

We may now derive a differential equation for F(r) using the many-body Schr¨odinger equation Hψex = Eex ψex , which becomes the matrix equation

Hk,k A(k ) = Eex A(k).

(9.121)

(9.122)

k

At this point, we need to describe the matrix elements of H in Eq. (9.122). The diagonal elements can be written as (using Koopmans’ theorem)

φkh ,ke H φke ,kh = Ec (ke ) − Ev (kh ) + G| H |G, (9.123)

9.5 Electron–hole interaction and exciton eﬀects

207

A (k)

k 0

Figure 9.13

The coeﬃcient A(k) for the exciton state in Eq. (9.119) is schematically plotted in k-space. In the weak binding approximation, the distribution is very narrow.

where Ec and Ev are the conduction and valence band state energies, respectively, and, without any loss in generality, we set the last term (which is the ground-state energy) to zero. Using the list of matrix elements above for the basis functions (free electron–hole pair excitations) |A, |B, and |C, the off-diagonal matrix elements become

−e2

2

φck φvk − 2δM φck φvk

−e φck φvk , φkMe ,kh H φkM ,k = φcke φvk e h h e e h h e h r12 r12 (9.124) where δM = 1 if S = 0, and δM = 0 if S = 1. The first term is attractive and is called the direct term because it resembles a direct interaction between two charges of opposite sign if ke = ke and kh = kh . Similarly, the second term is called the exchange term because it looks like a Hartree–Fock exchange interaction. Note that the exchange term is repulsive and is nonzero only for the spin singlet case. As we discussed above, a definite center of mass momentum implies that ke − kh = ke − kh for all transitions that make up the exciton state. If we make the weak binding approximation (that is, the wavefunction of the bound electron–hole pair in real space is large), which amounts to a narrow distribution in k-space, then ke − ke ≈ 0. This is shown in Figs. 9.13 and 9.14. The direct term can be written as

−e2 2

φck φvk = φck Tφvk −e

φck Tφvk , φcke φvk e h h e e h h r12 r12

(9.125)

where T is the time-reversal operator. This interaction is shown diagrammatically in Fig. 9.15.

9 Electronic transitions and optical properties of solids

Energy E

208

Wavevector k

Figure 9.14

All the transitions that make up the exciton state in the weak binding limit are close together in k-space.

vkh

cke q t cke

vkh

Figure 9.15

Diagram of the direct interaction in Eq. (9.124).

If we explicitly write out the direct term, we have

dir

=

dr1 dr2

−e2 −i(ke −ke )·(r1 −r2 ) ∗ e ucke (r1 )ucke (r1 )u∗vk (r2 )uvkh (r2 ). (9.126) h r12

The term involving the periodic part of the Bloch function u’s (we shall call it g(r1 , r2 )) can be seen in the weak binding approximation as g(r1 , r2 ) ≈ ρcke (r1 )ρvkh (r2 ) because all the k-points are near each other in k-space. The function g is periodic and can be expanded in planewaves of reciprocal lattice vectors g(r1 , r2 ) =

am,n eiGm ·r1 e−iGn ·r2 .

(9.127)

m,n

If the density is approximately constant in a unit cell, then am,n = 1 for m = n = 0, and am,n ≈ 0 otherwise. So, the direct term can now be written as

dir

≈

dr1 dr2

−e2 −i(ke −ke )·(r1 −r2 ) . e r12

(9.128)

9.5 Electron–hole interaction and exciton eﬀects

209

Similarly, for the exchange term in Eq. (9.124), we may argue that, to a good approximation because uck is orthogonal to uvk , = Jex (kex )δM , (9.129) ex

which is independent of ke − ke (which leads to a δ(r) in real space). Collecting all the terms, we get the final equation for the exciton eigenvalues and eigenfunctions (i.e. Eq. (9.122)) in the form 1 1 Ec k + kex − Ev k − kex − Eex A(k) 2 2 (9.130) e2 − dr e−i(k−k )·r + Jex (kex )δM A(k ) = 0. + r k

We now introduce some new notation to simplify the evaluation and interpretation of our results. We begin by defining 1 1 (9.131) Ecv (k, kex ) = Ec k + kex − Ev k − kex . 2 2 The envelope wavefunction F was introduced previously in Eq. (9.120). Since our goal is to derive an equation for Eex and F, we use these definitions and Eq. (9.130) to obtain

2 e −ik·r Ecv (k, kex ) A(k) + − dr F(r )e + Jex (kex )δM F(0) = Eex A(k). r Since mathematically for any function with variable −i∇, f(−i∇)F(r) = f(k)A(k)eik·r

(9.132)

(9.133)

k

and k

dr

e2 e2 F(r )e−ik·r eik·r = F(r), r r

(9.134)

if we multiply Eq. (9.132) by e−ik·r and then sum over k, we obtain e2 + Jex (kex )δM δ(r) F(r) = Eex F(r). Ecv (−i∇, kex ) − r

(9.135)

This equation is the effective mass equation describing excitons. Two assumptions were used to derive Eq. (9.135): a trial wavefunction represented by a linear combination of Slater determinants describing free electron–hole pair excitations, and the weak binding approximation. It is useful at this point to make a few comments regarding the effective mass equation (Eq. (9.135)). The excitation energy Eex is the energy needed to create an exciton. At this

9 Electronic transitions and optical properties of solids

210

Exciton wavefunction

e– amplitude

Figure 9.16

Hole

r

Schematic drawing of the exciton wavefunction ψex (re ,rh ) in real space, with r the electron–hole relative coordinates assuming a ﬁxed position for the hole.

point, we can go beyond our rather simple treatment since the electron–hole interaction 2 2 will be screened by the other electrons by changing − er → − er , where is the dielectric function of the material. In most cases, the static can be used since the relevant binding energy Eb = Eg − Eex is small compared to the bandgap energy. Only the relative coordinates between the electron and the hole remain within Eq. (9.135). We can expand the interband transition energy term in the form Ecv (−i∇, kex ) =

α,β n,m

n m Bnm αβ ∇α ∇β ,

(9.136)

with the coefficients Bnm αβ related to the band effective masses. Also, coming back to the definition of A(k) in Eq. (9.119), one can show that within our approximations the full exciton state is given by |ψex =

F(R1 − R2 )w1† w2 |G ,

(9.137)

R1 R2

where now the wi ’s are the Wannier function annihilation operators. The electron–hole F(R1 − R2 )wc (re − amplitude or wavefunction in real space is ψex (re , rh ) = R1 ,R2

R1 )wv (rh − Rh ), with wc and wv the Wannier functions. The exciton wavefunction in real space ψex (re , rh = 0) is illustrated schematically in Fig. 9.16.

9.5.2 Excitonic eﬀects in the isotropic two-band model As depicted in Fig. 9.17, we may assume for illustration purposes that both bands in an h¯ 2 2 ∇ , isotropic two-band model can be approximated as parabolas, Ecv (−i∇) = Eg − 2μ where

1 μ

=

1 me

+

1 mh ,

and that kex = 0, which is the case for the optical transitions. Putting

9.5 Electron–hole interaction and exciton eﬀects

211

Energy E

Conduction band

Eg

Valence band

Wavevector k

Figure 9.17

The isotropic two-band model.

all of these into the effective mass equation gives

−h¯ 2 2 e2 ∇ − + Jcv (0)δM δ(r) F(r) = (Eex − Eg )F(r), 2μ r

(9.138)

where (Eex − Eg ) = E is the negative of the exciton binding energy. In the weak binding approximation, = constant and J is typically negligible because of the large spatial extent of the exciton envelope function F. Equation (9.138) resembles the Schr¨odinger equation for a hydrogen atom. Therefore, in three-dimensional systems, we expect bound states (E < 0) of the form E=−

R , n2

(9.139)

where R = μe2 2 . This energy is typically < 0.01 Ry for most bulk semiconductors. The 2h¯ wavefunction F becomes a hydrogen-like wavefunction Fn,,m (r). For the unbound states E > 0, the wavefunctions are again hydrogen-like, Fs,l,m (r) = Rs,l (r)Yl,m , where s = 4

It should be noted that for E R, F → eike ·r and A(k) → δ(k − ke ). These results for most bulk semiconductors are consistent with the weak binding approximation. For example, the 1s exciton wavefunction has the form 2μE . h¯ 2

r 1 − F100 = e aex , π a3ex

(9.140)

with a spread determined by aex = a0 mμe , where a0 is the Bohr radius. Now, in general, me μ > 1 and ≈ 10 − 20 for semiconductors. So, aex ≈ 100a0 . Thus, for A(k), we have

9 Electronic transitions and optical properties of solids

212

(by Fourier-transforming Eq. (9.140)) 1 A(k) = A0 2 , 2 1 + (kaex )

(9.141)

where A0 = 2π a2ex / π a3ex is a constant, and the ratio of A at the Brillouin zone edge compared to the zone center is A(kBZ ) = A(0)

1 1 + (kBZ aex

)2

−4 −6 2 ≈ 10 − 10 ,

(9.142)

where we have used kBZ ≈ 1 in units of Bohr. Therefore, the weak binding approximation is consistent. For this model, Jex affects only s-states since it is a delta function at r = 0, and it is important only for more strongly bound excitons. Returning to the optical response function, we have from Eq. (9.69) the expression 2 (ω) = 8π2h¯ Wtot for the imaginary part of , where Wtot is the number of photons abE0

sorbed per volume per unit time. In the independent electron picture without considering excitonic effects, this becomes (rewriting Eq. (9.73) and using the subscript F to denote free or non-interacting particles) 2F (ω) =

4π 2 e2 h¯ 2 m2 ω2

BZ

2

2d3 k

ˆ e · M (k) δ E (k) − E (k) − hω ,

¯ c v c v (2π )3

(9.143)

where eˆ is the polarization vector of the photon and M is the interband transition matrix element. With excitonic effects included, the probability of a transition from the ground state to an exciton state (from Fermi’s golden rule) is P|G→|ψex = where HI =

|e| i

mc A(ri ) · pi .

(in particular, A| P|G→|ψex

i hi |B

2 2π

ψG | HI |ψex δ(Eex − h¯ ω), h¯

(9.144)

Using the rules introduced previously for the matrix elements

= ak | h1 |bk ), we find

π eA0 2 = δkex δM h¯ 2 | A(k)ˆe · Mcv (k)|2 δ(Eex − h¯ ω), 2h¯ mc

(9.145)

k

where A0 is the amplitude of the vector potential of the EM wave, A(k) is the exciton wavefunction in k-space, and Mcv (k) =

u∗c (k + q, r)(∇ + ik)uv (k, r)d3 r

is the interband matrix element, as before.

(9.146)

9.5 Electron–hole interaction and exciton eﬀects

213

For dipole-allowed transitions, the first term on the right-hand side of Eq. (9.146) for the matrix element (i.e. the ∇ term in the integrand) is assumed to be constant independent of k, and one neglects the ik term for M. Since k A(k) = F(r = 0), Eq. (9.145) becomes P|G|ψex ∝ δkex δM |ˆe · Mcv (0)|2 |F(0)|2 δ(Eex − hω). ¯

(9.147)

Since F(0) = 0 only for s-states for the hydrogenic functions where Fn00 (0) = √

1 , π a3ex n3 1 In ∝ n 3 .

this gives transition intensity to the excitons with principal quantum number n as Thus, we expect a series of lines at E = Eg − nR2 for n = 1, 2, . . . , with the intensity decreasing as n13 (Fig. 9.9(b)). At high values of n, we can express the absorption intensity in terms of the density of states n3 dn = , D(E) = 2 dE R

(9.148)

yielding the result that the intensity/energy = In (E)D(E) goes to a constant for transitions near Eg . This is shown as the shoulder in Fig. 9.18 near Eg . For the unbound excitons (E > 0), we have for dipole-allowed bands 2 (ω) = 2F (ω)|Fs00 (0)|2 = 2F (ω) where χ =

π χ eπ χ , sinh(π χ )

(9.149)

There are two interesting limiting cases: (1) hω ¯ − Eg R, 2 (ω) → √ h¯ ω−Eg = constant, which is the 2F (ω), and (2) hω ¯ − Eg R, 2 (ω) → 2π χ 2F (ω) ≈ √ R h¯ ω−Eg .

h¯ ω−Eg

Absorption coefficient

same constant that approaches from the E < 0 side. This behavior is sketched in Fig. 9.18. Up to this point, we have considered the case of dipole-allowed transitions where optical transitions lead to optically active (in linear response) excitons of hydrogen atom-like states with = 0 (s-states). But in the case of dipole-forbidden transitions, we shall see that the optically active excitons must have = 1, and they form hydrogen atom-like p-states. We

ω Eg

Figure 9.18

Plot of a typical optical spectrum with excitonic eﬀects included.

9 Electronic transitions and optical properties of solids

214

begin with Eq. (9.146) and rewrite M in the form M = Mallowed + ikMforbidden .

(9.150)

For the dipole-forbidden case, Mallowed = 0. We use only the second term in Eq. (9.150) for Eq. (9.145), and since

A(k) k =

k

∂ F(r)|r=0 , ∂r

(9.151)

the probability of creating an exciton state in the dipole-forbidden case is then P|G→|ψex

2

forbidden 2

∂ π eA0 2

eˆ · F(r)

δ(Eex − hω). = h¯ δkex δM M ¯

2h¯ mc ∂r r=0

Since there is only a nonzero transition probability for

∂ F(r)

= 0, ∂r r=0

(9.152)

(9.153)

which is the case for hydrogen atom-like p-states with

1 2

∂ n −1 2 = . Fn1m (r)

∂r π a5ex n5 r=0

(9.154)

This results in having peaks in the absorption spectra at energies E = Eg −

R n2

(9.155)

for n = 2, 3, 4, 5, . . . , ∞. Here, R is again the effective Rydberg for the exciton. The intensity of each absorption line is proportional to the transition probability n2 − 1 n5

(9.156)

1 as n → ∞. n3

(9.157)

In ∼ and In ∼

The absorption spectra are shown schematically in Fig. 9.19. Note that as the energy approaches the gap energy Eg , the absorption per unit energy becomes constant. This occurs because the intensity of each state times the density of states is a constant (as discussed above for the dipole-allowed case): lim In D(En ) = constant.

n→∞

(9.158)

9.5 Electron–hole interaction and exciton eﬀects

215

Absorption coefficient

n=2 (2p) n=3 (3p)

Free

n=4 (4p)

ω Eg

Figure 9.19

Absorption spectra for dipole-forbidden transitions of exciton states. For the case of unbound states, 2 is given by (again using hydrogenic wavefunctions) π χ (1 + χ 2 )eπ χ , (9.159) sinh π χ R where 2F is the independent electron 2 and χ = (h¯ ω−E . g) There are again two cases of interest. Case I is hω − E ¯ g R (high energy), 2 (ω) ∼ 2F (ω). Case II is hω ¯ − Eg R (near the continuum absorption edge), 2 (ω) ∼ 2F (ω)χ 3 = constant. The form of the absorption for energies approaching Eg from above is also a constant. An example of a system with dipole-forbidden transitions is Cu2 O. In Cu2 O, the cm−1 with absorption peaks fit very well into a hydrogen-like series4 vn = 17 250 − 786 n2 n = 2, 3, . . . So far, we have only been considering an onset of absorption with an M0 critical point or singularity in the joint density of states. However, excitonic effects at van Hove singularities of kinds M1 , M2 , and M3 can be significant. For the independent electron model, a model dipole-allowed absorption spectrum in three dimensions is shown in Fig. 9.20. The independent electron case is modified in several ways because of excitonic effects. The effect of excitons near the van Hove singularity M3 is to reduce the oscillator strength (Fig. 9.21) 2 (ω) = 2F (ω)

2 (ω) = 2F (ω)

π x eπ x , sinh π x

(9.160)

where x = E3 −Rh¯ ω , and there are no discrete lines above E3 like there are below E0 . For the other two cases, near M1 excitonic effects enhance 2 (ω) and near M2 excitonic effects weaken 2 (ω). In GaAs this leads to an apparent shift in the position of an absorption peak by about 0.5 eV in the higher-frequency region, even though no bound exciton is formed. 4 P. W. Baumeister, “Optical absorption of cuprous oxide,” Phys. Rev. 121(1961), 359.

9 Electronic transitions and optical properties of solids

Absorbtion coefficient

216

M1

M2

ω M0

Model of dipole-allowed absorption spectrum at diﬀerent critical points for a three-dimensional independent electron system.

Absorption coefficient

Figure 9.20

M3

With exciton effects

Free electron case

ω E3

Figure 9.21

Absorption at M3 van Hove singularity in the joint density of states is decreased due to excitonic eﬀects.

Moving beyond the strict hydrogenic model, we note that the exchange interaction term, which is given by J = J(kex )δ(r)δM ,

(9.161)

is repulsive and short-ranged. Since photons cannot flip spin, we expect only singlet states to be excited optically. However, if spin–orbit interactions are allowed and strong, the singlet and triplet states will mix and extra weak transitions will be activated. In first-order perturbation theory, the energy splitting between singlet and triplet states is given for s-like states by (see Fig. 9.22) E ∼ ψex | J |ψex ∼ |F(0)|2 ∼

1 . n3

(9.162)

Hence, the exchange energy E for Wannier excitons is small except for n = 1 and for strongly bound excitons.

9.5 Electron–hole interaction and exciton eﬀects

217

Absorption coefficient

Singlet

Triplet

ω ΔE

Figure 9.22

Single-triplet splitting of excitons. For many materials, the electron bands are anisotropic. In these cases, the effective masses and dielectric constants are tensors instead of scalars. For many materials, they are described in terms of two constants representing an in-plane and an out-of-plane component, μ → (μ , μ⊥ )

(9.163)

→ ( , ⊥ ).

(9.164)

and

For systems of this type, the anisotropic properties are characterized by the parameter γ , μ , ⊥ μ⊥

(9.165)

0 ≤ γ ≤ 1.

(9.166)

γ = with

This problem is difficult to solve analytically in general and is usually done numerically. For the specific case of γ = 0 (the case where μ⊥ → ∞, which corresponds to the two-dimensional case, e.g. the two-dimensional electron gas, quantum wells, etc.), the excitation energy for bound excitons (with dipole-allowed bands) is Eex = Eg −

R n+

1 2

2 ,

(9.167)

for n = 0, 1, 2, . . . For n = 0, the excitation energy becomes Eex = Eg − 4R.

(9.168)

This is an example of how, in reduced dimensions, Coulomb interaction and correlation effects become more important.

9 Electronic transitions and optical properties of solids

218

If we consider the effects of a magnetic field in the effective mass approximation, we may use e pe → pe − A(re ), c e ph → ph + A(rh ), c

(9.169) (9.170)

and the effective mass equation becomes

2 2 1 e 1 e e2 F(re , rh ) pe − A(re ) + ph + A(rh ) − 2me c 2mh c |re − rh | = Eex − Eg F(re , rh ).

(9.171)

For uniform magnetic field, the canonical transformation F(re , rh ) 1 ae nearly 2 i K+ c A(r) ·R e φ(r) may be used, and Eq. (9.171) becomes

p2 e 1 2eh¯ e2 2 1 e2 + − K · A(r) φ(r) A(r) · p + − A (r) − 2μ c mh mc 2μc2 r Mc h¯ 2 K2 φ(r), = Eex − Eg − 2M

=

(9.172)

−1 1 1 h rh where r = re − rh , R = memree +m , M = m + m , μ = + , and K = momentum e h +mh mc mh of the center of mass motion. Rearranging terms, Eq. (9.172) becomes h¯ 2 K2 H0 + Hz + Hd + Hs φ(r) = Eex − Eg − φ(r), 2M where H0 = we get

p2 2μ

−

e2 r

(9.173)

is the unperturbed Hamiltonian. For the unperturbed Hamiltonian,

E0ex = Eg +

μe4 h¯ 2 K2 − , 2M 2n2 h¯ 2 2

(9.174)

and the other terms correspond to (using the gauge A = − 12 r × B) eB 1 e 1 1 1 A(r) · p = Lz , (1) Zeeman splitting: Hz = − − c mh me 2c mh me (2) diamagnetic term: Hd =

e2 2 e2 B2 2 A (r) = (x + y2 ), 2 2μc 8μc2

(9.175) (9.176)

9.5 Electron–hole interaction and exciton eﬀects

219

and 2e 2e K · A(r) = − B · (r × K) Mc Mc 2e r · (K × B) =− Mc

(3) magneto-Stark effect: Hs = −

(9.177)

In the Hs term, K × B acts as an effective electric field and gives rise to a Stark effect. The study of excitons and shallow impurity states in a magnetic field in semiconductors is equivalent to studying atomic physics in extremely high magnetic fields. The relevant parameter to measure the effect of an external B-field on a system with binding energy R∗ and an effective cyclotron frequency ωc∗ is eB

h¯ μ∗ c hω ¯ c∗ = = δ= ∗ 4 ∗ 2R 2 μ2he2 ¯

hω ¯ c 2Ry

μ∗ m

2 .

(9.178)

For GaAs, δ = 1 at about a magnetic field of 7 Tesla. For an atomic system, for δ = 1, we need B = BGaAs

μ∗ −2 m

10 2 ≈7 T = 105 T. 0.07

(9.179)

Magnetic field studies of exciton and impurity states in semiconductors may thus have relevance in astrophysics because there are atoms and molecules in such large fields in outer space.

10

Electron–phonon interactions

The interplay between electrons and lattice vibrations is one of the most interesting and important physical processes in the study of solids. The static lattice with atoms assumed frozen at their equilibrium positions yields the crystal potential, which governs many electronic properties such as band structure effects. With vibrations of the lattice comes a host of new effects resulting from the interactions of electrons and phonons. These include the scattering of electrons by phonons, which gives rise to a temperature-dependent resistivity (Fig. 10.1). Other first-order processes include the non-radiative recombination of electron–hole pairs and their generation, which is responsible for ultrasonic attenuation (Fig. 10.2). Second-order electron–phonon processes lead to extraordinary effects. The emission and subsequent reabsorption of virtual phonons is the fundamental process for the creation of polarons in insulators and the mass enhancement of electrons in all types of solids (Fig. 10.3(a)). This process is also responsible for part of the temperature dependence of energy bandgaps. Another second-order process is the electron–electron interaction via the exchange of a virtual phonon, which can lead to bipolarons, Cooper pairs, and superconductivity (Fig. 10.4). The emission of virtual electron–hole pairs (Fig. 10.3(b)) by phonons and the subsequent destruction of the electron–hole pair renormalize the phonon energy. This can lead to softening (lowering of energy) of a phonon mode, which in turn can cause a structural phase transition.

10.1 The rigid-ion model The rigid-ion model is one of the simplest ways of formulating and understanding electron– phonon interactions. The idea is that each ion (or atom) is assumed to contribute rigidly to the total potential seen by the electrons in the solid. As an ion is moved away from its equilibrium position, the potential is no longer periodic, and this will scatter an electron from one Bloch state to another. Let V(r) be the static crystal potential which changes because of vibrations, i.e. V(r) → V(r, t) =

,a

Va r − Ra (t) ,

(10.1)

where Ra (t) = R + τ a + δRa (t) = Ra + δRa (t), 220

(10.2)

10.1 The rigid-ion model

221

(a) Emission

(b) Absorption k–q

k–q

k

k

q

Figure 10.1

q

Emission and absorption of a phonon by an electron.

k−q

q

q

k+q

k

Figure 10.2

k

Emission of a phonon in non-radiative recombination of an electron–hole pair (left) and generation (right) of an electron–hole pair. (a)

(b)

q

k

q k

k–q

q

k k–q

Figure 10.3

Emission and absorption of a virtual phonon by an electron (a) and emission and reabsorption of a virtual electron–hole pair by a phonon (b). where is the cell index, a is the atomic index, and τ a is the vector to atoms in the basis. We assume the displacement is much less than the atomic spacing d, i.e. ξ ≡ δRa d.

(10.3)

For typical vibrations, it can be shown that m 1/4 ξ ∼ d M

(10.4)

and the excitation or phonon energy Eph scales as m 1/2 Eph ∼ 10−2 , Eel M

(10.5)

m is the ratio of the electron and atomic masses. where Eel is a typical electron energy and M Because of these scaling arguments, we can assume that the large-scale band structure is

10 Electron–phonon interactions

222

k

k+q

q

k − q

k

Figure 10.4

Electron–electron interaction by the exchange of a virtual phonon.

not modified. However, the vibrations of the ions do affect the dynamics of electrons. For example, in the case of a metal, electron–phonon interactions can cause a “wrinkle” in the band structure within a few meV of the Fermi energy. This represents a modification of the effective mass of the electrons by the phonons but only at energy scales comparable to phonon energies. The derivation of the electron–phonon interaction matrix element proceeds as follows. Assuming a small displacement, at a specific time t, we can use the following Taylor expansion approach: V(r, t) =

,a

& % Va r − Ra +δRa · ∇r Va r − Ra . (10.6) Va r − Ra − δRa (t) ≈ ,a

Now the total Hamiltonian is Htot = Hel + Hph + Hel-ph , and we can write the electron– phonon contribution as Hel-ph =

,a

δRa · ∇ r Va r − Ra .

(10.7)

By expanding the displacement in phonon coordinates (see Chapter 4), we have δRa =

a Aaqα ˆ aqα eiq·R aqα + a†−qα ,

(10.8)

qα

where

( Aaqα =

h¯ , 2Ma Nωqα

(10.9)

where q is the wavevector, a labels the atomic species, α is the phonon branch index, and ˆ is the polarization vector. The phonon destruction and creation operators are represented by aqα and a†qα . They are not related to the atomic species label using the same letter a.

10.1 The rigid-ion model

223

In the language of second quantization, εnk c†nk cnk , Hel =

(10.10)

nk

Hph =

1 a†qα aqα + hω ¯ qα , 2 qα

(10.11)

and

Hel-ph =

n,k,n ,k

n k |Hel-ph |nkc†n k cnk

=

αq

n,k,n ,k ,q,α

Mnk→n k c†n k cnk (aqα + a†−qα ).

(10.12)

Equation (10.12) defines the electron–phonon matrix element M. Suppressing the band indices n and n by using an extended zone scheme so that k and k are not limited to the first Brillouin zone, Eq. (10.7) becomes a a Hel-ph = δRa ·∇r Va (r−Ra ) = Aaqa ˆqα · eiq·R ∇r Va (r − Ra ) (aqα +a†−qα ). ,a

a

qα

(10.13)

|k to evaluate the quantities in Eq. (10.12). Using the atomic form We now need k Hel-ph factor of the potential, 1 Va (q) = a

−iq·r

e

wN Va (r)dr =

e−iq·r Va (r)dr,

(10.14)

where a is the average volume per atom, w is the number of atoms per cell, is the crystal volume, and N is the number of cells in the crystal. To evaluate the matrix element we use the relations ∇r Va (r) =

i iq ·r q e Va (q ) wN

(10.15)

q

and ∇r Va (r − Ra ) =

i iq ·r a q e Va (q )e−iq ·R . wN

(10.16)

q

So, Eq. (10.13) becomes Hel-ph =

,a,α,q,q

Since

i a a a A ˆ · q eiq ·r ei(q−q )·R Va (q )(aqα + a†−qα ). wN qα qα

ei(q−q )·R = Nδ(q − q + G), a

(10.17)

(10.18)

10 Electron–phonon interactions

224

we obtain k |Hel-ph |k =

1 w

G

a · i(q + G)k |ei(q+G)·r |k. e−iG·τ α Va (q + G) ˆqα

(10.19)

Hence, the electron–phonon part of the Hamiltonian in the second quantization form is given by Mqa (k − k )c†k ck (aqα + a†−qα ), (10.20) Hel-ph = k,k ,q,α

and the electron–phonon matrix element is given by ( i h¯ Mqα (k − k ) = ˆqα · (q + G)eiG·τ α Va (q + G)k |ei(q+G)·r |k. (10.21) w 2Ma Nωqα a,G

10.2 Electron–phonon matrix elements for metals, insulators, and semiconductors

Let us consider an example appropriate for metals, which is to assume that k and |k are planewaves, as one expects in a pseudopotential approach. Hence, k |ei(q+G)·r |k = δk ,k+q+G

(10.22)

and i Mqα (k → k ) = w a,G

(

h¯ ˆqα · (q + G)eiG·τ α Va (q + G)δk ,k+q+G . 2Ma Nωqα

(10.23)

Therefore, if we know the pseudopotential form factor, we can, in principle, get Mqα . It is useful to distinguish the following two different processes. The first is the so-called “normal” process or N-process, where k is not far from k. This implies that k = k + q,

(10.24)

Mqα (k → k + q) = iAqα ˆqα · qV(q).

(10.25)

with G = 0, and assuming w = 1:

For these processes, there is no coupling if ˆ ⊥ q. Hence, transverse phonons are not effective in scattering electrons. The second process with G = 0 is called an Umklapp process or U-process (Fig. 10.5). The relative values of the matrix elements for these two processes are ˆα · qV(q) MN . = MU ˆα · (q + G)V(q + G)

(10.26)

225

10.2 Electron–phonon matrix elements for metals, insulators, and semiconductors

q

k = k + q + G k

Figure 10.5

Scattering of an electron in an Umklapp process. If G = 0, this is a normal process. ω LO

ω LO ω TO

TO LA TA k

Γ

Figure 10.6

X

Phonon dispersion relation for a polar diatomic crystal (schematic).

Usually V(q + G) < V(q) for a smooth pseudopotential, but Umklapp processes allow coupling to transverse phonon modes, and there are many of these processes (i.e. many G vectors) that contribute to the properties of metals. Another example is an ionic insulator or polar semiconductor where the energies of the longitudinal optical (LO) and transverse optical (TO) modes at long wavelengths are nondegenerate. This splitting of the phonon energies (Fig. 10.6) may be shown to be given by the ratio of the low- and high-frequency q = 0 dielectric constants 2 ωLO 2 ωTO

=

0 . ∞

(10.27)

For charged ions and two atoms per unit cell, small q terms dominate because of the longrange Coulomb interaction (∼ q12 in three dimensions). Here we use V1 (q) = −V2 (q) =

4π Ze2 ∞ q2 a

(10.28)

at small q, where Z is the charge of one of the ions and ∞ is the electronic dielectric constant of the polar material. The polarization vectors of the two atoms for the longitudinal mode have the form (1)

(2)

ˆLO = qˆ = −ˆLO ,

(10.29)

10 Electron–phonon interactions

226

Figure 10.7

–Z

+Z

–Z

+Z

M

M

M

M

Motion of ions in a diatomic ionic crystal (having charge Z and mass M) for long-wavelength LO phonon modes.

since the displacements are in opposite directions for nearest-neighbor atoms. (See Fig. 10.7.) Using Eq. (10.21), with w = 2 and M1 = M2 = M, i MLO (k → k + q) = 2

(

h¯ qˆ · qV1 (q) − 2MNωLO

(

h¯ qˆ · qV2 (q) . 2MNωLO

(10.30)

Using the relation 2 2 ωLO = ωTO + 2p ,

(10.31)

where p is the ionic plasma frequency and Eq. (10.27), we obtain MLO (k → k + q) = i

2π e2 hω ¯ LO q2

1 1 − ∞ 0

1/2 .

(10.32)

Here, 0 is the dielectric constant including both the electronic and phonon contributions. This is the electron–phonon matrix element Fr¨ohlich obtained by using an empirical approach, and this coupling is often referred to as the Fr¨ohlich interaction or Fr¨ohlich coupling.1 Our third example is the long-wavelength coupling of electrons to lattice vibrations in covalent semiconductors. This is called deformation potential coupling. This electron– phonon coupling is appropriate for excited electrons (or holes) in the conduction (valence) bands of semiconductors and insulators in the q ≈ 0 limit (Fig. 10.8) to describe how carriers are scattered to nearby states. Consider the scattering of carriers near a band extremum in the q → 0 limit. Within the framework of an effective Hamiltonian or effective mass theory (see Chapter 5), we express the conduction electron energy as E(k) = [E(k) − EC ] + EC (r),

(10.33)

where the bracketed term on the right-hand side is the band energy relative to the energy of the conduction band minimum EC , and the last term is the change in the conduction band minimum energy for a deformed crystal at location r. A periodic change of the lattice constant arising from a compressional wave will cause a periodic change in EC (r). The perturbation (from the effective mass or effective Hamiltonian point of view) will scatter the Bloch states, and this is associated with the coupling 1 H. Fr¨ohlich, “Electrons in lattice fields,” Adv. Phys. 3(1954), 325.

10.2 Electron–phonon matrix elements for metals, insulators, and semiconductors

227

E

Ec 0 k

Figure 10.8

Energy band structure for carriers near band extrema.

of the electrons to the lattice or phonons Hel-ph = EC (r) − EC = δEC (r).

(10.34)

This is then the perturbation potential that scatters an electron from one state to another. We may write δEC (r) in terms of the dilation (r) of the crystal volume : (r) ≡ Hence, δEC (r) =

δ(r) .

∂EC ∂EC δ = (r) = C1 (r), ∂ ∂

(10.35)

(10.36)

where C1 is defined as the deformation potential with units of energy.2 For example, consider a unit volume around an electron at r. Suppose the unit volume is strained (Fig. 10.9), then the original volume = xˆ · (ˆy × zˆ)

(10.37)

= xˆ · (ˆy × zˆ )

(10.38)

would change to

and

− . (10.39) We now need to express the dilation of the crystal near the position of an electron r in terms of the distortion of the crystal lattice sites. That is, =

(r) = f({δR (r)}, r),

(10.40)

2 J. Bardeen and W. Shockley, “Deformation potentials and mobilities in non-polar crystals,” Phys. Rev.

80(1950), 72.

10 Electron–phonon interactions

228

(a)

(b)

y

R艎 (r) z

z r

x

x r艎

Figure 10.9

(a) Unstrained unit volume. (b) Unit volume under strain. where the nearby lattice sites r (see Fig. 10.9(b)) when measured from the electron are denoted as (10.41) R (r) = r − r. Upon a uniform strain, the position of R (r) will change: R (r) → R (r) = R (r) + δR (r).

(10.42)

Under uniform or slowly varying dilation, the atoms will move away from their unstrained positions. The change in the lattice sites for the atoms near the electron will scale linearly with the distance from the electron and δR (r) → 0 as r (r) → r. We may write R (r) = R (r) +

μ

Rμ

(10.43)

∂δR(r)

. ∂Rμ r

(10.44)

Therefore, we can express the dilation as (r) =

− = −∇r · δR(r).

(10.45) →

The electron–phonon coupling comes from the dependence of ∇ r · δR(r) on the position of the electrons. Therefore, the perturbing Hamiltonian, using Eqs. (10.34) and (10.36), becomes (10.46) Hel-ph = −C1 ∇r · δR(r). We now express δR(r) in phonon coordinates: ( h¯ qˆ eiq·r (aq + a†−q ), δR(r) = 2ρω (q) q

(10.47)

10.3 Polarons

229

where the index counts longitudinal modes only and ρ is the mass density. From Eq. (10.45), we have ( h¯ |q|eiq·r (aq + a†−q ). (10.48) (r) = −i 2ρω (q) q

So, we have Hel-ph = −C1 ∇r · δR(r) = C1 k |k c†k ck k k

= −iC1

kq

(

h¯ |q| aq + a†−q c†k+q ck , 2ρω (q)

(10.49)

because k eiq·k |k = δk ,k+q for planewaves. Hence, we obtain ( Mq (k → k + q) = −iC1

h¯ |q|. 2ρω (q)

(10.50)

This is the deformation-potential coupling matrix element. We can estimate C1 for a free electron metal, where h¯ 2 EF = 2m Since

we have

3π 2 N

2/3 .

(10.51)

21 1 δEF =− , × EF δ 3

(10.52)

δEF 2 2 δ = − . =− EF 3 3

(10.53)

2 2 δE = − EF ⇒ |C1 | = EF ∼ 2 − 8 eV. 3 3

(10.54)

Hence, for metals,

For a semiconductor like silicon, if all the valence electrons are considered to be free electron-like, then EF is of order 16 eV, and C1 would be of order 10 eV.

10.3 Polarons We next explore an example of the coupling of an electron to LO phonons in a polar crystal. As shown in Fig. 10.10, when a dressed electron moves in an ionically bonded crystal, the

10 Electron–phonon interactions

230

(a)

(b)

e–

Figure 10.10

e–

An electron moving in an ionic crystal (schematic): (a) rigid lattice, and (b) in the presence of lattice distortion.

Coulomb attraction and repulsion of the positive and negative ions with the electron will cause distortions or strains of the lattice. The displacements of the lattice caused by the distortion can be expressed in terms of phonon excitations, and the combination of the electron and the “cloud of phonons” produced is viewed together as a new quasiparticle, a polaron. This use of the term polaron, which is an electron in a polar crystal coupled to LO phonons via the Fr¨ohlich interaction, is often extended to electrons coupled via lattice polarization in other situations and materials, such as polymers and metals. The electron–lattice polarization lowers the electron energy. It also increases the effective mass of the electron since the electron composing the polaron is now traveling with a lattice strain. In addition, there is a change in the electron mobility since the polaron experiences scattering effects that are different from those of a free quasielectron. Often polarons are sorted into two classes, large and small. If we define the size of a polaron p to be an effective radius of the phonon cloud or polarization area, then large polarons are those for which p > d (interatomic distance), and this indicates weak electron–phonon coupling. For small polarons, p d suggests strong coupling. Sometimes the coupling can be so strong that an electron becomes “self-trapped” in its polarization region. For large polarons and weak coupling, we are in a regime where we may use perturbation theory for the electron–phonon interaction. More sophisticated mathematical techniques are needed to solve for polaron properties for stronger coupling. If we consider the weak coupling case, the Hamiltonian for this problem is (with the last term on the right side considered to be small) H = Hel + Hph + Hel-ph = εk c†k ck + (a†q aq + 12 )hω Mq (k → k )c†k ck (aq + a†−q ). ¯ q+ k

(10.55)

k kq

q

For the present case, we consider that the electron only couples to LO phonons, hence M can be written (Eq. (10.32)) as Mq = i

hω ¯ LO |q|

h¯ 2mωLO

1/4

4π α

1/2 ,

(10.56)

10.3 Polarons

231

E

E

+ Phonon

k

k

Figure 10.11

Self-energy shift for a polaron.

where the dimensionless Fr¨ohlich coupling constant is defined as e2 α= h¯

1 1 − ∞ 0

'

m , 2hω ¯ LO

(10.57)

where m is the electron band mass. Using the definitions given in Eqs. (10.56) and (10.57), we arrive at our earlier expression for M given in Eq. (10.32). Assuming weak coupling α < 1 allows the use of perturbation theory to compute the self-energy shift of an electron, its effective mass m∗ to lowest order, and the number of phonons associated with an electron in a polaron. The self energy arising from electron–phonon interactions lowers the energy of an electron in a band, as shown in Fig. 10.11. The expression for the self energy at T = 0, using second-order perturbation theory, is (for an electron in state a) a = Ea =

|a|Hel-ph |b|2 b

Ea − Eb

,

(10.58)

where b are all possible intermediate states and the scattering processes are illustrated in Fig. 10.12. For the initial state a, we assume an electron is in a free electron state |k with no phonons present so that the total wavefunction can be represented by |k, 0 and the total energy of 2 2 state a is Ea = h¯2mk . When the electron is scattered to an intermediate state b, the electron is in state |k − q and one phonon is created. Hence, the total wavefunction is a†q |k − q, 0 and the energy is now Eb =

h¯ 2 (k − q)2 + hω ¯ q 2m

h¯ 2 k · q h¯ 2 q2 h¯ 2 k2 − + + hω = ¯ LO 2m m 2m

(10.59)

10 Electron–phonon interactions

232

a

b

c

k–q

k

q

k

Figure 10.12

Scattering diagrams for calculating the self energy of a polaron.

and Ea =

|Mq |2 =− Ea − Eb q hω ¯

LO

b

|Mq |2 +

h¯ 2 q2 2m

−

h¯ 2 k·q m

.

(10.60)

If we denote |Mq |2 = where

2 A = (hω ¯ LO )

A , q2

h¯ 2mωLO

1/2

(10.61) 4π α ,

(10.62)

and we convert the sum to an integral,

→

q

where μ =

k·q |k||q| ,

(2π )3

2π q2 dqdμ,

(10.63)

then

− Ek = A (2π )3

−1

⎛

1

qBZ

dμ 0

dq ⎝

⎞ 1 hω ¯ LO +

h¯ 2 q2 2m

−

h¯ 2 kqμ m

⎠.

(10.64)

Although this may be evaluated exactly, we can extract the main physical results by expanding for small k, letting qBZ → ∞, and evaluating the definite integrals to obtain E = −α hω ¯ LO −

hk ¯ 2 α + O(k4 ). 2m 6

(10.65)

The energy of the electron is E(k) =

h¯ 2 k2 + E(k). 2m

(10.66)

10.3 Polarons

233

Table 10.1 Experimental values of α for a variety of polar crystals.3 substance

α

substance

α

KCl KBr AgCl AgBr

4.0 3.5 2.0 1.7

ZnO PbS GaAs InSb

0.85 0.16 0.06 0.014

Combining Eqs. (10.65) and (10.66), we see that the ground-state energy is decreased by the factor α hω ¯ LO , and the k2 -dependent part of the energy, i.e. Ekin (k), has the form Ekin (k) =

1 h¯ 2 h¯ 2 k2 (1 − α)k2 = . 2m 6 2m∗

(10.67)

Hence, the effective mass m∗ of the polaron is m∗ =

α m . α ≈m 1+ (1 − 6 ) 6

(10.68)

As expected, the polaron mass is larger than the electron mass at the bottom of the conduction band. Another interesting calculation related to polarons is to estimate the average number of phonons coupled to an electron in a polaron at T = 0. The phonon number operator is given by ˆ ph = a†q aq , (10.69) N q

and its average value is Nˆ ph = ψ|

a†q aq |ψ,

(10.70)

q

where |ψ is the polaron wavefunction. For an electron wavevector k, |ψk = |k, 0 + |δψk ,

(10.71)

where |δψ is the change in the electron wavefunction |k, 0 due to the electron–phonon interaction. Using standard perturbation theory, to first order in M we have |δψk =

q

Mq a†q |k − q, 0 . Ek − (Ek−q + h¯ ωLO )

3 C. Kittel, Introduction to Solid State Physics, 8th ed. (New York, NY: Wiley, 2005).

(10.72)

10 Electron–phonon interactions

234

Following the same procedure as was done in Eqs. (10.60)–(10.64), the expression for the average number of phonons given by Eq. (10.70) in |ψk becomes Nˆ ph =

q

hω ¯ LO +

|Mq |2 h¯ 2 q2 2m

−

h¯ 2 kqμ m

2 .

(10.73)

Converting the above sum to an integral and expanding for small k, we obtain to lowest order in k 2 ∞ 2m dq α ˆ Nph = 2A (10.74) 2 = . 2 2 (2π ) 2 h¯ 2mωLO 0 2 + q h¯ So α is, in some sense, a measure of the number of phonons traveling with an electron in a polaron. Although the above three results, the self-energy shift, the renormalization of the effective mass, and the relationship between α and the average number of phonons “in a polaron” are calculated only for small α, they give considerable insight into the properties of this quasiparticle. As α becomes larger, this approach breaks down, but there are techniques for dealing with stronger coupling.4 Some representative values for α in different materials are given in Table 10.1.

4 R. P. Feynman, R. W. Hellwarth, C. K. Iddings, and P. M. Platzman, “Mobility of slow electrons in a polar

crystal,” Phys. Rev. 127(1962), 1004.

11

Dynamics of crystal electrons in a magnetic ﬁeld

In general, the motion of an electron is quantized in the presence of a magnetic field. We can learn a great deal about the electronic properties of a crystalline solid by examining the behavior of the material in a magnetic field. Various magnetic field-induced phenomena have been observed and have been used as detailed probes in characterizing materials. Moreover, they have led to the discovery of new phases of matter and have been exploited in various applications. Examples include striking phenomena such as the integer and fractional quantum Hall effects, Wigner electron crystallization, and giant magnetoresistance. Much of the behavior of electrons in a crystal with an applied magnetic field may be understood by assuming that the electrons are non-interacting fermionic quasiparticles. In this chapter, we shall consider the dynamics of crystal electrons in a magnetic field within this picture. That is, the electrons are non-interacting fermions but with masses and energywavevector dispersion relations that are modified by band structure, electron–electron, and electron–phonon interaction effects. We defer the discussion of the integer quantum Hall effect to Chapter 12 as part of the discussion on transport properties.

11.1 Free electrons in a uniform magnetic ﬁeld and Landau levels We first consider the simple case of free electrons in a uniform magnetic field B. Let B = Bˆz and allow the electrons to be confined to a large box of dimension L on each side (see Fig. 11.1). Classically, we know that the electron moves freely along the z-directon, and its motion in the x–y plane is confined to cyclotron orbits. Quantum mechanically, the energy eigenvalue ε and eigenfunction ψ of the electron are given by 2 q 1 ψ(r) = εψ(r), p − A(r) Hψ(r) = 2m c

(11.1)

where q = −|e| is the electron charge and A(r) is the vector potential, which, in the Landau gauge, is given by A(r) = (0, x, 0)B. In this gauge, A depends only on x. Since A is static and translationally invariant along the y- and z-directions, the energy and y- and z-components of the momentum of the electron are constants of motion. Equation (11.1) may be transformed to that of a one-dimensional harmonic oscillator. Substituting ψ(r) = 235

ei(kz z+ky y) φ(x) L

(11.2)

11 Dynamics of crystal electrons in a magnetic ﬁeld

236

B

L

Figure 11.1

Free electrons conﬁned in a box of dimension L in the presence of a uniform magnetic ﬁeld B. in Eq. (11.1) yields

2 hc h¯ 2 k2z p2x q2 B2 ¯ φ(x). x − φ(x) = ε − + k y 2m 2mc2 qB 2m

(11.3)

The above equation corresponds to the Schr¨odinger equation of a simple harmonic oscilla2 2 h¯ c tor located at position x0 = qB ky with spring constant κ = qmcB2 . The electron energies are given by h¯ 2 k2z 1 , hω ελ (kz ) = λ + ¯ c+ 2 2m

(11.4)

λ = 0, 1, 2, 3, . . . ,

(11.5)

with

' ωc = and

|e|B κ = , m mc

(11.6)

2π nz , L

(11.7)

kz =

where nz are integers. The expression for ωc has the same value as the classical cyclotron frequency. Thus, the electron behaves like a free particle parallel to B and performs cyclotron motion in the 2 2 plane perpendicular to B. The free electron energy dispersion relation ε(k) = h¯2mk is now changed into a series of parabolic curves as a function of kz labeled by the quantum number λ, as illustrated in Fig. 11.2. Each of the curves is called a Landau level.1 The Landau levels are highly degenerate because any value of ky yields the same set of solutions in Eq. (11.3). For given λ and kz , it can be shown that the number of degenerate states D is given by 2|e| 2BL2 D= BL2 = . (11.8) hc φ0 1 L. Landau, “Diamagnetism of metal,” Z. Phys. 64(1930), 629.

11.2 Crystal electrons in a static B-ﬁeld

237

(a)

(b) λ=2 E

E λ=1 λ=0 ħωc k

B≠0

B=0

Figure 11.2

kz

Energy vs. wavevector dispersion relation for a free electron in a magnetic ﬁeld B: (a) B = 0 and (b) B = 0. The Landau-level subbands labeled by λ are separated by h¯wc , where wc is the cyclotron frequency. hc Here φ0 ≡ |e| is the quantum of magnetic flux, which has a value of 4.136 × 10−7 G-cm2 . Thus, D may be viewed as two times the number of magnetic fluxoids penetrating the sample. In a field of 103 G or 0.1 T and sample size of L = 1 cm, D ∼ 1010 . The large degeneracy D here reflects the fact that an electron with a given energy and kz classically spirals about a line parallel to the z-axis, which can have arbitrary x and y coordinates. This is the reason D is proportional to the sample area L2 . For a two-dimensional electron gas (2DEG), kz does not come into consideration. The degeneracy of each Landau level is given by Eq. (11.8) and the total number of occupied Landau levels is given by

ν=

φ N 0 =n , D 2B

(11.9)

where N and n are the total number of electrons and the number of electrons per unit area, respectively.

11.2 Crystal electrons in a static B-ﬁeld Many phenomena of interest involve electrons with energies near the Fermi level EF . Under moderate magnetic fields in laboratory conditions, these electrons are in highly excited quantum states with the Landau-level index λF at the Fermi energy given by λF ∼

EF EF = . hω ¯ c h¯ |e|B mc

(11.10)

For an applied field B = 1 Tesla and EF =5 eV, λF ∼ 104 . Thus, most conventional experiments are not in the extreme quantum limit, where λF is a small integer, and a semiclassical

238

11 Dynamics of crystal electrons in a magnetic ﬁeld

treatment of the phenomena should be adequate. Exceptions are phenomena such as the integer and fractional quantum Hall effects, Wigner electron crystallization, etc., which occur at high B-field and low electron-density conditions.

11.2.1 Semiclassical analysis As discussed in Chapter 5, the dynamics of electrons in a crystal in a slowly varying applied field are basically determined by its band structure E(k), i.e. by the Hamiltonian H(p) = E(p),

(11.11)

with p = h¯ k. Given H(p), classically we obtain the Hamiltonian for B = 0 by using the substitution (here e is the charge of the electron, i.e. e = −|e|) P=p+

|e|A , c

(11.12)

where p = h¯i ∇ is the total momentum and P is defined using Eq. (11.12), which is known as the kinetic momentum of the electron, resulting in |e|A . H(P) = E p + c

(11.13)

We can formally derive the equation of motion for an electron in the semiclassical picture. The velocity is given by v = r˙ =

∂E(P) ∂H = , ∂p ∂P

(11.14)

which is only a function of the band structure. (Here, for simplicity, we shall neglect the anomalous velocity term due to a possible nonzero Berry curvature of the band structure. This term, as discussed in Chapter 5, can be important for some phenomena.) The time derivative of P is −|e| |e| ˙ v(P) × B (11.15) = P˙ = p˙ + A c c and is also a function of P only. Let us consider a uniform static field along the zˆ -direction B = (0, 0, B). Equation (11.15) in Cartesian coordinates is −|e| vy B, c |e| P˙ y = vx B, c P˙ z = 0. P˙ x =

(11.16)

Since dE = F · r = qc (v × B) · vdt, the electron cannot gain energy from a uniform B-field. The motion of the electron in P space is dictated by the band structure E(P) and constrained

11.3 Eﬀective mass and real-space orbits

239

Pz Plane of constant Pz e Py Surface of constant energy E Px

Figure 11.3

Schematic of the electron orbit in P-space for an electron in a magnetic ﬁeld B along the ˆz-direction. Py b υ l (t) a

Figure 11.4

Px

P-space path of an electron in a magnetic ﬁeld along the ˆz-direction; (t) is the length traveled in time t.

to move in a path formed by the intersection of a surface of constant energy and a plane of constant Pz , as shown in Fig. 11.3. Thus, the trajectory in P-space is dependent on the energy of the electron and the orientation of the applied B-field. The dynamics, i.e. how fast the electron is moving in P-space, is however determined by the strength of the magnetic field through Eq. (11.16).

11.3 Eﬀective mass and real-space orbits Since many experimental studies, such as cyclotron resonance measurements, are of the magneto-transport type, it is useful to introduce the concept of an effective dynamical mass. Consider an electron moving along a closed trajectory (called a closed orbit) in P-space in the presence of a B-field, as shown in Fig. 11.4. Let (t) be the distance from points a to b along the orbit in P-space. Then, using Eq. (11.16), |e|B 2 |e|B d 2 vx + vy2 = = P˙ x + P˙ 2y = v⊥ (Pz , E, ). dt c c

(11.17)

240

11 Dynamics of crystal electrons in a magnetic ﬁeld

Here v⊥ is the velocity that is perpendicular to B and to the tangent of the orbit. The electron goes around the orbit in a period T with 5 5 c d . (11.18) T = dt = |e|B v⊥ The frequency for going around the orbit ωc∗ = 2π T is the cyclotron frequency measured in experiment. Thus, we may define an effective mass m∗ through the identification ωc∗ = |e|B m∗ c , where m∗ (E, Pz ) =

1 2π

5

d . v⊥ (Pz , E, )

(11.19)

2 2

For a free electron with dispersion relation E(k) = h¯2mke , the orbit is circular and one obtains m∗ = me . In general, m∗ depends on the band structure, electron energy, and direction of the magnetic field. Moreover, if we go beyond an independent picture, manybody interactions will modify the quasiparticle energy dispersion, giving rise to corrections to the band structure effective mass.

11.3.1 A geometric expression for m* Let A(E, Pz ) be the area of the P-space orbital formed by E(P) = constant and Pz = constant. The effective mass m∗ of Eq. (11.19) in fact is related to A(E, Pz ). Consider δn(Px , Py ) = (δPx , δPz ) the vector normal to the constant energy surface due to a change in E (see Fig. 11.5). The change A in area of the orbit as E → E + δE is given by the area of a strip around the orbit, δA = |δn|d, because P˙ z = 0. Since δE = v⊥ δn, we have 5 5 δEd δA = δnd = . (11.20) v⊥ Comparing Eqs. (11.19) and (11.20), we have the relation m∗ (E, Pz ) =

1 ∂A(E, Pz ) . 2π ∂E

(11.21)

Py

δn E + δE E Px

Figure 11.5

Electron orbital change in P-space as the energy changes from E to E + δE.

11.4 Quantum oscillations: periodicity in 1/B

241

y

Py

x

Px

Reciprocal space

Figure 11.6

Real space

Electron in a magnetic ﬁeld along the ˆz-direction. (Left) Orbit in P-space and (right) orbit in real space. A measurement of the cyclotron frequencies thus contains geometric information on the electron orbits.

11.3.2 Real-space orbits Within the semiclassical approach, we can also easily obtain the motions of the carriers in real space. Integrating Eq. (11.16) with respect to time, we obtain y(t) − y0 =

−c Px (t) |e|B

x(t) − x0 =

c Py (t). |e|B

and (11.22)

The orbit in real space is centered about some position (x0 , y0 ), y(t) depends on Px (t), c . To obtain the real-space orbit, one and x(t) depends on Py (t) with a scaling factor of |e|B translates the P-space orbit to (x0 , y0 ), rotates it by 90◦ counterclockwise, and rescales it, as seen in Fig. 11.6. The shape of the real-space orbits is dictated by the P-space orbit. In general, it can be quite complex because of band structure (i.e. interaction of the electron with the lattice) effects. As expected, the scaling factor also tells us that the orbit in real space tightens as the strength of the magnetic field increases. We shall return to the concept of carrier orbits in metals when we discuss magnetoresistivity in the next chapter.

11.4 Quantum oscillations: periodicity in 1/B and the de Haas–van Alphen eﬀect in metals Many of the electronic properties of crystalline metals at low temperature T are oscillatory functions of 1/B, where B is an applied field. Examples include the oscillatory behaviors

242

11 Dynamics of crystal electrons in a magnetic ﬁeld

in the resistivity ρ(1/B), known as the Shubnikov–de Haas effect, and in the magnetic susceptibility χ (1/B), known as the de Haas–van Alphen effect.2 These effects, generally called quantum oscillations, have proven to be extraordinarily powerful probes of the electronic structure, particularly the Fermi surface properties, of metals. We shall focus on the physics of the de Haas–van Alphen effect in this section. The periodic behavior in 1/B in other effects has a similar physical origin. The presence of an external magnetic field causes the formation of a magnetization M(B) in metals. The magnetic susceptibility χ (B) = M(B)/B at low field can be measured using different means, such as the induced torque on a sample. The oscillations in the measured magnetization or magnetic susceptibility owe their origin to the quantization of the electron orbits. As a simple example, we consider the free electron gas. Again, taking B = Bˆz, a uniform magnetic field, the electron energy eigenvalues are given by Eq. (11.4). For a given kz , the states are quantized into Landau levels, each having a large degeneracy given by Eq. (11.8). The induced magnetic moment of the system is (in a unit volume) f m , (11.23) M=

where m is the moment of the th state and f is the Fermi–Dirac distribution function f (T) =

1 eβ(ε −μ)

+1

.

(11.24)

In a magnetic field B, as seen in Eq. (11.4), the energy of the states is B-dependent, i.e. ε (B), and m =

−∂ε . ∂B

(11.25)

Equation (11.25) follows from δH = 1−m · δB, where 2 m is the dipole moment operator, ∂ε (ξ ) ∂H and the Hellmann–Feynman theorem ∂ξ = ∂ξ . Equation (11.23) becomes M=

∂

∂ε = − − . ∂B ∂B β,μ eβ(ε −μ) + 1 1

(11.26)

Here is the usual grand potential in thermal physics for fermions, =−

& % 1 1 log Z = log 1 + e−β(ε −μ) , β β

(11.27)

where Z denotes the grand partition function. In order to evaluate (B, μ, β), the sum over the states in Eq. (11.27) may be converted to an integral using the density of states of the system g(ε, B). Owing to the formation of 2 W. J. de Haas and P. M. van Alphen, “ The dependence of the susceptibility of diamagnetic metals on the field,”

Proc. Koninklijke Akademie van Wetenschappen te Amsterdam 33(1930), 1106.

11.4 Quantum oscillations: periodicity in 1/B

(a)

(b)

Density of states g(ε)

Density of states g (ε, B)

243

ħωc

Energy ε

Figure 11.7

Energy ε

Schematic of the density of states of a free electron: (a) for B = 0 and (b) in the presence of a uniform magnetic ﬁeld with some broadening to mimic experiment.

Landau levels, the density of states of an electron gas in an applied uniform B-field no √ longer has the simple form g(ε) ∼ ε, but becomes one with structures that are separated by energy hω ¯ c . This is illustrated in Fig. 11.7. It is the structure of g(ε, B) that induces structure in the physical properties of a metal as a function of B. If we define an integrated density of state G(ε, B) =

ε

−∞

g(ε , B)dε ,

(11.28)

then the grand potential, which is

(B, β, μ) = −

1 β

dεg(ε, B) log 1 + e−β(ε−μ) ,

(11.29)

may be expressed as (using integration by parts twice) (B, β, μ) = −

∞ ε −∞

∂f(ε) dε, G(ε , B)dε − ∂ε −∞

(11.30)

where f(ε) is again the Fermi–Dirac distribution function. The evaluation of the grand potential is thereby reduced to the evaluation of g(ε, B) and its integral, i.e. a counting of electronic states. In evaluating g(ε, B) or G(ε, B) in three dimensions, we need to include the motion of the electron along z (i.e. the quantum number kz ) and the degeneracy of the Landau levels D as given in Eq. (11.8). The final expression needed for the integrand of

11 Dynamics of crystal electrons in a magnetic ﬁeld

244

Eq. (11.30) is

ε

−∞

2 1/2 G(ε , B)dε = aε5/2 + b(hω ¯ c) ε

2π nε π 5/2 ∞ cos − 4 h ω 1 V 2m 3/2 hω ¯ c ¯ c − 4 (−1)n , π 2 2 n5/2 h¯ 2 n=1

(11.31)

where a and b are constants and V is the volume. The three terms in Eq. (11.31) lead to (B, β, μ) = a + b + c .

(11.32)

The first term a is independent of B and does not contribute to M = − ∂ ∂B β,μ . The second term is of the form ∞ ∂f 2 1/2 dεε (11.33) b (B, β, μ) = −b(hω − ∼ −B2 . ¯ c) ∂ε −∞ This term leads to a contribution to the magnetic moment, which is of the form Mb (B) = −

N 2 μ B, 2EF B

(11.34)

where N is the number of electrons, EF is the Fermi energy, and μB the Bohr magneton in a metal is replaced with an effective Bohr magneton μ∗B =

eh¯ , 2m∗ c

(11.35)

which may differ from the Bohr magneton because the effective mass m∗ may be different from the electron mass in vacuum. This term gives a diamagnetic response due to the minus sign appearing in Eq. (11.34), and is called the Landau diamagnetism. If m∗ = me , then Eq. (11.34) in fact is numerically equal to −1/3 of the Pauli paramagnetic moment due to the spins of the electrons. The physical origin of Landau diamagnetism arises from the electrons orbiting to screen the applied B-field and has nothing to do with the spins of the electrons. The third term in Eq. (11.32) leads to another contribution to the magnetic moment c Mc (B, β, μ) = − ∂ ∂B β,μ . This may be evaluated to yield the dominant contributions n+1 sin π EF n − π ∞ 4 3π Nμ∗B EF 1/2 ˆ (−1) μ∗B B . Mc (B, β, μ) = B 2 EF β μ∗B B π 2n 1/2 n=1 n sinh μ∗ Bβ

(11.36)

B

The total magnetic moment M = Mb + Mc is hence a function of T and has an oscillatory component from Mc that is periodic in 1/B.

11.4 Quantum oscillations: periodicity in 1/B

245

Magnetic susceptibility χ

P

1/B1

1/B2 Inverse magnetic field 1/B

Figure 11.8

Schematic of the magnetic susceptibility χ of a free electron gas as a function of the inverse of the applied magnetic ﬁeld B. At high temperature, i.e. kB T hω ¯ c = 2μ∗B B, −

1

∼e 2 sinh π μk∗BBTn

π 2 kB Tn μ∗ BB

.

(11.37)

B

Thus, the contribution of Mc to M is exponentially small. The oscillatory component of M can only be observed at low temperature in the regime of kB T ≤ 2μ∗B B. In this limit, the terms in the sum in Eq. (11.36) are on the order of 1 and k T E 1/2 Mc B F ∼ 1, Mb μ∗B B μ∗B B

(11.38)

showing that the oscillatory component can be quite large at low temperature. Taking the largest term n = 1 in Eq. (11.36) and defining K = πμE∗F , we have B

K π 1 − , Mc (B) ∼ √ sin B 4 B

(11.39)

which is oscillatory as a function of 1/B. In a de Haas–van Alphen experiment, χ = M/B 2μ∗ will also be an oscillatory function in 1/B with period P = B11 − B12 = EFB , as shown in Fig. 11.8. h2 k 2

For the free electron case, EF = ¯2m∗F . Thus, we may rewrite P in terms of the Fermi surface cross-section area, AFS = π k2F , and obtain P=

2π e/hc ¯ AFS

=

4π 2 , φ0 AFS

(11.40)

where φ0 is the flux quantum. Equation (11.40) can be shown (see below) to hold for any arbitrary Fermi surface if one replaces AFS with the extremal cross-section areas of the Fermi surface.

11 Dynamics of crystal electrons in a magnetic ﬁeld

246

y

Density of states g(ε, B)

∆ε = ħωc

x 1/2

3/2

5/2

7/2

Energy ε in units of ħωc

Figure 11.9

(Left) Density of states of a two-dimensional electron gas in a perpendicular magnetic ﬁeld. (Right) Real-space orbit of an electron in a Landau level. This oscillatory phenomenon has its physical origin from (1) the quantization of the electron orbits in a magnetic field, (2) the fact that adding a quantum of flux inside a fixed orbit does not change any physical measurable properties, and (3) the factor −∂f/∂ε in Eq. (11.30), only orbits of energy within kB T of the Fermi level contribute to the grand potential and hence M. Under a change of magnetic field, the quantum states within kB T of EF will change, but will map into a set that is identical to the original set after a quantum of magnetic flux is either added or subtracted from the enclosure of the orbit. This can be seen more clearly in two dimensions. In a uniform magnetic field, the density of states of a two-dimensional electron system is a series of delta functions and the electrons undergo a closed orbit motion in real space, as illustrated in Fig. 11.9. For quantum mechanical systems, if {E0 , ϕ0 } are solutions to the Hamiltonian 2 P − ec A0 + V(r), (11.41) H0 = 2m then, if B0 → B0 + δB (with the corresponding change A = A0 + δA), it can be shown that ie r

ϕ(r) = e h¯ c

δA·d

ϕ0 (r)

(11.42)

1 e 22 P− c A satisfies the Schr¨odinger equation with the new H = + V(r), and is a solution of 2m the same energy if 5 e δA · d = 2π n (n = integer), (11.43) hc ¯ owing to the requirement of single-valueness for φ as it goes around the real-space orbit. The line integral of Eq. (11.43) may be converted to a surface integral resulting in the condition that δBAorbit = nφ0 ,

(11.44)

where Aorbit is the area of the real-space orbit. This result implies that the states near EF and the properties of the system determined by these states will duplicate themselves if B is

247

Figure 11.10

11.4 Quantum oscillations: periodicity in 1/B

Diﬀerent orbits and therefore cross-sectional areas of the orbits for electrons on the Fermi surface for a given orientation of the applied B-ﬁeld.

changed by an amount that adds or removes a flux quantum in the orbit. This is the general principle of gauging away the effect of an integer quantum of flux in a loop system. Since the states of importance in the de Haas–van Alphen effect are those at the Fermi energy, this gives the condition for the periodicity in 1/B as (using Eq. (11.44)) P=

1 δB φ0 1 − = 2 = 2 . B − δB B B B Aorbit

(11.45)

For the states at the Fermi level, the real-space orbital area is related to the P-space orbital 2 2 area by h¯ 2 AFS = ( e cB2 )Aorbit , giving rise to P=

B2

φ0 h2 c 2 1 A e2 B2 FS

=

4π 2 , φ0 AFS

(11.46)

which is the same as Eq. (11.40). In real materials, the Fermi surface may be quite complex. For a given orientation of B, each cross-sectional area will contribute a frequency of oscillations, as seen in Fig. 11.10. However, only the extremal cross sections will constructively add to provide experimental 2μ∗ 1 signals. Since P = B1 − B+B = EFB , for most metals P is very small, on the order of 10−9 /G. Thus, one needs a very high field, typically B ∼ 10T, to perform de Haas–van Alphen measurements. The sinh term in Eq. (11.36) provides further information since it is temperature dependent. Even at low temperature, usually only the n = 1 term is observable. By varying 2 the temperature at a fixed magnetic field, we may measure the combination πμ∗kBBT . Such B measurements yield μ∗B and hence information on m∗ . A careful de Haas–van Alphen experiment will provide detailed information on the cross-sectional area of the Fermi surface of a metal and on the effective mass of the carriers. Moreover, since (B, μ, β) is oscillatory in 1/B, we expect other physical quantities derived from to show similar oscillatory behavior. The conductivity of a metal also exhibits oscillations as a function of 1/B. This is called the Shubnikov–de Haas effect.

12

Fundamentals of transport phenomena in solids

The electronic and thermal transport behaviors are among the most important properties of a material, being fundamental to their understanding and characterization and central in their applications. We have discussed topics such as electrical conductivity in previous chapters. In this chapter, we develop the fundamentals of transport phenomena. The discussions focus on the important physical processes and make use of mostly kinetic theory and semiclassical formalisms.1 Topics to be presented include elementary treatments of magnetoresistance, the conventional Hall and integer quantum Hall effects, and various transport processes and phenomena in materials employing the Boltzmann equation formalism.

12.1 Elementary treatment of magnetoresistance and the Hall eﬀect An applied magnetic field in general changes the electrical conduction of a metal or semiconductor. This phenomenon of magnetoresistance has led to fundamental discoveries (such as the integer and fractional quantum Hall effects), and a number of important technologies such as magnetic recording devices. The experimental setup for measuring magnetoresistance usually takes the arrangement shown schematically in Fig. 12.1. In this standard geometry, the sample takes on the form of a bar (often called a Hall bar) with current drawn along its length (the xˆ -direction) and a magnetic field applied transverse to its flat face (the zˆ-direction). The interesting experiments are those carried out at low temperature T and high magnetic field B on a pure sample. These conditions correspond to large cyclotron frequency ωc and long collision time τ . That is, |e|B τ 1. (12.1) ωc τ = mc The carriers go through many orbits before a collision; the details of the collision processes, as discussed below, are suppressed and the details of the electronic structure, in particular the Fermi surface, are exhibited. 1 Some pioneering papers on the quantum theory of transport in metals include: W. Kohn and J. M. Luttinger,

“Quantum theory of electrical transport phenomena,” Phys. Rev. 108(1957), 590; J. M. Luttinger and W. Kohn, “Quantum theory of electrical transport phenomena. II,” Phys. Rev. 109(1958), 1892; and I. M. Lifshitz, “Quantum theory of the electrical conductivity of metals in a magnetic field,” Soviet Phys. JETP 5(1957), 1227.

248

249

12.1 Elementary treatment of magnetoresistance and the Hall eﬀect

B = Bz z εx , jx

y x

Vx

Figure 12.1

Schematic of a standard experimental setup for a magnetoresistance measurement. This is known as a Hall bar geometry.

General experimental findings for the magnetoresistance with a transverse B field include: I. Weak fields. The fractional change in resistance at low field tends to increase as B2 . That is, R(B) − R(0)

R = ∼ (ωc τ )2 ∼ B2 , R R(0)

(12.2)

where R (sometimes denoted as Rxx ) is given by Vx /Ix and Ix is the total current through the Hall bar. (See Fig. 12.1.) II. Strong fields. (a) Saturation. R(B) goes to a constant as B increases for all orientations of B with respect to the crystalline directions. This is found for metals with a closed Fermi surface, e.g. In, Al, Na, Li, etc. (b) No saturation. R(B) keeps increasing as B increases. This occurs in crystals with equal numbers of electron and hole carriers, e.g. Bi, Sb, W, Mo, etc. (c) Selected saturation directions. R(B) is unsaturated for B oriented along some crystalline directions, but not for all orientations. This occurs in some metals, e.g. Cu, Ag, Au, Mg, Zn, etc. The magnetoresistance has been used successfully to study the topology of the Fermi surface of both simple and complex metals. The above-mentioned differences in the observed behavior of the magnetoresistance may be understood from elementary considerations of charge particles moving in electric and magnetic fields within the formalism of crystalline electron dynamics, which we developed in Chapter 5. The basic physics is that the Lorentz force, e F = v × B, c

(12.3)

deflects the carriers with charge e from their trajectory, and thus makes it less effective for the electric field to impart momentum to the charge carriers. Classically, for a pure sample with no collisions, the particle would drift in the direction perpendicular to the applied electric E and magnetic B fields with a drift velocity vd = cBE .

12 Fundamentals of transport phenomena in solids

250

12.1.1 One-carrier-type model We first consider the case of a metal with a single type of carrier that is characterized by an isotropic effective mass m∗ and a constant collision (or relaxation) time τ . This model corresponds to an idealized simple metal with a spherical Fermi surface and weak scattering centers. The equation of motion for the carrier is given by 1 1 (12.4) m∗ v˙ + v = e E + v × B , τ c where E and B are uniform, static, and applied electric and magnetic fields, respectively. At steady state, v˙ = 0, Eq. (12.4) reduces to 1 eτ (12.5) v= ∗ E + v×B . m c Let B = Bˆz, and defining μ = eτ/m∗ and ξ = eBτ/m∗ c, the components of Eq. (12.5) are vz = μEz , μ vx = 1 + ξ2 μ vy = 1 + ξ2

1 2 Ex + ξ Ey ,

(12.6)

1 2 Ey − ξ Ex .

Here we take e as the carrier charge. The quantity μ is the mobility of the system in the absence of the B-field. Thus, the B-field reduces the effective mobility of the carriers along directions that are perpendicular to the direction of the B-field. ↔ The conductivity tensor σ is given through the relation ↔

j = σ E,

(12.7)

where j is the current density. Since j = nev, where n is the carrier density, we obtain in this elementary treatment for the conductivity tensor ⎛ 1 neμ ⎝ σ = −ξ 1 + ξ2 0

↔

ξ 1 0

⎞ 0 0 ⎠, 1 + ξ2

(12.8)

and the resistivity tensor ⎛ 1 1 ⎝ ρ= ξ neμ 0

↔

↔

by taking the inverse of σ .

−ξ 1 0

⎞ 0 0⎠ , 1

(12.9)

12.1 Elementary treatment of magnetoresistance and the Hall eﬀect

251

In the standard experimental geometry shown in Fig. 12.1, jy = jz = 0. The measured quantities satisfy the relation ⎛ ⎛ ⎞ 1 Ex 1 ⎝ξ ⎝Ey ⎠ = neμ Ez 0

−ξ 1 0

⎞⎛ ⎞ 0 jx 0⎠ ⎝ 0 ⎠ , 1

(12.10)

0

which yields Ex =

1 jx . neμ

(12.11) ∗

1 = nem2 τ is indepenEq. (12.11) shows that the longitudinal resistance ρxx = Ex /jx = neμ dent of B. The absence of magnetoresistance in this model is the result of an electric field generated along the y-direction in Fig. 12.1, called the Hall field Ey , which just balances the Lorentz force from the magnetic field.2 From Eqs. (12.10) and (12.11), the Hall field is

Ey =

ξ jx = ξ E x . neμ

(12.12)

This result arises from having one relaxation time τ and one kind of carrier. In this case, we can determine the density and the charge of the carriers by measuring the transverse or Hall resistivity ρyx . From Eq. (12.12), eB m∗ c τ Ey ξ B = = . (12.13) = ρyx = jx neμ nec eτ ne m∗ The material parameters m∗ and τ do not enter the Hall resistivity, leaving a simple relation that yields the density and sign of the charge of the carriers within this simple model. In general, there will be magnetic field dependence on ρxx , and the Hall resistivity ρyx may be more complex than Eq. (12.13). The complexities arise because there are, in general, many carrier types in a metal and the Hall field Ey may not balance the Lorentz force on each carrier, resulting in a magnetoresistance in ρxx .

12.1.2 Two-carrier-type model The simplest model to illustrate the physics of magnetoresistance in ρxx is to assume two carrier types in the metal. In this case, at steady state, the velocity of each of the carrier types, i = 1 or 2, is given by ei τi ei τi E + ∗ vi × B. (12.14) vi = ∗ mi mi c 2 This was discovered by E. H. Hall in 1879, 18 years before the discovery of the electron: E. H. Hall, “On a

new action of the magnet on electric currents,” Amer. J. Math. 2(1879), 287.

12 Fundamentals of transport phenomena in solids

252

The current density j is ↔

↔

j = n1 e1 v1 + n2 e2 v2 = (σ 1 + σ 2 ) · E.

(12.15) ↔

In the standard geometry with B = Bˆz, we may drop the z-components of σ , since, as seen in Eq. (12.10), it is not relevant to the analysis. Equation (12.15) yields ↔ ↔ ↔ σxx σxy , (12.16) σ = σ1 + σ2 = −σxy σyy with (i) σxx

=

(i) σyy

(i)

σ0 ni e2 τi i = = ∗ 2 1 + βi2 B2 mi 1 + ξi

(12.17)

and (i) σxy = (i)

Here we have used the notation σ0 given by

=

σ0(i) βi B 1 + βi2 B2 ni e2i τi m∗i

1 ρ= 2 σxx σyy + σxy

↔

.

(12.18)

and βi =

σyy σxy

eτi m∗i c .

The resistivity tensor is

−σxy . σxx

(12.19)

The explicit expression for ρxx is given by (using σxx = σyy ) (1)

(2)

σyy + σyy ρxx = . (1) (2) 2 (1) (2) 2 σxx + σxx + σxy + σxy

(12.20)

We may evaluate the change in ρxx due to the magnetic field and obtain σ0(1) σ0(2) (β1 − β2 )2 B2 ρxx ρxx (B) − ρxx (0) = = . ρxx ρxx (0) (1) (2) 2 (1) (2) 2 σ0 + σ0 + B2 β2 σ0 + β1 σ0

(12.21)

Equation (12.21) exhibits the experimental behavior observed in many metals. At weak field, the first term in the denominator in Eq. (12.21) dominates. Hence, we have ρxx (B)/ρxx (0) ∼ B2 and the change in resistivity is positive. At high field, the B2 dependence of the numerator and that of the denominator cancel each other and ρxx (B)/ρxx (0) saturates to a constant value. The phenomenon of saturation may be understood as follows. At high field, as B → ∞, Eq. (12.17) gives σxx → 0. This does not mean that jx is zero, because jx = σxx Ex + σxy Ey .

(12.22)

12.1 Elementary treatment of magnetoresistance and the Hall eﬀect

253

εy

y

εx , jx

x

B = Bz

Figure 12.2

z

Schematic of current density jx , and electric and magnetic ﬁeld components in a Hall experiment. In the large B-field limit, although σxx vanishes, the existence of an electric field along the x-direction Ex induces a Hall field Ey along the y-direction, to annul any Hall current that may be generated along the y-direction. In turn, Ey generates a Hall current in the xσ Ex . Thus, the current along the wire, direction. The fact that jy = 0 leads to Ey = − σyx yy as given in Eq. (12.22), in the large B limit, is due to the Hall current generated by Ey , and the current is proportional to Ex but independent of B, leading to the phenomenon of saturation. In the high B-field limit, the Hall conductivity σxy simplifies in the two-carrier-type (1) (2) model. Since σxy = σxy + σxy and 1 + ξi2 → ξi2 as B → ∞, we have from Eq. (12.18) (i) → σxy

ni e2 τi2 ξi m∗i ξi2

=

ni ei c B

(12.23)

and σxy =

(n1 e1 + n2 e2 )c , B

(12.24)

independent of m∗i and τi . For a compensated metal in which there are equal numbers of electrons and holes, we have n1 = n2 and e1 = −e2 . Examples of this kind of system are the semimetals Bi and Sb. For such metals, Eq. (12.24) gives σxy = 0. This implies that there is no Hall field Ey to contribute a current to jx in Eq. (12.22) and from Eq. (12.20), ρxx (B) =

2 σxx

σyy ∼ B2 . 2 + σxy

(12.25)

Physically, because one cannot establish a Hall field, it becomes increasingly hard for the field Ex to impart momentum to the carriers. The magnetoresistance does not saturate if there are equal numbers of holes and electrons, explaining the experimental observation stated in II(b) of Section 12.1. In fact, we can get the condition for unsaturated magnetoresistance directly from Eq. (12.21). Notice that in the denominator of Eq. (12.21), β2 σ01 + β1 σ02 =

τ1 τ2 e1 e2 (n1 e1 + n2 e2 ) . m1 m2 c

When we have (n1 e1 + n2 e2 ) = 0, there will be no saturation of magnetoresistance in the high B-field. Such a condition can be achieved in the case where n1 = n2 and e1 = −e2 .

12 Fundamentals of transport phenomena in solids

254

12.1.3 Inﬂuence of open orbits in high ﬁeld What remains to be explained is behavior II(c), i.e. the phenomenon of saturation at high field only in selected crystalline directions. This kind of behavior occurs in metals with open orbits for states near the Fermi surface. That is, the intersection of the surface of constant energy and the plane of constant Pz does not form a loop, but joins continuously to the next Brillouin zone indefinitely in the repeated zone scheme. Let us consider a metal with an open orbit along the Px -direction. Such an orbit can create a current in real space along the y-direction, as illustrated in Fig. 12.3. This arises from Eq. (11.16) in the standard geometry for B = Bˆz, i.e. eB˙x c

(12.26)

eB˙y . c

(12.27)

P˙ y = − and P˙ x =

If an electric field is applied along the y-direction, there is an imbalance in the occupation of orbits in the upper plane versus the lower plane in Fig. 12.3(a), leading to a net current along the y-direction in Fig. 12.3(b). Thus, for open orbits along Px , there will be an extra contribution to σyy . From the discussion in Chapter 11, we can show that in the presence of a uniform electric field E in addition to the B-field, the projection of the real-space orbit in a plane perpendicular to B is r⊥ (t) − r⊥ (0) =

(a)

−hc ¯ ˆ B × [k(t) − k(0)] + vd t, eB

(b)

Py

y

x

Px

Reciprocal space open orbit

Figure 12.3

(12.28)

Real space open orbit

Sketch of an open orbit in reciprocal space (a) and the corresponding orbit in real space (b). The applied magnetic ﬁeld is along the ˆz-direction.

12.1 Elementary treatment of magnetoresistance and the Hall eﬀect

255

ˆ is the drift term and k(t) is the orbital motion given by where vd = c EB (Eˆ × B) ¯ e 1 ∂ E(k) × B, (12.29) c h¯ ∂k 2 eE aB 1 E e ¯ with E(k) = E(k) − hk in general is negligibly ¯ · vd . But hk ¯ · vd < h¯ aB c B = aB h¯ ωc ¯ small in laboratory conditions and we can just take E(k) as equal to E(k). (Here aB is the Bohr radius.) In calculating the current density j = nev, the velocity v should be the drift velocity of the electron acquired after collision averaged over all states, i.e. : 9 : 9 hc k(0) − k(−τ ) r⊥ (0) − r⊥ (−τ ) ¯ ˆ = − B× + τ vd . (12.30) v = τ eB τ h¯ k˙ =

For closed orbits, k = k(0) − k(−τ ) is bounded in the high field limit of ωc τ 1. The dominant term in Eq. (12.30) is vd . This is not the case for open orbits, however. 0 from the open In the high B-field limit, we can then associate an extra conductivity σyy orbits along Px , which is independent of B in the form of 0 σyy = sneμ,

(12.31)

where s is a constant. The expression in Eq. (12.31) is independent of B because the first term on the right-hand side of Eq. (12.30) is independent of B since k(t) ∼ B. The ↔ conductivity tensor σ in the high field limit takes on the form

ξ −2 σ = neμ −ξ −1

↔

ξ −1 , s

(12.32)

including the contribution from the open orbit along Px . For σyy , we have dropped the term ξ −2 in comparison to s, since ξ −2 vanishes as B−2 . In the standard geometry of drawing a current along the x-direction, jy = 0 dictates that Ey is now scaled like B1 Ex and becomes vanishingly small at large B. The resistivity along the x-direction takes on the form, for ξ 1, s ξ2 ∼ B2, ρxx (B) = neμ s + 1

(12.33)

which shows no saturation. However, if the open orbit is along Py , then, for ξ 1,

s σ = neμ −ξ −1

↔

ξ −1 ξ −2

(12.34)

and ρxx

1 1 = . neμ 1 + s

(12.35)

12 Fundamentals of transport phenomena in solids

256

Therefore, for this orientation of the open orbit, the resistance saturates at high field. For an open orbit in a general direction and ξ 1, we have, with s1 and s2 constants,

s1 σ = neμ −ξ −1

↔

ξ −1 s2

(12.36)

and ρxx =

s2 1 , neμ s1 s2 + ξ −2

which shows saturation. The analysis here shows that, in general, the magnetoresistance saturates except when the open orbit carries current almost precisely parallel to the y-direction (i.e. the open orbit in P-space is parallel to x). The existence of open orbits is the key to understanding the behavior of selected saturation directions described above as behavior II(c). Good examples of materials that exhibit this kind of behavior are the noble metals, such as Cu and Ag. Figure 12.4 depicts the Fermi surface of copper. There are many kinds of orbits that can be formed by intersection of the Fermi surface with a plane perpendicular to the direction of the magnetic field. Since the Fermi surface is connected to the neighboring Brillouin zones, open orbits are possible for the appropriate orientation of the B-field. Hence, the magnetoresistance shows non-saturation along selected orientations of the B-field with respect to the crystal axes.

b

a

Figure 12.4

Fermi surface of copper in the repeat zone scheme, showing both closed and open orbits.

12.2 The integer quantum Hall eﬀect

257

12.2 The integer quantum Hall eﬀect The integer quantum Hall effect (IQHE) was an unexpected discovery made by K. von Klitzing, G. Dorda, and M. Pepper in 1980,3 and von Klitzing was awarded the 1985 Nobel Prize in Physics for the discovery. The IQHE is the manifestation of a new phase of matter of a two-dimensional electron gas (2DEG) system in the quantum limit of low carrier density, low temperature, and high magnetic field. It is an early example of the so-called topological insulators.4 The IQHE has been used to make the most precise measurement of 2 the fine structure constant α = he¯ c and to set a new standard for resistance. In this section, we describe the phenomenon, the experimental setup and results, and the physical origin of the effect.

12.2.1 The phenomenon The IQHE occurs in a 2DEG. As was discussed in the previous section, the magnetoconductivity in the standard geometry is given by (from Eq. (12.8)) ne2 τ ↔ 1 −ωc τ (12.37) σ = 1 ωc τ m 1 + (ωc τ )2 and ↔

ρ=

ρ0 B nec

B − nec , ρ0

(12.38)

with ρ0 = nem2 τ . (For notation simplicity, we shall use m to denote the carrier effective mass in this section.) In the quantum limit, in which the experimental conditions are such that only a few Landau levels are occupied, it is found that the measured quantities, as a function of Bn over large ranges, unlike those given by Eqs. (12.37) and (12.38), take the form 3 4 2 ↔ 0 − νeh σ = νe2 (12.39) 0 h and

3 ↔

ρ=

0

− νeh2

h νe2

0

4 ,

(12.40)

where ν is a small integer corresponding to the number of occupied Landau levels, as shown in Fig. 12.5. 3 K. von Klitzing, G. Dorda, and M. Pepper, “New method for high-accuracy determination of the fine-structure

constant based on quantized Hall resistance,” Phys. Rev. Lett. 45(1980), 494. 4 See, for example, the review by M. Z. Hasan and C. L. Kane, “Colloquium: Topological insulators,” Rev. Mod.

Phys. 82(2010), 3045.

12 Fundamentals of transport phenomena in solids

258

1/ρxy in units of e2 /h

4 3 ρxx

2 1

0

1

2

3

4

Landau level filling factor ν

Figure 12.5

A sketch of the Hall conductivity and the longitudinal resistivity of a 2DEG with impurities, illustrating the IQHE at low Landau-level ﬁlling factor ν. This is an extraordinary result in that the Hall plateaus in Fig. 12.5 are found to be 2 quantized to eh , the fundamental unit of conductance, to better than one part in 109 . Since c, the speed of light, is an exactly defined quantity, the IQHE plateau value provides one of 2 the most accurate measurements of the fine structure constant he¯ c . It also gives a new and convenient standard for resistance. Moreover, the diagonal resistance in the IQHE regime is exactly zero, except in narrow transition regions between plateaus in σxy . Thus, there is dissipationless current flow along the Hall bar, i.e. no voltage drop in the Hall plateau regions in Fig. 12.5.

12.2.2 Experimental setup The typical setup for an IQHE experiment is schematically shown in Fig. 12.6. A 2DEG is created at a metal-oxide-semiconductor (MOS) interface or at a semiconductor heterojunction. Contacts are made in the standard Hall bar geometry (of length L and width W) to measure the current flow and voltage drop along and across the Hall bar. The resistance along the Hall bar is E ×L VL L = = ρxx · , (12.41) RL = I j×W W and the Hall resistance is RH =

Ey W Ey VH = ρyx . = = I jx W jx

(12.42)

In two-dimensional (2D) systems, the dimensions of resistance are the same as those of resistivity. Furthermore, for the Hall resistance ρyx (or ρH ), the geometric size factors drop out of Eq. (12.42), making precise geometry-independent measurements possible.

12.2 The integer quantum Hall eﬀect

259

VL L Source

VH

2DEG

y

B = Bz^

Drain

W

x z

Figure 12.6

Sketch of the experimental setup for an IQHE study.

(a)

(b)

E Oxide

Metal

Semiconductor cb

SiO2

0

EF

VG

p-Si

vb

z

0

(d)

(c)

2nd subband

E

V(z) 2(z)

E2

1st subband

1(z)

z

Figure 12.7

E1

k

Schematic of the sample used in the IQHE study: (a) a MOS junction, (b) band structure of a p-doped semiconductor near the oxide-semiconductor interface, (c) potential V(z) and subband states at the oxide-semiconductor interface, (d) subband dispersions as a function of the wavevector parallel to the oxide-semiconductor interface (k ) in absence of a magnetic ﬁeld.

The original experiment by von Klitzing, Dorda, and Pepper was performed on an MOS device (see Fig. 12.7(a)). By applying a gate voltage across the interface, a layer of electrons is accumulated at the interface on the p-doped silicon side by bending the conduction band of Si below the Fermi level EF . These electrons see a confining potential V(z) along the z-direction perpendicular to the interface forming discrete subband states (see Fig. 12.7(c)), which are freely propagating in the x−y plane. Each of the subbands gives rise to a 2D flat density of states. At sufficiently low temperature T and electron density n, only the lowest subband is occupied, making the system a 2DEG. The conditions

12 Fundamentals of transport phenomena in solids

260

Density of states D(ε, B)

B = Bz^

y

D(ε, B ≠ 0) eB DL = hc

D(ε, B = 0) 5/2 1/2 3/2 Energy ε in units of ħωc

x

Figure 12.8

∆ε = ħωc

Density of states of a 2DEG in a perpendicular magnetic ﬁeld.

for 2DEG formation correspond to kB T < E2 − E1 and EF < E2 − E1 , where Ei is the energy of the bottom of the ith subband.

12.2.3 Two-dimensional magnetoresistance in the quantum limit For a 2DEG under a uniform perpendicular magnetic field, its density of states per unit area D(ε) transforms to a series of delta functions separated by hω ¯ c due to the formation of Landau levels, as discussed in Chapter 11 (see Fig. 12.8). Each of the delta functions has a degeneracy per unit area of DL = |e|B hc (we neglect spin for now). The number of Landau levels occupied at density n at low T(kB T h¯ ωc ) is n hc ν= . =n DL |e|B

(12.43)

As the electron density or the magnetic field is varied, the Fermi level will move and ν will change. From the discussion so far, we have two possibilities. (a) The Fermi level is in one of the Landau levels. This corresponds to an arbitrary density. ↔ In this case, ρ is given by Eq. (12.38), and both ρxx and ρxy behave as expected for a traditional metal. (b) The Fermi level is in between Landau levels, i.e. ν is an integer. Then there is a gap in the excitation spectrum, which means that there is no scattering that can dissipate B = νeh2 , resulting energy. Therefore, τ now goes to infinity, ρxx → 0, and ρxy = − nec ↔

↔

in the expressions for ρ and σ in Eqs. (12.40) and (12.39), respectively.

The above naive analysis, however, has serious problems in explaining the experimental data. (i) Why are the plateaus in ρxy so extended as a function of Bn ? The scenario in case (b) above should occur only at singular points on the Bn -axis. (ii) Why is the quantization so perfect and not dependent on details of sample quality and geometry? The answer to (i) involves the effects of impurities and imperfections in the 2DEG, and the answer to (ii) involves knowing that the electron charge is quantized and may be understood in terms of a gauge argument.

12.2 The integer quantum Hall eﬀect

261

12.2.4 Eﬀects of random impurities and defects Owing to various defects in or nearby the 2DEG, the potential seen by an electron has a randomly fluctuating component, as illustrated in Fig. 12.9. The random potential fluctuations lead to a broadening of the Landau-level density of states as well as the existence of localized states. Classically, a charged particle in a magnetic field can only move along paths defined by iso-energy contours on the energy surface. For a large-sized sample, virtually all states are trapped by local potential fluctuations that are either above or below the mean value. Only states with energy virtually exactly at the mean potential can propagate across the sample. Thus, as shown schematically in Fig. 12.9, only states at the original Landau-level energies are extended, and all other states with energy between Landau levels are localized states. Since localized states do not carry current as the carrier density is varied, the conductivity σxy of the system does not change as long as EF remains in the mobility gap (defined as the energy region over which the states are localized) between the Landau levels. These constant σxy regimes correspond to the plateaus in the ρxy vs. Bn curve. When EF moves through the extended state portion of the density of states, ρxy makes a transition from one plateau to the next. What remains to be explained is why σxy is exactly an integer times e2 /h.

(a)

V(r) –

E>V

y –

E=V

x –

E